RHEOLOGY SERIES Advisory Editor: K. Walters, Department of Mathematics, University College of Wales, Aberystwyth, U.K.
Vol.
1 Numerical Simulation of NonNewtonian Flow (Crochet, Davies and Walters)
Vol.
2 Rheology of Materials and Engineering Structures (Sobotka)
Vol.
3 An Introduction to Rheology (Barnes, Hutton and Walters)
The photograph used on the cover shows an extreme example of the Weissenberg effect. It illustrates one of the most important nonlinear effects in rheology, namely, the existence of normal stresses. The effect is produced, quite simply, by rotating a rod in a dish of viscoelastic liquid. The liquid in the photograph was prepared by dissolving a high molecularweight polyisobutylene (Oppanol B200) in a low molecularweight solvent of the same chemical nature (Hyvis 07, polybutene). As the rod rotates, the liquid climbs up it, whereas a Newtonian liquid would move towards the rim of the dish under the influence of inertia forces. This particular experiment was set up and photographed at the Thornton Research Centre of Shell Research Ltd., and is published by their kind permission.
AN INTRODUCTION TO RHEOLOGY H.A.Barnes Senior Scientist and Subject Specialist in Rheology and Fluid Mechanics, Unilever Research, Port Sunlight Laboratory, Wirral, U. K.
J.F: Hutton Formerly: Principal Scientist and Leader of Tribology Group, Shell Research Ltd., Ellesmere Port, U.K. and
K. Walters
~
R. S.
Professor of Mathematics, University College of Wales, Aberystwyth, U.K
Elsevier Amsterdam  London  New York  Tokyo
ELSEVIER SCIENCE PUBLISHERS B.V. Sara Burgerhartstraat 25 P.O. Box 211,1000 AE Amsterdam, The Netherlands
I ''If, i;~" ..
First edition 1989 Second impression 1991 Third impression 1993
•
u
:.
••
• __ "
ZA m::::_l::uta
~
_.
.1."1
81 b ~~ . .J
( t:.
',~

KA
ISBN 0444871403 (Hardbound) ISBN 0444874690 (Paperback)
© 1989 Elsevier Science Publishers B. V. All rights reserved. No partofthis publication may be reproduced, stored in a retrieval system ortransmitted in any form or by any means, electronic, mechanical, photocopying, recording or otherwise, without the prior written permission of the publisher, Elsevier Science Publishers B.V./Physical Sciences & Engineering Division, P.O. Box 521,1000 AM Amsterdam, The Netherlands. Special regulations for readers in the USA  This publication has been registered with te Copyright Clearance Center Inc. (CCC), Salem, Massachusetts, Information can be obtained from the CCC about conditions under which photocopies of parts of this publication may be made in the USA. All other copyright questions, including photocopying outside of the USA, should be reffered to the publisher. No responsibility is assumed by the Publisher for any injury and/or damage to persons or property as a matter of products liability, negligence or otherwise, or from any use or operation of any methods, products, instructions or ideas contained in the material herein. Printed in The Netherlands
PREFACE
Rheology, defined as the science of deformation and flow, is now recognised as an important field of scientific study. A knowledge of the subject is essential for scientists employed in many industries, including those involving plastics, paints, printing inks, detergents, oils, etc. Rheology is also a respectable scientific discipline in its own right and may be studied by academics for their own esoteric reasons, with no major industrial motivation or input whatsoever. The growing awareness of the importance of rheology has spawned a plethora of books on the subject, many of them of the highest class. It is therefore necessary at the outset to justify the need for yet another book. Rheology is by common consent a difficult subject, and some of the necessary theoretical components are often viewed as being of prohibitive complexity by scientists without a strong mathematical background. There are also the difficuities inherent in any multidisciplinary science, like rheology, for those with a specific training e.g. in chemistry. Therefore, newcomers to the field are sometimes discouraged and for them the existing texts on the subject, some of which are outstanding, are of limited assistance on account of their depth of detail and highly mathematical nature. For these reasons, it is our considered judgment after many years of experience in industry and academia, that there still exists a need for a modern introductory text on the subject; one which will provide an overview and at the same time ease readers into the necessary complexities of the field, pointing them at the same time to the more detailed texts on specific aspects of the subject. In keeping with our overall objective, we have purposely (and with some difficulty) minimised the mathematical content of the earlier chapters and relegated the highly mathematical chapter on Theoretical Rheology to the end of the book. A glossary and bibliography are included. A major component of the anticipated readership will therefore be made up of newcomers to the field, with at least a first degree or the equivalent in some branch of science or engineering (mathematics, physics, chemistry, chemical or mechanical engineering, materials science). For such, the present book can be viewed as an important (first) stepping stone on the journey towards a detailed appreciation of the subject with Chapters 15 covering foundational aspects of the subject and Chapters 68 more specialized topics. We certainly do not see ourselves in competition with existing books on rheology, and if this is not the impression gained on reading the present book we have failed in our purpose. We shall judge the success v
VI
Preface
or otherwise of our venture by the response of newcomers to the field, especially those without a strong mathematical background. We shall not be unduly disturbed if longstanding rheologists find the book superficial, although we shall be deeply concerned if it is concluded that the book is unsound. We express our sincere thanks to all our colleagues and friends who read earlier drafts of various parts of the text and made useful suggestions for improvement. Mr Robin Evans is to be thanked for his assistance in preparing the figures and Mrs Pat Evans for her tireless assistance in typing the final manuscript. H.A. Barnes J.F. Hutton K. Walters
CONTENTS
PREFACE
'"
..
v
1.1 What is rheology? . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.2 Historical perspective 1.3 The importance of nonlinearity ,................ 1.4 Solids and liquids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.5 Rheology is a difficult subject 1.6 Components of rheological research ,........................... 1.6.1 Rheometry......,............................................ 1.6.2 Constitutive equations. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 1.6.3 Complex flows of elastic liquids . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
1 1 4 4 6 9 9 10 10
2. VISCOSITY 2.1 Introduction ,................................. 2.2 Practical ranges of variables which affect viscosity . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.1 Variation with shear rate. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.2.2 Variation with temperature 2.2.3 Variation with pressure. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3 The sheardependent viscosity of nonNewtonian liquids 2.3.1 Definition of Newtonian behaviour. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.2 The shearthinning nonNewtonian liquid . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.3 The shearthickening nonNewtonian liquid. . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.3.4 Time effects in nonNewtonian liquids 2.3.5 Temperature effects in twophase nonNewtonian liquids . . . . . . . . . . . . . . . . . . 2.4 Viscometers for measuring shear viscosity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.1 General considerations 2.4.2 Industrial shopfloor instruments . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.3 Rotational instruments; general comments 2.4.4 The narrowgap concentriccylinder viscometer . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.5 The widegap concentriccylinder viscometer . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.6 Cylinder rotating in a large volume of liquid 2.4.7 The coneandplate viscometer. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.8 The parallelplate viscometer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.9 Capillary viscometer . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 2.4.10 Slit viscometer ..................... ....... 2.4.11 Online measurements. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
11 12 12 12 14 15 15 16 23 24 25 25 25 26 26 27 28 29 30 31 32 34 35
3. LINEAR VISCOELASTICITY 3.1 Introduction....................................................... 3.2 The meaning and consequences of linearity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
37 38
1. INTRODUCTION
vii
viii 3.3 3.4 3.5 3.6 3.7
Contents
The Kelvin and Maxwell models. . . . . . . . . . . . . . . . . The relaxation spectrum Oscillatory shear . . . . . . . . . . . . . . . . . . . . . . . . . . . . Relationships between functions of linear viscoelasticity Methods of measurement. . . . . . . . . . . . . . . . . . . . . . 3.7.1 Static methods .................. 3.7.2 Dynamic methods: Oscillatory strain 3.7.3 Dynamic methods: Wave propagation. . . . . . . . 3.7.4 Dynamic methods: Steady flow .,. . . . . . . . . .
........................ . . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
........................ ........................
4. NORMAL STRESSES 4.1 The nature and origin of normal stresses . . . . . . . . . . . . . . . . . . . . . . . . . 4.2 Typical behaviour of N 1 and N z . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.3 Observable consequences of N 1 and N z . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4 Methods of measuring N 1 and N z . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4.1 Coneandplate flow . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 4.4.2 Torsional flow 4.4.3 Flow through capillaries and slits . . . . . . . . . . . . . . . . . . . . . . . . . 4.4.4 Other flows 4.5 Relationship between viscometric functions and linear viscoelastic functions
..........
39 43 46 50 51 51 52 53 54
..........
55 57 60 64 65 68 70 71 71
5. EXTENSIONAL VISCOSITY 5.1 Introduction....................................................... 5.2 Importance of extensional flow 5.3 Theoretical considerations. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4 Experimental methods . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.1 General considerations 5.4.2 Homogeneous stretching method .. 5.4.3 Constant stress devices 5.4.4 Spinning .... . . . . . . . . . . . . . . . . . . . . : . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.5 Lubricated flows. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.6 Contraction flows. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.4.7 Opensyphon method 5.4.8 Other techniques. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.5 Experimental results . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 5.6 Some demonstrations of high extensional viscosity behaviour
75 77 80 82 82 83 84 84 86 87 88 89 89 95
6. RHEOLOGY OF POLYMERIC LIQUIDS 6.1 Introduction....................................................... 6.2 General behaviour 6.3 Effect of temperature on polymer rheology ............... 6.4 Effect of molecular weight on polymer rheology . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.5 Effect of concentration on the rheology of polymer solutions. . . . . . . . . . . . . . . . . . . . . 6.6 Polymer gels. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.7 Liquid crystal polymers. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 6.8 Molecular theories 6.8.1 Basic concepts .. ,................................... . . . . . . . . . . 6.8.2 Beadspring models: The RouseZimm linear models. . . . . . . . . . . . . . . . . . . . . 6.8.3 The GiesekusBird nonlinear models. . . . . . . . . . . . . . . . . . â€˘ . . . . . . . . . . . . . 6.8.4 Network models. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.8.5 Reptation models . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 6.9 The method of reduced variables 6.10 Empirical relations between rheological functions. . . . . . . . . . . . . . . . . . . . . . . . . . . . .
97 97 101 102 103 104 105 106 106 106 107 108 108 109 111
.......... .......... .......... .......... ..........
Contents
6.11 Practical applications 6.11.1 Polymer processing . . . . . . . . . . . . . . . . . . . . 6.11.2 Polymers in engine lubricants. . . . . . . . . . . . . 6.11.3 Enhanced oil recovery . . . . . . . . . . . . . . . . . . 6.11.4 Polymers as thickeners of waterbased products
IX
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
. . . .
, . . .
. . . .
.. .. .. ..
111 III 113 113 114
7. RHEOLOGY OF SUSPENSIONS 7.1 Introduction....................................................... 7.1.1 The general form of the viscosity curve for suspensions. . . . . . . . . . . . . . . . . . . . 7.1.2 Summary of the forces acting on particles suspended in a liquid. . . . . . . . . . . . . . 7.1.3 Rest structures . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.1.4 Flowinduced structures ,... 7.2 The viscosity of suspensions of solid particles in Newtonian liquids 7.2.1 Dilute dispersed suspensions . . .. 7.2.2 Maximum packing fraction ............. ....... 7.2.3 Concentrated Newtonian suspensions. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.2.4 Concentrated shearthinning suspensions 7.2.5 Practical consequences of the effect of phase volume 7.2.6 Shearthickening of concentrated suspensions 7.3 The colloidal contribution to viscosity. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3.1 Overall repulsion between particles. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.3.2 Overall attraction between particles 7.4 Viscoelastic properties of suspensions . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 7.5 Suspensions of deformable particles ............ ................. 7.6 The interaction of suspended particles with polymer molecules also present in the continuous phase 7.7 Computer simulation studies of suspension rheology
136 137
8. THEORETICAL RHEOLOGY 8.1 Introduction....................................................... 8.2 Basic principles of continuum mechanics. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . 8.3 Successful applications of the formulation prin~iples 8.4 Some general constitutive equations . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 8.5 Constitutive equations for restricted classes of flows. . . . . . . . . . . . . . . . . . . . . . . . . . . 8.6 Simple constitutive equations of the Oldroyd/Maxwell type . . . . . . . . . . . . . . . . . . . . . '8.7 Solution of flow problems . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
141 142 145 149 150 152 156
GLOSSARY OF RHEOLOGICAL TERMS. . . .. . . . . . . . . . . . . . . .. . . . . . . . . . . . . . . . . .
159
REFERENCES . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
171
AUTHOR INDEX. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .
181
SUBJECT INDEX. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . ..
185
115 115 116 117 119 119 119 120 121 125 127 128 131 131 133 134 135
CHAPTER 1
INTRODUCTION
1.1 What is rheology? The term 'Rheology' * was invented by Professor Bingham of Lafayette College, Easton, PA, on the advice of a colleague, the Professor of Classics. It means the study of the deformation and flow of matter. This definition was accepted when the American Society of Rheology was founded in 1929. That first meeting heard papers on the properties and behaviour of such widely differing materials as asphalt, lubricants, paints, plastics and rubber, which gives some idea of the scope of the subject and also the numerous scientific disciplines which are likely to be involved. Nowadays, the scope is even wider. Significant advances have been made in biorheology, in polymer rheology and in suspension rheology. There has also been a significant appreciation of the importance of rheology in the chemical processing industries. Opportunities no doubt exist for more extensive applications of rheology in the biotechnological industries. There are now national Societies of Rheology in many countries. The British Society of Rheology, for example, has over 600 members made up of scientists from widely differing backgrounds, including mathematics, physics, engineering and physical chemistry. In many ways, rheology has come of age.
1.2 Historical perspective In 1678, Robert Hooke developed his "True Theory of Elasticity". He proposed that "the power of any spring is in the same proportion with the tension thereof", i.e. if you double the tension you double the extension. This forms the basic premise behind the theory of classical (infinitesimalstrain) elasticity. At the other end of the spectrum, Isaac Newton gave attention to liquids and in the" Principia" published in 1687 there appears the following hypothesis associated with the steady simple shearing flow shown in Fig. 1.1: "The resistance which arises from the lack of slipperiness of the parts of the liquid, other things being equal, is proportional to the velocity with which the parts of the liquid are separated from one another". * Definitions of terms in single quotation marks are included in the Glossary. 1
Introduction
2
[Chap. 1
A
'...J....J<::......4
"''
L
)(
Fig. 1.1 Showing two parallel planes, each of area A, at y = 0 and y = d, the intervening space being filled with sheared liquid. The upper plane moves with relative velocity U and the lengths of the arrows between the planes are proportional to the local velocity Vx in the liquid.
This lack of slipperiness is what we now call 'viscosity'. It is synonymous with "internal friction" and is a measure of "resistance to flow". The force per unit area required to produce the motion is F/ A and is denoted by (J and is proportional to the' velocity gradient' (or' shear rate') U/ d, i.e. If you double the force you double the velocity gradient. The constant of proportionality 11 is called the coefficient of viscosity, i.e. (J
=
(1.1)
11U/d.
(It is usual to write y for the shear rate U/ d; see the Glossary.) Glycerine and wa~er are common liquids that obey Newton's postulate. For glycerine, the viscosity in SI units is of the order of 1 Pa.s, whereas the viscosity of water is about 1 mPa.s, i.e. one thousand times less viscous. Now although Newton introduced his ideas in 1687, it was not until the nineteenth century that Navier and Stokes independently developed a consistent three~dimensional theory for what is now called a Newtonian viscous liquid. The governing equations for such a fluid are called the NavierStokes equations. For the simple shear illustrated in Fig. 1.1, a 'shear stress' (J results in 'flow'. In the case of a Newtonian liquid, the flow persists as long as the stress is applied. In contrast, for a Hookean solid, a shear stress (J applied to the surface y = d results in an instantaneous deformation as shown in Fig. 1.2. Once the deformed state is reached there is no further movement, but the deformed state persists as long as the stress is applied. The angle y is called the 'strain' and the relevant 'constitutive equation' is (J
(1.2)
= Gy,
where G is referred to as the' rigidity modulus'. y
y
I:r::,..       D
(T
Ir;~
c d c '
A B """"'x   ""'~=x
Fig. 1.2 The result of the application of a shear stress a to a block of Hookean solid (shown in section). On the application of the stress the material section ABCO is deformed and becomes A'B'C'O'.
1.2]
Historical perspective
3
Three hundred years ago everything may have appeared deceptively simple to Hooke and Newton, and indeed for two centuries everyone was satisfied with Hooke's Law for solids and Newton's Law for liquids. In the case of liquids, Newton's law was known to work well for some common liquids and people probably assumed that it was a universal law like his more famous laws about gravitation and motion. It was in the nineteenth century that scientists began to have doubts (see the review article by Markovitz (1968) for fuller details). In 1835, Wilhelm Weber carried out experiments on silk threads and found out that they were not perfectly elastic. "A longitudinal load", he wrote, "produced an immediate extension. This was followed by a further lengthening with time. On removal of the load an immediate contraction took place, followed by a gradual further decrease in length until the original length was reached". Here we have a solidlike material, whose behaviour cannot be described by Hooke's law alone. There are elements of flow in the described deformation pattern, which are clearly associated more with a liquidlike response. We shall later introduce the term' viscoelasticity' to describe such behaviour. So far as fluidlike materials are concerned, an influential contribution came in 1867 from a paper entitled "On the dynamical theory of gases" which appeared in the "Encyclopaedia Britannica". The author was James Clerk Maxwell. The paper proposed a mathematical model for a fluid possessing some elastic properties (see ยง3.3). The definition of rheology already given would allow a study of the behaviour of all maUer, including the classical extremes of Hookean elastic solids and Newtonian viscous liquids. However, these classical extremes are invariably viewed as being outside the scope of rheology. So, for example, Newtonian fluid mechanics based on the NavierStokes equations is not regarded as a branch of rheology and neither is classical elasticity theory. The overriding concern is therefore with materials between these classical extremes, like Weber's silk threads and Maxwell's elastic fluids. Returning to the historical perspective, we remark that the early decades of the twentieth century saw only the occasional study of rheological interest and, in general terms, one has to wait until the second World War to see rheology emerging as a force to be reckoned with. Materials used in flamethrowers were found to be viscoelastic and this fact generated its fair share of original research during the War. Since that time, interest in the subject has mushroomed, with the emergence of the syntheticfibre and plasticsprocessing industries, to say nothing of the appearance of liquid detergents, multigrade oils, nondrip paints and contact adhesives. There have been important developments in the pharmaceutical and food industries and modern medical research involves an important component of biorheology. The manufacture of materials by the biotechnological route requires a good understanding of the rheology involved. All these developments and materials help to illustrate the substantial relevance of rheology to life in the second half of the twentieth century.
4
Introduction
[Chap. 1
1.3 The importance of nonlinearity So far we have considered elastic behaviour and viscous behaviour in terms of the laws of Hooke and Newton. These are linear laws, which assume direct propor~ tionality between stress and strain, or strain rate, whatever the stress. Further, by implication, the viscoelastic behaviour so far considered is also linear. Within this linear framework, a wide range of rheological behaviour can be accommodated. However, this framework is very restrictive. The range of stress over which materials behave linearly is invariably limited, and the limit can be quite low. In other words, material properties such as rigidity modulus and viscosity can change with the applied stress, and the stress need not be high. The change can occur either instantaneously or over a long period of time, and it can appear as either an increase or a decrease of the material parameter. A common example of non~linearity is known as 'shear~thinning' (d. Â§2.3.2). This is a reduction of the viscosity with increasing shear rate in steady flow. The toothpaste which sits apparently unmoving on the bristles of the toothbrush is easily squeezed from the toothpaste tubea familiar example of shear~thinning. The viscosity changes occur almost instantaneously in toothpaste. For an example of shear~thinning which does not occur instantaneously we look to non~drip paint. To the observer equipped with no more than a paintbrush the slow recovery of viscosity is particularly noticeable. The special term for time~dependent shearthinning fol~ lowed by recovery is â€˘thixotropy', and non~drip paint can be described as thixo~ tropic. Shear~thinning is just one manifestation of non~linear behaviour, many others could be cited, and we shall see during the course of this book that it is difficult to make much headway in the understanding of rheology without an appreciation of the general importance of non~linearity.
1.4 Solids and liquids
It should now be clear that the concepts of elasticity and viscosity need to be qualified since real materials can be made to display either property or a combina~ tion of both simultaneously. Which property dominates, and what the values of the parameters are, depend on the stress and the duration of application of the stress. The reader will now ask what effect these ideas will have on the even more primitive concepts of solids and liquids. The answer is that in a detailed discussion of real materials these too will need to be qualified. When we look around at home, in the laboratory, or on the factory floor, we recognise solids or liquids by their response to low stresses, usually determined by gravitational forces, and over a human, everyday time~scale, usually no more than a few minutes or less than a few seconds. However, if we apply a very wide range of stress over a very wide spectrum of time, or frequency, using rheological apparatus, we are able to observe liquid~like properties in solids and solidlike properties in liquids. It follows therefore that difficulties can, and do, arise when an attempt is made to label a given material as a
1.4]
Solids and liquids
5
solid or a liquid. In fact, we can go further and point to inadequacies even when qualifying terms are used. For example, the term plasticrigid solid used in structural engineering to denote a material which is rigid (inelastic) below a 'yield stress' and yielding indefinitely above this stress, is a good approximation for a structural component of a steel bridge but it is nevertheless still limited as a description for steel. It is much more fruitful to classify rheological behaviour. Then it will be possible to include a given material in more than one of these classifications depending on the experimental conditions. A great advantage of this procedure is that it allows for the mathematical description of rheology as the mathematics of a set of behaviours rather than of a set of materials. The mathematics then leads to the proper definition of rheological parameters and therefore to their proper measurement (see also ยง3.1). To illustrate these ideas, let us take as an example, the silicone material that is nicknamed "Bouncing Putty". It is very viscous but it will eventually find its own level when placed in a containergiven sufficient time. However, as its name suggests, a ball of it will also bounce when dropped on the floor. It is not difficult to conclude that in a slow flow process, occurring over a long time scale, the putty behaves like a liquidit finds its own level slowly. Also when it is extended slowly it shows ductile fracturea liquid characteristic. However, when the putty is extended quickly, i.e. on a shorter time scale, it shows brittle fracturea solid characteristic. Under the severe and sudden deformation experienced as the putty strikes the ground, it bouncesanother solid characteristic. Thus, a given material can behave like a solid or a liquid depending on the time scale of the deformation process. The scaling of time in rheology is achieved by means of the 'Deborah number', which was defined by Professor Marcus Reiner, and may be introduced as follows. Anyone with a knowledge of the QWERTY keyboard will know that the letter "R" and the letter" T" are next to each other. One consequence of this is that any book on rheology has at least one incorrect reference to theology. (Hopefully, the present book is an exception!). However, this is not to say that there is no connection between the two. In the fifth chapter of the book of Judges in the Old Testament, Deborah is reported to have declared, "The mountains flowed before the Lord ... ". On the basis of this reference, Professor Reiner, one of the founders of the modern science of rheology, called his dimensionless group the Deborah number De' The idea is that everything flows if you wait long enough, even the mountains! (1.3) where T is a characteristic time of the deformation process being observed and T is a characteristic time of the material. The time T is infinite for a Hookean elastic solid and zero for a Newtonian viscous liquid. In fact, for water in the liquid state T is typically 10 12 s whilst for lubricating oils as they pass through the high pressures encountered between contacting pairs of gear teeth T can be of the order of 10 6 s
6
Introduction
[Chap. 1
and for polymer melts at the temperatures used in plastics processing 'r may be as high as a few seconds. There are therefore situations in which these liquids depart from purely viscous behaviour and also show elastic properties. High Deborah numbers correspond to solidlike behaviour and low Deborah numbers to liquidlike behaviour. A material can therefore appear solid路like either because it has a very long characteristic time or because the tleformation process we are using to study it is very fast. Thus, even mobile liquids with low characteristic times can behave like elastic solids in a very fast deformation process. This sometimes happens when lubricating oils pass through gears. Notwithstanding our stated decision to concentrate on material behaviour, it may still be helpful to attempt definitions of precisely what we mean by solid and liquid, since we do have recourse to refer to such expressions in this book. Accordingly, we define a solid as a material that will not continuously change its shape when subjected to a given stress, i.e. for a given stress there will be a fixed final deformation, which mayor may not be reached instantaneously on application of the stress. We define a liquid as a material that will continuously change its shape (i.e. will flow) when subjected to a given stress, irrespective of how small that stress may be. The term' viscoelasticity' is used to describe behaviour which falls between the classical extremes of Hookean elastic response and Newtonian viscous behaviour. In terms of ideal material response, a solid material with viscoelasticity is invariably called a 'viscoelastic solid' in the literature. In the case of liquids, there is more ambiguity so far as terminology is concerned. The terms 'viscoelastic liquid', 'elastico路viscous liquid', 'elastic liquid' are all used to describe a liquid showing viscoelastic properties. In recent years, the term' memory fluid' has also been used in this connection. In this book, we shall frequently use the simple term elastic liquid. Liquids whose behaviour cannot be described on the basis of the NavierStokes equations are called 'nonNewtonian liquids'. Such liquids mayor may not possess viscoelastic properties. This means that all viscoelastic liquids are nonNewtonian, but the converse is not true: not all nonNewtonian liquids are viscoelastic.
1.5 Rheology is a difficult subject By common consent, rheology is a difficult subject. This is certainly the usual perception of the newcomer to the field. Various reasons may be put forward to explain this view. For example, the subject is interdisciplinary and most scientists and engineers have to move away from a possibly restricted expertise and develop a broader scientific approach. The theoretician with a background in continuum mechanics needs to develop an appreciation of certain asp.ects of physical chemistry, statistical mechanics and other disciplines related to microrheological studies to fully appreciate the breadth of present~day rheological knowledge. Even more daunting, perhaps, is the need for nonmathematicians to come to terms with at least some aspects of nontrivial mathematics. A cursory glance at most text books
1.5]
Rheology is a difficult subject
7
on rheology would soon convince the uninitiated of this. Admittedly, the apparent need of a working knowledge of such subjects as functional analysis and general tensor analysis is probably overstated, but there is no doubting the requirement of some working knowledge of modem mathematics. This book is an introduction to rheology and our stated aim is to explain any mathematical complication to the nonspecialist. We have tried to keep to this aim throughout most of the book (until Chapter 8, which is written for the more mathematically minded reader). At this point, we need to justify the introduction of the indicial notation, which is an essential mathematical tool in the development of the subject. The concept of pressure as a (normal) force per unit area is widely accepted and understood; it is taken for granted, for example, by TV weather forecasters who are happy to display isobars on their weather maps. Pressure is viewed in these contexts as a scalar quantity, but the move to a more sophisticated (tensor) framework is necessary when viscosity and other rheological concepts are introduced. We consider a small plane surface of area Lls drawn in a deforming medium (Fig. 1.3). Let n x' n y and n z represent the components of the unit normal vector to the surface in the x, y, z directions, respectively. These define the orientation of Lls in space. The normal points in the direction of the + ve side of the surface. We say that the material on the + ve side of the surface exerts a force with components F.x(n) Lls, F;,(n) Lls, ~(n) Lis on the material on the  ve side, it being implicitly assumed that the area Lls is small enough for the 'stress' components F.x(n>, Fy(n), ~(n) to be regarded as constant over the small surface Lls. A more convenient notation is to replace these components by the stress components O'nx' O'ny' O'nz' the first index referring to the orientation of the plane surface and the second to the direction of the stress. Our sign convention, which is universally accepted, except by Bird et al. (l987(a) and (b)), is that a positive O'zz (and similarly O'yy and O'xx) is a tension. Components O'xx' O'yy and O'zz are termed 'normal stresses' and O'zx' O'zy etc. are called 'shear stresses'. It may be formally shown that O'xy = O'yx, O'xz = O'zx and O'yz = O'zy (see, for example Schowalter 1978, p. 44). Figure 1.4 may be helpful to the newcomer to continuum mechanics to explain
z
y
Fig. 1.3 The mutually perpendicular axes Ox, Oy, Oz are used to define the position and orientation of the small area .:is and the force on it.
Introduction
8
[Chap. 1
z
Uzy
Fig. 1.4 The components of stress on the plane surfaces of a volume element of a deforming medium.
the relevance of the indicial notation. The figure contains a schematic representation of the stress components on the plane surfaces of a small volume which forms part of a general continuum. The stresses shown are those acting on the small volume due to the surrounding material. The need for an indicial notation is immediately illustrated by a more detailed consideration of the steady simpleshear flow associated with Newton's postulate (Fig. 1.1), which we can conveniently express in the mathematical form:
(1.4) where vx ' vy' Vz are the velocity components in the x, y and z directions, respectively, and y is the (constant) shear rate. In the case of a Newtonian liquid, the stress distribution for such a flow can be written in the form
(1.5) and here there would be little purpose in considering anything other than the shear stress O'yx which we wrote as 0' in eqn. (1.1). Note that it is usual to work in terms of normal stress differences rather than the normal stresses themselves, since the latter are arbitrary to the extent of an added isotropic pressure in the case of incompressible liquids, and we would need to replace (1.5) by
Try,
O'yx
=
O'xx
= 
p,
O'xz
=
O'yy
=
O'yz

= 0, p,
_ O'zz 
} 
p,
(1.6)
where p is an arbitrary isotropic pressure. There is clearly merit in using (1.5) rather than (1.6) since the need to introduce p is avoided (see also Dealy 1982, p. 8). For elastic liquids, we shall see in later chapters that the stress distribution is more complicated, requiring us to modify (1.5) in the following manner:
= 1]( i' )y, O'xz = O'yz = 0, } O'xx  O'yy = N l (1'), O'yy  O'zz = N 2 (1' ), O'yx
(1.7)
1.6]
Components of rheological research
9
where it is now necessary to allow the viscosity to vary with shear rate, written mathematically as the function 1J( y), and to allow the normal stresses to be nonzero and also functions of y. Here the so called normal stress differences N 1 and N z are of significant importance and it is difficult to see how they could be conveniently introduced without an indicial notation *. Such a notation is therefore not an optional extra for mathematicallyminded researchers but an absolute necessity. Having said that, we console nonmathematical readers with the promise that this represents the only major mathematical difficulty we shall meet until we tackle the notoriously difficult subject of constitutive equations in Chapter 8.
1.6 Components of rheological research Rheology is studied by both university researchers and industrialists. The former may have esoteric as well as practical reasons for doing so, but the industrialist, for obvious reasons, is driven by a more pragmatic motivation. But, whatever the background or motivation, workers in rheology are forced to become conversant with certain welldefined subareas of interest which are detailed below. These are (i) rheometry; (ii) constitutive equations; (iii) measurement of flow behaviour in (nonrheometric) complex geometries; (iv) calculation of behaviour in complex flows.
1.6.1 Rheometry In 'rheometry', materials are investigated in simple flows like the steady simpleshear flow already discussed. It is an important component of rheological research. Smallamplitude oscillatoryshear flow (ยง3.5) and extensional flow (Chapter 5) are also important. The motivation for any rheometrical study is often the hope that observed behaviour in industrial situations can be correlated with some easily measured rheometrical function. Rheometry is therefore of potential importance in quality control and process control. It is also of potential importance in assessing the usefulness of any proposed constitutive model for the test material, whether this is based on molecular or continuum ideas. Indirectly, therefore, rheometry may be relevant in industrial process modelling. This will be especially so in future when the full potential of computational fluid dynamics using large computers is realized within a rheological context. A number of detailed texts dealing specifically with rheometry are available. These range from the "How to" books of Walters (1975) and Whorlow (1980) to the "Why?" books of Walters (1980) and Dealy (1982). Also, most of the standard texts * By common convention
N] is called the first normal stress difference and N 2 the second normal stress difference. However, the terms" primary" and" secondary" are also used. In some texts N] is defined as 0xxozz, whilst N 2 remains as 0yyozz'
10
Introduction
[Chap. 1
on rheology contain a significant element of rheometry, most notably Lodge (1964, 1974), Bird et al. (1987(a) and (b)), Schowalter (1978), Tanner (1985) and JaneschitzKriegl (1983). This last text also considers 'flow birefringence', which will not be discussed in detail in the present book (see also Doi and Edwards 1986, ยง4.7). 1.6.2 Constitutive equations Constitutive equations (or rheological equations of state) are equations relating suitably defined stress and deformation variables. Equation (1.1) is a simple example of the relevant constitutive law for the Newtonian viscous liquid. Constitutive equations may be derived from a microrheological standpoint, where the molecular structure is taken into account explicitly. For example, the solvent and polymer molecules in a polymer solution are seen as distinct entities. In recent years there have been many significant advances in microrheological studies. An alternative approach is to take a continuum (macroscopic) point of view. Here, there is no direct appeal to the individual microscopic components, and, for example, a polymer solution is treated as a homogeneous continuum. The basic discussion in Chapter 8 will be based on the principles of continuum mechanics. No attempt will be made to give an allembracing discourse on this difficult subject, but it is at least hoped to point the interested and suitably equipped reader in the right direction. Certainly, an attempt will be made to assess the status of the more popular constitutive models that have appeared in the literature, whether these arise from microscopic or macroscopic considerations. 1.6.3 Complex flows of elastic liquids The flows used in rheometry, like the viscometric flow shown in Fig. 1.1, are generally regarded as being simple in a rheological sense. By implication, all other flows are considered to be complex. Paradoxically, complex flows can sometimes occur in what appear to be simple geometrical arrangements, e.g. flow into an abrupt contraction (see ยง5.4.6). The complexity in the flow usually arises from the coexistence of shear and extensional components; sometimes with the added complication of inertia. Fortunately, in many cases, complex flows can be dealt with by using various numerical techniques and computers. The experimental and theoretical study of the behaviour of elastic liquids in complex flows is generating a significant amount of research at the present time. In this book, these areas will not be discussed in detail: they are considered in depth in recent review articles by Boger (1987) and Walters (1985); and the important subject of the numerical simulation of nonNewtonian flow is covered by the text of Crochet, Davies and Walters (1984).
12
Viscosity
[Chap. 2
but a function of the shear rate 1'. We define the function l}( 1') as the 'shear viscosity' or simply viscosity, although in the literature it is often referred to as the 'apparent viscosity' or sometimes as the sheardependent viscosity. An instrument designed to measure viscosity is called a 'viscometer'. A viscometer is a special type of 'rheometer' (defined as an instrument for measuring rheological properties) which is limited to the measurement of viscosity. The current SI unit of viscosity is the Pascalsecond which is abbreviated to Pa.s. Formerly, the widely used unit of viscosity in the cgs system was the Poise, which is smaller than the Pa.s by a factor of 10. Thus, for example, the viscosity of water at 20.2 0 C is 1 mPa.s (milIi Pascal~second) and was 1 cP (centipoise). In the following discussion we give a general indication of the relevance of viscosity to a number of practical situations; we discuss its measurement using various viscometers; we also study its variation with such experimental conditions as shear rate, time of shearing, temperature and pressure.
2.2 Practical ranges of variables which affect viscosity The viscosity of real materials can be significantly affected by such variables as shear rate, temperature, pressure and time of shearing, and it is clearly important for us to highlight the way viscosity depends on such variables. To facilitate this, we first give a brief account of viscosity changes observed over practical ranges of interest of the main variables concerned, before considering in depth the shear rate, which from the rheological point of view, is the most important influence on viscosity. 2.2.1 Variation with shear rate Table 2.2 shows the approximate magnitude of the shear rates encountered in a number of industrial and everyday situations in which viscosity is important and therefore needs to be measured. The approximate shear rate involved in any operation can be estimated by dividing the average velocity of the flowing liquid by a characteristic dimension of the geometry in which it is flowing (e.g. the radius of a tube or the thickness of a sheared layer). As we see from Table 2.2, such calculations for a number of important applications give an enormous range, covering 13 orders of magnitude from 10 6 to 10 7 S1. Viscometers can now be purchased to measure viscosity over this entire range, but at least three different instruments would be required for the purpose. In view of Table 2.2, it is clear that the shearrate dependence of viscosity is an important consideration and, from a practical standpoint, it is as well to have the particular application firmly in mind before investing in a commercial viscometer. We shall return to the shearrate dependence of viscosity in ยง2.3. 2.2.2 Variation with temperature So far as temperature is concerned, for most industrial applications involving aqueous systems, interest is confined to 0 to 100 0 C. Lubricating oils and greases are
2.2]
Practical ranges of variables which affect viscosity
13
TABLE 2.2 Shear rates typical of some familiar materials and processes Situation Sedimentation of fine powders in a suspending liquid Levelling due to surface tension Draining under gravity Extruders Chewing and swallowing Dip coating Mixing and stirring Pipe flow Spraying and brushing
Typical range of shear rates (s 1)
Medicines, paints 10 2_10 1 10 1 _10 1
101 _10 2 101 _10 2 10 1 _10 3 10 0 _10 3 10 3 _10 4
Paints, printing inks Painting and coating. Toilet bleaches Polymers Foods Paints, confectionary Manufacturing liquids Pumping. Blood flow Spraydrying, painting, fuel atomization Application of creams and lotions to the skin
10 3 _10 5 10 5 _10 6 10 3 _10 7
Paints, printing inks Paper Gasoline engines
100~102
Rubbing Milling pigments in fluid bases High speed coating Lubrication
Application
used from about  50 0 C to 300 0 C. Polymer melts are usually handled in the range 150 0 C to 300 0 C, whilst molten glass is processed at a little above 500 0 C. Most of the available laboratory viscometers have facilities for testing in the range  50 0 C to 150 0 C using an external temperature controller and a circulating fluid or an immersion bath. At higher temperatures, air baths are used. The viscosity of Newtonian liquids decreases with increase in temperature, approximately according to the Arrhenius relationship: (2.2) where T is the absolute temperature and A and B are constants of the liquid. In general, for Newtonian liquids, the greater the viscosity, the stronger is the temperature dependence. Figure 2.1 shows this trend for a number of lubricating oil fractions. The strong temperature dependence of viscosity is such that, to produce accurate results,great care has to be taken with temperature control in viscometry. For instance, the temperature sensitivity for water is 3% per 0 C at room temperature, so that + 1 % accuracy requires the sample temperature to be maintained to within + 0.3 0 C. For liquids of higher viscosity, given their stronger viscosity dependence on temperature, even greater care has to be taken.
Viscosity
14
[Chap. 2
o I
f::"1
"t)"t)
2
I
4
1/ in Po.s
t in deg C 5 6_l......_...J..  _ J . . . .'_I...... O.L' 4 2 3 log 1/
Fig. 2.1. Logarithm of viscosity/temperature derivative versus logarithm of viscosity for various lubricating oil fractions (Cameron 1966, p. 27).
It is important to note that it is not sufficient in viscometry to simply maintain control of the thermostat temperature; the act of shearing itself generates heat within the liquid and may thus change the temperature enough to decrease the viscosity, unless steps are taken to remove the heat generated. The rate of energy dissipation per unit volume of the sheared liquid is the product of the shear stress and shear rate or, equivalently, the product of the viscosity and the square of the shear rate. Another important factor is clearly the rate of heat extraction, which in viscometry depends on two things. First, the kind of apparatus: in one class the test liquid flows through and out of the apparatus whilst, in the other, test liquid is permanently contained within the apparatus. In the first case, for instance in slits and capillaries, the liquid flow itself convects some of the heat away. On the other hand, in instruments like the concentric cylinder and coneandplate viscometers, the conduction of heat to the surfaces is the only significant heattransfer process. Secondly, heat extraction depends on the dimensions of the viscometers: for slits and capillaries the channel width is the controlling parameter, whilst for concentric cylinders and coneandplate devices, the gap width is important. It is desirable that these widths be made as small as possible.
2.2.3 Variation with pressure The viscosity of liquids increases exponentially with isotropic pressure. Water below 30 0 C is the only exception, in which case it is found that the viscosity first decreases before eventually increasing exponentially. The changes are quite small for pressures differing from atmospheric pressure by about one bar. Therefore, for most practical purposes, the pressure effect is ignored by viscometer users. There
2.3]
15
The sheardependent viscosity 01 nonNewtonian liquids
]r, 2
2
_]
~
o
_ ______L.
200
_'____ _
_ ____L__ _____J
_ _ _ _ _ ' ~
400 600 800 Isotropic pressure, P//VtPa
1000
Fig. 2.2. Variation of viscosity with pressure: (a) Di(2ethylhexyl) sebacate; (b) Naphthenic mineral oil at 210 0 F; (c) Naphthenic mineral oil at 100 0 F. (Taken from Hutton 1980.)
are, however, situations where this would not be justified. For example, the oil industry requires measurements of the viscosity of lubricants and drilling fluids at elevated pressures. The pressures experienced by lubricants in gears can often exceed 1 GPa, whilst oilwell drilling muds have to operate at depths where the pressure is about 20 MPa. Some examples of the effect of pressure on lubricants is given in Fig. 2.2 where it can be seen that a viscosity rise of four orders of magnitude can occur for a pressure rise from atmospheric to 0.5 GPa.
2.3 The sheardependent viscosity of nonNewtonian liquids 2.3.1 Definition of Newtonian behaviour Since we shall concentrate on nonNewtonian viscosity behaviour in this section, it is important that we first emphasize what Newtonian behaviour is, in the context of the shear viscosity. Newtonian behaviour in experiments conducted at constant temperature and pressure has the following characteristics: (;) The only stress generated in simple shear flow normal stress differences being zero.
IS
the shear stress
(1,
the two
(ii) The shear viscosity does not vary with shear rate. (iii) The viscosity is constant with respect to the time of shearing and the stress in
the liquid falls to zero immediately the shearing is stopped. In any subsequent
16
Viscosity
[Chap. 2
shearing, however long the period of resting between measurements, the viscosity is as previously measured. (iv) The viscosities measured in different types of deformation are always in simple
proportion to one another, so, for example, the viscosity measured in a uniaxial extensional flow is always three times the value measured in simple shear flow (d. ยง5.3). A liquid showing any deviation from the above behaviour is nonNewtonian.
2.3.2 The shearthinning nonNewtonian liquid As soon as viscometers became available to investigate the influence of shear rate on viscosity, workers found departure from Newtonian behaviour for many materials, such as dispersions, emulsions and polymer solutions. In the vast majority of cases, the viscosity was found to decrease with increase in shear rate, giving rise to what is now generally called 'shearthinning' behaviour although the terms temporary viscosity loss and' pseudoplasticity' have also been employed. * We shall see that there are cases (albeit few in number) where the viscosity increases with shear rate. Such behaviour is generally called 'shearthickening' although the term 'dilatancy' has also been used. For shearthinning materials, the general shape of the curve representing the variation of viscosity with shear stress is shown in Fig. 2.3. The corresponding graphs of shear stress against shear rate and viscosity against shear rate are also gIven. The curves indicate that in the limit of very low shear rates (or stresses) the viscosity is constant, whilst in the limit of high shear rates (or stresses) the viscosity is again constant, but at a lower level. These two extremes are sometimes known as the lower and upper Newtonian regions, respectively, the lower and upper referring to the shear rate and not the viscosity. The terms" first Newtonian region" and "second Newtonian region" have also been used to describe the two regions where the viscosity reaches constant values. The higher constant value is called the "zeroshear viscosity". Note that the liquid of Fig. 2.3 does not show 'yield stress' behaviour although if the experimental range had been 10 4 S1 to 10 1 S1 (which is quite a wide range) an interpretation of the modified Fig. 2.3(b) might draw that conclusion. In Fig. 2.3(b) we have included socalled 'Bingham' plastic behaviour for comparison purposes. By definition, Bingham plastics will not flow until a critical yield stress Oy is exceeded. Also, by implication, the viscosity is infinite at zero shear rate and there is no question of a first Newtonian region in this case. There is no doubt that the concept of yield stress can be helpful in some practical situations, but the question of whether or not a yield stress exists or whether all nonNewtonian materials will exhibit a finite zeroshear viscosity becomes of more
... The German word is "strukturviscosiHit" which is literally translated as structural viscosity, and is not a very good description of shearthinning.
2.3]
The sheardependent viscosity of nonNewtonian liquids
17
1Il
ci
~
10
3
(a)
I::"
~'Ol 1Il
o
U
~ 10IL_ _
..L.._ _
/01
~
_'__~==:::::i::====::.
IDa 10 1 Sheaf stress
10 1
C1
103
/Pa
10 3
t>
vi 1Il
~
(b)
101
1Il
.... o
<l.J
65 10 1 ~...L_'___'__L.._'__'___'____''_'__ 1 1
.....
10 5
1Il
10' 10IDa Shear rate, ; /
10
10'
Sl
10 5
& "I::" 10
3
(e)
::
'iii 10' o
u
'!!! ~ 10 1 L.....L_''_L....'''___'''' /05
10" 101 IDa 101 Shear rate. ; /S1
10'
Fig. 2.3. Typical behaviour of a nonNewtonian liquid showing the interrelation between the different parameters. The same experimental data are used in each curve. (a) Viscosity versus shear stress. Notice how fast the viscosity changes with shear stress in the middle of the graph; (b) Shear stress versus shear rate. Notice that, in the middle of the graph, the stress changes very slowly with increasing shear rate. The dotted line represents ideal yieldstress (or Bingham plastic) behaviour; (c) Viscosity versus shear rate. Notice the wide range of shear rates needed to traverse the entire flow curve.
than esoteric interest as the range and sophistication of modern constantstress viscometers make it possible to study the very low shearrate region of the viscosity curve with some degree of precision (cr. Barnes and Walters 1985). We simply remark here that for dilute solutions and suspensions, there is no doubt that flow occurs at the smallest stresses: the liquid surface levels out under gravity and there is no yield stress. For more concentrated systems, particularly for such materials as gels, lubricating greases, ice cream, margarine and stiff pastes, there is understandable doubt as to whether or not a yield stress exists. It is easy to accept that a lump of one of these materials will never level out under its own weight. Nevertheless there is a growing body of experimental evidence to suggest that even concentrated systems flow in the limit of very low stresses. These materials appear not to flow merely because the zero shear viscosity is so high. If the viscosity is 10 10 Pa.s it would take years for even the slightest flow to be detected visually! The main factor which now enables us to explore with confidence the very low shearrate part of the viscosity curve is the availability, on a commercia) basis, of
Viscosity
18
[Chap. 2
constant stress viscometers of the Deer type (Davis et al. 1968). Before this development, emphasis was laid on the production of constant shearrate viscometers such as the FerrantiShirley coneandplate viscometer. This latter machine has a range of about 20 to 20,000 s ], whilst the Haake version has a range of about 1 to 1000 s\ in both cases a 10 3 fold range. The Umstatter capillary viscometer, an earlier development, with a choice of capillaries, provides a 10 6fold range. Such instruments are suitable for the middle and upper regions of the general flow curve but they are not suitable for the resolution of the low shearrate region. To do this, researchers used creep tests (Â§3.7.1) and devices like the plastometer (see, for example, Sherman, 1970, p 59), but there was no overlap between results from these instruments and those from the constant shearrate devices. Hence the low shearrate region could never be unequivocally linked with the high shearrate region. This situation has now changed and the overlap has already been achieved for a number of materials. Equations that predict the shape of the general flow curve need at least four parameters. One such is the Cross (1965) equation given by TI  TI 00
1
(2.2a)
Tlo  Tloo
or, what is equivalent, (2.2b) where Tlo and Tl oo refer to the asymptotic values of viscosity at very low and very high shear rates respectively, K is a constant parameter with the dimension of time and m is a dimensionless constant. A popular alternative to the Cross model is the model due to Carreau (1972) TI  TI 00 TI 0

Tl oo
1
(2.3)
where K] and m] have a similar significance to the K and m of the Cross model. By way of illustration, we give examples in Fig. 2.4 of the applicability of the Cross model to a number of selected materials. It is informative to make certain approximations to the Cross model, because, in so doing, we can introduce a number of other popular and widely used viscosity models. * For example, for TI ÂŤTlo and TI Âť Tl oo ' the Cross model reduces to (2.4)
... We have used shear rate as the independent variable. However, we could equally well have employed the shear stress in this connection, with, for instance, the socalled Ellis model as the equivalent of the Cross model.
2.3]
The sheardependent viscosity of nonNewtonian liquids
reI
VI
& E: 26
rd}
XANTHAN GU,., SOLUTION
AQUEOUS LA TEX
"~22 ~
~JO'I
"
"_ 18 VI 1l.
VI
S
.!!) ~1O~L'=....l_l
JO
19
O
10 1 Sheaf fate. ;/SI
10'
S 10]
~
10'1 10 ' Sheaf fate, ;/SI
10 3
Fig. 2.4. Examples of the applicability of the Cross equation (eqn. (2.2a)): (a) 0.4% aqueous solution of polyacrylamide. Data from Boger (1977(b)). The solid line represents the Cross equation with 110 = 1.82 Pa.s, 11 00 = 2.6 mPa.s, K = 1.5 s, and m = 0.60; (b) Blood (normal human, Hb = 37%). Data from Mills et al. (1980). The solid line represents the Cross equation with 110 = 125 mPa.s, 'l}oo = 5 mPa.s, K = 52.5 s and m = 0.715; (c) Aqueous dispersion of polymer latex spheres. Data from Quemada (1978). The solid line represents the Cross equation with 110 = 24 mPa.s, 11 00 = 11 mPa.s, K = 0.018 sand m = 1.0; (d) 0.35% aqueous solution of Xanthan gum. Data from Whitcomb and Macosko (1978). The solid line represents the Cross equation with 110 = 15 Pa.s, 1100 = 5 mPa.s, K = 10 s, m = 0.80.
which, with a simple redefinition of parameters can be written
(2.5) This is the well known (powerlaw' model and n is called the powerlaw index. K 2 called the 'consistency' (with the strange units of Pa.s n ). Further, if TJ 芦 TJo, we have
IS
(2.6) which can be rewritten as TJ = TJ oo
+ K 2Y路n} .
(2.7)
This is called the Sisko (1958) model. If n is set equal to zero in the Sisko model, we obtain TJ = TJ oo
K
+ ,2 , Y
(2.8a)
Viscosity
20
,
JO'
,,
[Chap. 2
, " , ,, ,, ,,
,, \
, \
''_L..'_''L..''
103
10 1
'_.1...'
10 1
Shear ra fe. ; /5 1
Fig. 2.5 Typical viscosity/shear rate graphs obtained using the Cross, powerlaw and Sisko models. Data for the Cross equation curve are the same as used in Fig. 2.3. The other curves represent the same data but have been shifted for clarity.
which, with a simple redefinition of parameters can be written (2.8b) where (Jy is the yield stress and l1 p the plastic viscosity (both constant). This is the Bingham model equation. The derived equations apply over limited parts of the 'flow curve'. Figure 2.5 illustrates how the powerlaw fits only near the central region whilst the Sisko model fits in the midtohigh shearrate range. The Bingham equation describes the shear stress/ shear rate behaviour of many shearthinning materials at low shear rates, but only over a onedecade range (approximately) of shear rate. Figures 2.6(a) and (b) show the Bingham plot for a synthetic latex, over two different shearrate ranges. Although the curves fit the equation, the derived parameters depend on the shearrate range. Hence, the use of the Bingham equation to characterize viscosity behaviour is unreliable in this case. However, the concept of yield stress is sometimes a very good approximation for practical purposes, such as in characterizing the ability of a grease to resist slumping in a roller bearing. Conditions under which this approximation is valid are that the local value of n is small (say < 0.2) and the ratio 110/11 00 is very large (say > 10 9 ). The Binghamtype extrapolation of results obtained with a laboratory viscometer to give a yield stress has been used to predict the size of solid particles that could be permanently suspended in a gelled liquid. This procedure rarely works in practice for thickened aqueous systems because the liquid flows, albeit slowly, at stresses below this stress. The use of 110 and Stokes' drag law gives a better prediction of the settling rate. Obviously, if this rate can be made sufficiently small the suspension becomes" nonsettling" for practical purposes.
2.3]
The sheardependent viscosity 0/ non·Newtonian liquids
200
21
14 (b)
(0) J50
/0
/00
6
_.
•
C1
y
=5'0 Po
50 o ~ b
vi
2
~"y=9'5Pa 00
40
Vl
~Vl 7 ~
80 120 Sheaf fate. 7/5. 1
160
0
2
4
6
Sheaf fate, 7/5"
(c)
<lJ
6j 5 3 ~.:
C1'y:;'1
10l Sheaf fate. 7/5 1
/0' ''_ _' I... /0' Sheaf fa te. ; /5'
J
/02
/0' (e)
(s <lJ
6j
JOG l...''_L....'_"'=__J JO· S 10'3 10'1 JO I 10 3 1 Sheaf ro te. 5
i/
Fig. 2.6. Flow curves for a synthetic latex (taken from Barnes and Walters 1985): (a and b) Bingham plots over two different ranges of shear rate, showing two different intercepts; (c) Semilogarithmic plot of data obtained at much lower shear rates, showing yet another intercept; (d) Logarithmic plot of data at the lowest obtainable shear rates, showing no yieldstress behaviour; (e) The whole of the experimental data plotted as viscosity versus shear rate on logarithmic scales.
The powerlaw model of eqn. (2.5) fits the experimental results for many materials over two or three decades of shear rate, making it more versatile than the Bingham model. It is used extensively to describe the nonNewtonian flow properties of liquids in theoretical analyses as well as in practical engineering applications. However, care should be taken in the use of the model when employed outside the range of the data used to define it. Table 2.3 contains typical values for the powerlaw parameters for a selection of wellknown nonNewtonian materials. The powerlaw model fails at high shear rates, where the viscosity must ulti
Viscosity
22
[Chap. 2
TABLE 2.3 Typical powerlaw parameters of a selection of wellknown materials for a particular range of shear rates. Material
K 2 (Pa.s n )
n
Shear rate range (s  I)
Ballpoint pen ink Fabric conditioner Polymer melt Molten chocolate Synovial fluid Toothpaste Skin cream Lubricating grease
10 10 10000 50 0.5 300 250 1000
0.85 0.6 0.6 0.5 0.4 0.3 0.1 0.1
10° _10 3 10°_10 2 10 2 _10 4 10 1 _10 10 1 _10 2 10° _10 3 100 _10 2 10 1 _10 2
mately approach a constant value; in other words, the local value of n must ultimately approach unity. This failure of the powerlaw model can be rectified by the use of the Sisko model, which was originally proposed for high shearrate measurements on lubricating greases. Examples of the usefulness of the Sisko model in describing the flow properties of shearthinning materials over four or five decades of shear rate are given in Fig. 2.7. Attempts have been made to derive the various viscosity laws discussed in this
FABRIC SOFTENER
CARBOPOL SOLUTION
(0)
VI
a.. 'o
(b)
_I
c:i
"
~
JQI
Shear rate, ;/5 1 YOGURT
(dl
POLYMER LIQUID CRYSTAL
JO I ~'_~:J....'=....J JQ1
100
Shear ra te,
J01
i/
51
JO1 JO 3L...::'_~L..":....J JOO /0 1 10' Shear ra te, j /5 1
Fig. 2.7. Examples of the applicability of the Sisko model (eqn. (2.7»: (a) Commercial fabric softener. Data obtained by Barnes (unpublished). The solid line represents the Sisko model with "7"" = 24 mPa.s, K 2 = 0.11 Pa.s nand n = 0.4; (b) 1% aqueous solution of Carbopol. Data obtained by Barnes (unpublished). The solid line represents the Sisko model with "7"" = 0.08 Pa.s, K 2 = 8.2 Pa.s n and n = 0.066; (c) 40% Racemic poly y benzyl glutamate polymer liquid crystal. Data points obtained from Onogi and Asada (1980). The solid line represents the Sisko model with "7"" = 1.25 Pa.s, K 2 = 15.5 Pa.s n, n = 0.5; (d) Commercial yogurt. Data points obtained from deKee et al. (1980). The solid line represents the Sisko model with "7"" = 4 mPa.s, K 2 = 34 Pa.s n and n = 0.1.
2.3]
The sheardependent viscosity of nonNewtonian liquids
23
section from microstructural considerations. However, these laws must be seen as being basically empirical in nature and arising from curvefitting exercises. 2.3.3 The shearthickening nonNewtonian liquid It is possible that the very act of deforming a material can cause rearrangement of its microstructure such that the resistance to flow increases with shear rate. Typical examples of the shearthickening phenomenon are given in Fig. 2.8. It will be observed that the shearthickening region extends over only about a decade of shear rate. In this region, the powerlaw model can usually be fitted to the data with a value of n greater than unity. In almost all known cases of shearthickening, there is a region of shearthinning at lower shear rates. (b)
JO (0)
(1)
o
Q...
E=
"b (3) lI)
~
5
.... o
lI)
<lJ
65 f~~~~~
,,82 S1 ,,85 S1
o0~5~0:':0:::0,0,J000='5=0J.....00....J Shear rate.
i /S1
째0'~~~....L..~'.l.......J
30
60
90
Time of shearing, t/min
5oo,...., ~70
lI)
(c)
ci
Q...
E
"
~IOO
~
.~I..l
66 50 '              
.~ l5
'               62
~
~
"
64
60
10 ':::20~0:::',6::'::0:::0,',:::0:'::0=0~
Shear rate,
i/
SI
Fig. 2.8. Examples of shearthickening behaviour: (a) Surfactant solution. CTAsal. solution at 25 0 C, showing a timeeffect (taken from Gravsholt 1979); (b) Polymer solution. Solution of antimisting polymer in aircraft jet fuel, showing the effect of photodegradation during (l) 1 day, (2) 15 days, (3) 50 days exposure to daylight at room temperature (taken from Matthys and Sabersky 1987); (c) Aqueous suspensions of solid particles. Deflocculated clay slurries showing the effect of concentration of solids. The parameter is the %w/w concentration (taken from Beazley 1980).
Viscosity
24
[Chap. 2
2.3.4 Time effects in nonNewtonian liquids We have so far assumed by implication that a given shear rate results in a corresponding shear stress, whose value does not change so long as the value of the shear rate is maintained. This is often not the case. The measured shear stress, and hence the viscosity, can either increase or decrease with time of shearing. Such changes can be reversible or irreversible. According to the accepted definition, a gradual decrease of the viscosity under shear stress followed by a gradual recovery of structure when the stress is removed is called' thixotropy'. The opposite type of behaviour, involving a gradual increase in viscosity, under stress, followed by recovery, is called 'negative thixotropy' or 'antithixotropy'. A useful review of the subject of time effects is provided by Mewis路 (1979). Thixotropy invariably occurs in circumstances where the liquid is shearthinning (in the sense that viscosity levels decrease with increasing shear rate, other things being equal). In the same way, antithixotropy is usually associated with shearthickening behaviour. The way that either phenomenon manifests itself depends on the type of test being undertaken. Figure 2.9 shows the behaviour to be expected from relatively inelastic colloidal materials in two kinds of test: the first involving step changes in applied shear rate or shear stress and the second being a loop test with
STEP CHANGE

LOOP TEST

QI
QI
lJ lJ
lJ .... ....
..c:
..c:
.... ....
lJ
QI
QI
VI
VI
TimfJ
III III CI>
~ III
.... lJ
Breakdown Equilibrium / , / levels of __ _str fJSS \
QI
Time III III QI
~
III
'lJ"
QI
..c:
..c:
VI
VI
Time
Time
Shear rote
Fig. 2.9. Schematic representation of the response of an inelastic thixotropic material to two shearrate histories.
2.4]
Viscometers for measuring shear viscosity
25
the shear rate increased continuously and linearly in time from zero to some maximum value and then decreased to zero in the same way. If highly elastic colloidal liquids are subjected to such tests, the picture is more complicated, since there are contributions to the stress growth and decay from viscoelasticity. The occurrence of thixotropy implies that the flow history must be taken into account when making predictions of flow behaviour. For instance, flow of a thixotropic material down a long pipe is complicated by the fact that the viscosity may change with distance down the pipe. 2.3.5 Temperature effects in twophase nonNewtonian liquids In the simplest case, the change of viscosity with temperature in twophase liquids is merely a reflection of the change in viscosity of the continuous phase. Thus some aqueous systems at room temperature have the temperature sensitivity of water, i.e. 3% per 0 C. In other cases, however, the behaviour is more complicated. In dispersions, the suspended phase may go through a melting point. This will result in a sudden and largerthanexpected decrease of viscosity. In those dispersions, for which the viscosity levels arise largely from the temperaturesensitive colloidal interactions between the particles, the temperature coefficient will be different from that of the continuous phase. For detergentbased liquids, small changes in temperature can result in phase changes which may increase or decrease the viscosity dramatically. In polymeric systems, the solubility of the polymer can increase or decrease with temperature, depending on the system. The coiled chain structure may become more open, resulting in an increase in resistance to flow. This is the basis of certain polymerthickened multigrade oils designed to maintain good lubrication at high temperatures by partially offsetting the decrease in viscosity with temperature of the base oil (see also ยง6.11.2). 2.4 Viscometers for measuring shear viscosity 2.4.1 General considerations Accuracy of measurement is an important issue in viscometry. In this connection, we note that it is possible in principle to calibrate an instrument in terms of speed, geometry and sensitivity. However, it is more usual to rely on the use of standardized Newtonian liquids (usually oils) of known viscosity. Variation of the molecular weight of the oils allows a wide range of viscosities to be covered. These oils are chemically stable and are not very volatile. They themselves are calibrated using glass capillary viscometers and these viscometers are, in turn, calibrated using the internationally accepted standard figure for the viscosity of water (1.002 mPa.s at 20.00 0 C, this value being uncertain to + 0.25 %). Bearing in mind the accumulated errors in either the direct or comparative measurements, the everyday measurement of viscosity must obviously be worse than the 0.25% mentioned above. In fact for mechanical instruments, accuracies of ten times this figure are more realistic.
Viscosity
26 VISCOMETER TYPE
~
0
e
~0
VARIABLES TO CHANGE
MEASUREMENT
BOB SPEED AND DIAMETER
COUPLE
EXIT TUBE DIAMETER
EFFLUX TIME
BALL SIZE
VELOCITY
CONVENIENCE
[Chap. 2 ROBUSTNESS
**
*
** **
** **
**
**
Fig. 2.10. Examples of industrial viscometers with complicated flow fields, including starratings for convenience and robustness.
2.4.2 Industrial shopfloor instruments Some viscometers used in industry have complicated flow and stress fields, although their operation is simple. In the case of Newtonian liquids, the use of such instruments does not present significant problems, since the instruments can be calibrated with a standard liquid. However, for nonNewtonian liquids, complicated theoretical derivations are required to produce viscosity information, and in some cases no amount of mathematical complication can generate consistent viscosity data (see, for example, Walters and Barnes 1980). Three broad types of industrial viscometer can be identified (Fig. 2.10). The first type comprises rotational devices, such as the Brookfield viscometer. There is some hope of consistent interpretation of data from such instruments (d. Williams 1979). The second type of instrument involves what we might loosely call "flow through constrictions" and is typified by the Fordcup arrangement. Lastly, we have those that involve, in some sense, flow around obstructions such as in the Glen Creston fallingball instrument (see, for example, van Wazer et al. 1963). Risingbubble techniques can also be included in this third category. For all the shopfloor viscometers, great care must be exercised in applying formulae designed for Newtonian liquids to the nonNewtonian case. 2.4.3 Rotational instruments; general comments Many types of viscometer rely on rotational motion to achieve a simple shearing flow. For such instruments, the means of inducing the flow are twofold: one can either drive one member and measure the resulting couple or else apply a couple and measure the subsequent rotation rate. Both methods were well established before the first World War, the former being introduced by Couette in 1888 and the latter by Searle in 1912. There are two ways that the rotation can be applied and the couple measured: the first is to drive one member and measure the couple on the same member, whilst the other method is to drive one member and measure the couple on the other. In
2.4]
Viscometers for measuring shear viscosity
27
modern viscometers, the first method is employed in the Haake, Contraves, FerrantiShirley and Brookfield instruments; the second method is used in the Weissenberg and Rheometrics rheogoniometers. For coupledriven instruments, the couple is applied to one member and its rate of rotation is measured. In Searle's original design, the couple was applied with weights and pulleys. In modem developments, such as in the Deer constantstress instrument, an electrical dragcup motor is used to produce the couple. The couples that can be applied by the commercial constant stress instruments are in the range 10 6 to 10 2 Nm; the shear rates that can be measured are in the range 10 6 to 10 3 S  I , depending of course on the physical dimensions of the instruments and the viscosity of the material. The lowest shear rates in this range are equivalent to one complete revolution every two years; nevertheless it is often possible to take steadystate measurements in less than an hour. As with all viscometers, it is important to check the calibration and zeroing from time to time using calibrated Newtonian oils, with viscosities within the range of those being measured. 2.4.4 The narrowgap concentriccylinder viscometer If the gap between two concentric cylinders is small enough and the cylinders are in relative rotation, the test liquid enclosed in the gap experiences an almost constant shear rate. Specifically, if the radii of the outer and inner cylinders are r o and r 1, respectively, and the angular velocity of the inner is QI' (the other being stationary) the shear rate y is given by (2.9) For the gap to be classed as "narrow" and the above approximation to be valid to within a few percent, the ratio of r 1 to r o must be greater than 0.97. If the couple on the cylinders is C, the shear stress in the liquid is given by (1=
C
,
(2.10)
21TrJL and from (2.9) and (2.10), we see that the viscosity is given by
(2.11) where L is the effective immersed length of the liquid being sheared. This would be the real immersed length, I, if there were no end effects. However, end effects are likely to occur if due consideration is not given to the different shearing conditions which may exist in any liquid covering the ends of the cylinders.
Viscosity
28
[Chap. 2
One way to proceed is to carry out experiments at various immersed lengths, l, keeping the rotational rate constant. The extrapolation of a plot of C against 1 then gives the correction which must be added to the real immersed length to provide the value of the effective immersed length L. In practice, most commercial viscometer manufacturers arrange the dimensions of the cylinders such that the ratio of the depth of liquid to the gap between the cylinders is in excess of 100. Under these circumstances the end correction is negligible. The interaction of one end of the cylinder with the bottom of the containing outer cylinder is often minimized by having a recess in the bottom of the inner cylinder so that air is entrapped when the viscometer is filled, prior to making measurements. Alternatively, the shape of the end of the cylinder can be chosen as a cone. In operation, the tip of the cone just touches the bottom of the outer cylinder container. The cone angle (equal to tan 1 [(ro  r1)/rO ]) is such that the shear rate in the liquid trapped between the cone and the bottom is the same as that in the liquid between the cylinders. This arrangement is called the Mooney system, after its inventor. 2.4.5 The widegap concentriccylinder viscometer
The limitations of very narrow gaps in the concentriccylinder viscometer are associated with the problems of achieving parallel alignment and the difficulty of coping with suspensions containing large particles. For these reasons, in many commercial viscometers the ratio of the cylinder radii is less than that stated in ยง2.4.4; thus some manipulation of the data is necessary to produce the correct viscosity. This is a nontrivial operation and has been studied in detail by Krieger and Maron (1954). Progress can be readily made if it is assumed that the shear stress/ shear rate relationship over the interval of shear rate in the gap can be described by the powerlaw model of eqn. (2.5). The shear rate in the liquid at the inner cylinder is then given by (2.12)
where b is the ratio of the inner to outer radius (i.e. b = r./ro )' Note that the shear rate is now dependent on the properties of the test liquid, unlike the narrowgap instrument. The shear stress in the liquid at the inner cylinder is given by C
(2.13)
The value of n can be determined by plotting C versus D 1 on a doublelogarithmic basis and taking the slope at the value of D1 under consideration.
2.4]
Viscometers for measuring shear viscosity
29
20 III
~
0 .... .... 18
..,.
0 Cll
..,
o.
.c: III ~ 0
E )(
....0
8:0
~
"0 ::J U 0
"
0 0
~
0
ct
10 05
06
07
08
09
b. ratIO of Inner to outer cylinder radII
Fig. 2.11. Ratio of actual (eqn. 2.12) to approximate (eqn. 2.9) shear rates at the rotating cylinder as a function of the ratio of the inner to the outer cylinder radii, with n, the power law index, as parameter.
The viscosity (measured at the innercylinder shear rate) is given by Cn(l  b 2/ 11=
4'1Trl Lfl 1
n
)
(2.14)
The error involved in employing the narrowgap approximation instead of the widegap expression, eqn. (2.14), is shown in Fig. 2.11. Clearly, using values of b < 0.97 gives unacceptable error when the liquid is shearthinning (n < 1). The lower limit of shear rate achievable in a rotational viscometer is obviously governed by the drive system. The upper limit, however, is usually controlled by the test liquid. One limit is the occurrence of viscous heating of such a degree that reliable correction cannot be made. However, there are other possible limitations. Depending on which of the cylinders is rotating, at a critical speed the simple circumferential streamline flow breaks down, either with the appearance of steady (Taylor) vortices or turbulence. Since both of these flows require more energy than streamline flow, the viscosity of the liquid apparently increases. In practical terms, for most commercial viscometers, it is advisable to consider the possibility of such disturbances occurring if the viscosity to be measured is less than about 10 mPa.s.
2.4.6 Cylinder rotating in a large volume of liquid If we take the widegap Couette geometry to the extreme with the radius of the outer cylinder approaching infinity, the factor (l  b 2/ n ) in (2.12) and (2.14)
Viscosity
30
[Chap. 2
Couple measuring device
.'8.. 0
,,
",
/
/
t\\\\\\\\\\\\l 52,
Drive
Fig. 2.12. The cone.and.plate viscometer. Crosssectional diagram of one possible configuration, viz. cone on top, rotating plate and couple measured on the cone. The inset shows the form of truncation used in many instruments.
approaches unity. For a powerlaw liquid, the values of the shear rate and shear stress in the liquid at the rotating cylinder of radius rl are then given by (2.15) and (2.16) Again, at any particular value of .o}' n can be calculated as the local value of d(ln C)/d(ln .0 1 ). These equations are applicable to viscometers of the Brookfield type in which a rotating bob is immersed in a beaker of liquid. The technique is restricted to moderately low shear rates: 0.1 s } to 10 s } is a typical range. 2.4.7 The coneandplate viscometer In the coneandplate geometry shown in Fig. 2.12, the shear rate is very nearly the same everywhere in the liquid provided the gap angle 80 is small (see Chapter 4 for the details). The shear rate in the liquid is given by (2.17) where .o} is the angular velocity of the rotating platten. Note that the shear rate does not depend on the properties of the liquid. The shear stress (measured via the couple C on the cone) is given by 3C
(]=   ,
2'1Ta 3
(2.18)
where a is the radius of the cone. Thus the viscosity is given by (2.19) If the liquid under investigation has a low viscosity, high rotational speeds are
2.4]
Viscometers for measuring shear viscosity
31
often necessary to produce torques large enough to be measured accurately. However, under these circumstances, 'secondary flows' may arise (see, for example, Walters 1975). The secondary flow absorbs extra energy, thus increasing the couple, which the unwary may mistakenly associate with shearthickening. Cheng (1968) has provided an empirical formula which goes some way towards dealing with the problem. All coneandplate instruments allow the cone to be moved away from the plate to facilitate sample changing. It is very important that the cone and plate be reset so that the tip of the cone lies in the surface of the plate. For a 1 0 gap angle and a cone radius of 50 mm, every 10 p.m of error in the axial separation produces an additional 1% error in the shear rate. To avoid error in contacting the cone tip (which might become worn) and the plate (which might become indented), the cone is often truncated by a small amount. In this case, it is necessary to set the virtual tip in the surface of the plate as shown in Fig. 2.12 (b). A truncated cone also facilitates tests on suspensions. 2.4.8 The parallelplate viscometer For torsional flow between parallel plates (see Fig. 2.13) the shear rate at the rim (r = a) is given by (2.20) It is this shear rate that finds its way into the interpretation of experimental data for torsional flow. It can be shown (Walters 1975, p. 52) that the viscosity is given by
3Ch
.,., =         4
(
21Ta .!lj 1 +
(2.21)
1 dIn C ) 3 d In .!lj
where C is the couple on one of the plates. For powerlaw models, eqn. (2.21) becomes 3Ch
C
(2.22)
Couple measuring device
~..,.,..,...,.""..,.,.,...,.....,.~.,...,..,...,.,~~
iti::: ;': ":: : :';:'::':>":;:~.:'/ :"::.~"'. :.:{:"':'\?
~
a~
fi,
Drive
Fig. 2.13. Crosssectional diagram of the torsional parallelplate viscometer.
Viscosity
32
[Chap. 2
It will be noticed from eqn. (2.20) that the rim shear rate may be changed by adjusting either the speed .Q) or the gap h.
In the torsionalbalance rheometer, an adaptation of the parallelplate viscometer (see Chapter 4 for the details), shear rates in the 10 4 to lOs s ) range have been attained. 2.4.9 Capillary viscometer If a Newtonian liquid flows down a straight circular tube of radius a at a volume flowrate Q (see Fig. 2.14), the pressure gradient generated along it (dPIdl) is given by the Poiseuille equation:
dP dl
8Q11 '!Ta 4
=
(2.23)
â€˘
In this situation, the shear stress in the liquid varies linearly from (aI2)(dPIdl) at the capillary wall to zero at the centre line. For Newtonian liquids, the shear rate varies similarly from 4Q/( '!Ta 3 ) in the immediate vicinity of the wall to zero at the centreline. If, however, the viscosity varies with shear rate the situation is more complex. Progress can be made by concentrating on flow near the wall. Analysis shows (cf. Walters 1975, Chapter 5) that for a nonNewtonian liquid, the shear rate at the wall is modified to
(1 + 1:
. _ 4Q '!Ta 3
4
yw
d In Q )
4 d In
Ow
(2.24)
'
whilst the shear stress at the wall Ow, is unchanged at (aI2) (dP Idl). The bracketed term in (2.24) is called the Rabinowitsch correction. Then finally (2.25)
When shearthinning liquids are being tested, d(ln Q)/d(ln ow) is greater than 1 and for powerlaw liquids is equal to lin. Since n can be as low as 0.2, the contribution Velocity profile VOlumetric I flow rate __
a \
f(
...
"~\
T
20
~

/
./
1
IDifferentiol pressure dP over length dlJ,
Fig. 2.14. Cutaway diagram of laminar Newtonian flow in a straight circular capillary tube.
2.4]
Viscometers for measuring shear viscosity
33
of the d(ln Q)/d(ln ow) factor to the bracketed term can be highly significant in determining the true wall shear rate. Care has to be taken in defining and measuring the pressure gradient dP/dl. If the pressure in the external reservoir supplying the capillary and the receiving vessel are measured, then, unless the ratio of tube length to radius is very large (> 100), allowance must be made for entrance and exit effects. These arise from the following sources for all types of liquid: (i) Viscous and inertial losses in the converging stream up to the entrance. (ii) Redistribution of the entrance velocities to achieve the steady state velocity
profile within the tube. (iii) Similar effects to the above at the exit.
Formulae exist which account for these effects for Newtonian liquids, (i) and (iii) being associated with the names of Hagenbach and Couette (see, for example Kestin et al. 1973). However, these effects are small if the ratio of tube length to radius is 100 or more. The main end effects can be avoided if at various points on the tube wall, well away from the ends, the pressures are measured by holes connected to absolute or differential pressure transducers. Any error arising from the flow of the liquid past the holes in the tube wall (see ยง4.4.1.II) is cancelled out when identical holes are used and the pressure gradient alone is required. It is not often convenient to drill pressuretappings, and a lengthy experimental programme may then be necessary to determine the type(i) errors in terms of an equivalent pressuredrop and type(ii) errors in terms of an extra length of tube. The experiments required can be deduced from the theoretical treatment of Kestin et al. (1973) and a recent application of them has been published by Galvin et al. (1981). If the liquid is highly elastic, an additional entrance and exit pressure drop arises from the elasticity. The socalled Bagley correction then allows an estimate of the elastic properties to be calculated. It is also used to provide an estimate of the extensional viscosity of the liquid (see ยง5.4.6). Before leaving the discussion of the capillary viscometer, it is of interest to study the pressuregradient/flowrate relationship for the powerlaw model (2.5): dP = 2K 2 dl a
[
(3n + l)Q] n ~na3
(2.26)
From this equation we see the effect of changes in such variables as pipe radius. For Newtonian liquids, the pressure drop for a given flow rate is proportional to the fourth power of the radius, but this is changed if the liquid is shearthinning. For instance, if n = t, the pressure drop is proportional to the square of the radius. This is clearly important in any scaleup of pipe flow from pilot plant to factory operation.
Viscosity
34
[Chap. 2
, ......
~
\
Power (ow index, n
"'
\
"
\
"
\:
02 04    1路0
\
:
I
,:
/
I I
"\
I
, /. / , /
/
,/ ,/
'/
Fig. 2.15. The velocity profiles for the laminar flow of powerlaw liquids in a straight circular pipe, calculated for the same volumetric throughput. Note the increase in the wall shear rate and the increasingly pluglike nature of the flow as n decreases.
The velocity profile in pipe flow is parabolic for Newtonian liquids. For powerlaw liquids this is modified to v(r)=
Q(3n+l) ( 2
'lTa (n
+ 1)
(r)(n+l)/n) .
1 
a
(2.27)
Figure 2.15 shows the effect of progressively decreasing the powerlaw index, i.e. increasing the degree of shear thinning. We see the increasing pluglike nature of the flow with, effectively, only a thin layer near the wall being sheared. This has important consequences in heattransfer applications, where heating or cooling is applied to the liquid from the outside of the pipe. The overall heat transfer is partly controlled by the shear rate in the liquid near the pipe wall. For a powerlaw liquid, this shear rate is changed from the Newtonian value by a factor [3 + (l/n)]/4. This means that heat transfer is increased for shearthinning liquids (n < 1) and decreased for shearthickening liquids (n > 1), but the former is the larger effect. 2A.l0 Slit viscometer Flow under an applied pressure gradient between two parallel stationary walls is known as slit flow. It is a twodimensional analogue of capillary flow. The governing equations for slit flow are (d. Walters 1975, Chapter 5)
(2.28) and
.
2Q (
y w = bh 2 2
din Q)
+ d In
Ow
'
(2.29)
2.4]
Viscometers for measuring shear viscosity
35
where h is the slit height and b is the slit width, Q is the flow rate and dP/dl is the pressure gradient. Slit flow forms the basis of the viscometer version of the Lodge stressmeter. The stressmeter is described more fully in Chapter 4. The viscometer version differs from that discussed in ยง4.4.3 in that the transducer T 1 in Fig. 4.13 is unnecessary and is replaced by a solid wall. The instrument has the advantage that shear rates in excess of 10 6 S1 can be achieved with little interference from viscous heating. 2.4.11 Online measurements It is frequently necessary to monitor the viscosity of a liquid "on line" in a number of applications, particularly when the constitution or temperature of the liquid is likely to change. Of the viscometers described in this chapter, the capillary viscometer and the concentriccylinder viscometer are those most conveniently adapted for such a purpose. For the former, for example, the capillary can be installed directly in series with the flow: the method has attractive features, but its successful application to nonNewtonian liquids is nontrivial. Care must be taken with the online concentriccylinder apparatus, since the interpretation of data from the resulting helical flow is not easy. Other online methods involve obstacles in the flow channel: for example, a float in a vertical tapered tube, as in the Rotameter, will arrive at an equilibrium position in the tube depending on the precise geometry, the rate of flow, the viscosity and the weight of the obstacle. The parallelplate viscometer has also been adapted for online measurement (see, for example, Noltingk 1975).
CHAPTER 3
LINEAR VISCOELASTICITY
3.1 Introduction The word 'viscoelastic' means the simultaneous existence of viscous and elastic properties in a material (d. ยง1.2). It is not unreasonable to assume that all real materials are viscoelastic, i.e. in all materials, both viscous and elastic properties coexist. As was pointed out in the Introduction, the particular response of a sample in a given experiment depends on the timescale of the experiment in relation to a natural time of the material. Thus, if the experiment is relatively slow, the sample will appear to be viscous rather than elastic, whereas, if the experiment is relatively fast, it will appear to be elastic rather than viscous. At intermediate timescales mixed, i.e. viscoelastic, response is observed. The concept of a natural time of a material will be referred to again later in this chapter. However, a little more needs to be said about the assumption of viscoelasticity as a universal phenomenon. It is not a generallyheld assumption and would be difficult to prove unequivocally. Nevertheless, experience has shown that it is preferable to assume that all real materials are viscoelastic rather than that some are not. Given this assumption, it is then incorrect to say that a liquid is Newtonian or that a solid is Hookean. On the other hand, it would be quite correct to say that suchandsuch a material shows Newtonian, or Hookean, behaviour in a given situation. This leaves room for ascribing other types of behaviour to the material in other circumstances. However, most rheologists still refer to certain classes of liquid (rather than their behaviour) as being Newtonian and to certain classes of solid as being Hookean, even when they know that these materials can be made to deviate from the model behaviours. Indeed, it is done in this book! Old habits die hard. However, it is considered more important that an introductory text should point out that such inconsistencies exist in the literature rather than try to maintain a purist approach. For many years, much labour has been expended in the determination of the linear viscoelastic response of materials. There are many reasons for this (see, for example, Walters 1975, p. 121, Bird et al. 1987(a), p. 225). First there is the possibility of elucidating the molecular structure of materials from their linearviscoelastic response. Secondly, the material parameters and functions measured in the relevant experiments sometimes prove to be useful in the qualitycontrol of industrial products. Thirdly, a background in linear viscoelasticity is helpful before proceeding to the much more difficult subject of nonlinear viscoelasticity (d. the relative simplicity of the mathematics in the present chapter with that in Chapter 8 37
38
Linear viscoelasticity
[Chap. 3
which essentially deals with nonlinear viscoelasticity). Finally, a further motivation for some past studies of viscoelasticity came from tribology, where knowledge of the steady shear viscosity function 11 ( Y) discussed in ยง2.3 was needed at high shear rates (10 6 s lor higher). Measurements of this function on lowviscosity" Newtonian" lubricants at high shear rates were made difficult by such factors as viscous heating, and this led to a search for an analogy between shear viscosity and the corresponding dynamic viscosity determined under linear viscoelastic conditions, the argument being that the latter viscosity was easier to measure (see, for example, Dyson 1970). Many books on rheology and rheometry have sections on linear viscoelasticity. We recommend the text by Ferry (1980) which contains a wealth of information and an extensive list of references. Mathematical aspects of the subject are also well covered by Gross (1953) and Staverman and Schwarzl (1956).
3.2 The meaning and consequences of linearity The development of the mathematical theory of linear viscoelasticity is based on a "superposition principle". This implies that the response (e.g. strain) at any time is directly proportional to the value of the initiating signal (e.g. stress). So, for example, doubling the stress will double the strain. In the linear theory of viscoelasticity, the differential equations are linear. Also, the coefficients of the time differentials are constant. These constants are material parameters, such as viscosity coefficient and rigidity modulus, and they are not allowed to change with changes in variables such as strain or strain rate. Further, the time derivatives are ordinary partial derivatives. This restriction has the consequence that the linear theory is applicable only to small changes in the variables. We can now write down a general differential equation for linear viscoelasticity as follows:
(3.1) where n = m or n = m  1 (see for example, Oldroyd 1964). Note that for simplicity we have written (3.1) in terms of the shear stress a and the strain y, relevant to a simple shear of the sort discussed in Chapter 1, except that we now allow a and y to be functions of the time t. However, we emphasise that other types of deformation could be included without difficulty, with the stress and strain referring to that particular deformation process. Mathematically, this means that we could replace the scalar variables a and y by their tensor generalizations. For example, a could be replaced by the stress tensor ai)'
3.3]
The Kelvin and Maxwell models
39
3.3 The Kelvin and Maxwell models We now consider some important special cases of eqn. (3.1). If f30 is the only nonzero parameter, we have
(3.2) which is the equation of Hookean elasticity (i.e. linear solid behaviour) with f30 as the rigidity modulus. If f3I is the only nonzero parameter, we have (3.3)
or (J
(3.4)
f3d
=
in our notation. This represents Newtonian viscous flow, the constant f3I being the coefficient of viscosity. If f30 (= G) and f3I (= 11) are both nonzero, whilst the other constants are zero, we have (J
=
Gy +11Y,
(3.5)
which is one of the simplest models of viscoelasticity. It is called the' Kelvin model', although the name' Voigt' is also used. If a stress ii is suddenly applied at t = 0 and held constant thereafter, it is easy to show that, for the Kelvin model, y
=
(iii G) [1  exp (  tiT K ) ] ,
(3.6)
where TK has been written for the ratio 11IG. It has the dimension of time and controls the rate of growth of strain y following the imposition of the stress ii. Figure 3.1 shows the development of the dimensionless group yGIii diagrammatically. The equilibrium value of y is iilG; hence yGlii = 1, which is also the value for the Hooke model. The difference between the two models is that, whereas the 1路0r~====~HOOKE MODEL
rG/B
o
L...
=
_
Time
Fig. 3.1 Growth of strain y following the application of stress ii at time Hooke model.
t
= 0 for a Kelvin model and
Linear viscoelasticity
40
[Chap. 3
Hooke model reaches its final value of strain "instantaneously", in the Kelvin model the strain is retarded. The time constant 'TK is accordingly called the 'retardation time'. The word instantaneously is put in quotation marks because in practice the strain could not possibly grow in zero time even in a perfectly elastic solid, because the stress wave travels at the speed of sound, thus giving rise to a delay. It is useful at this stage to introduce "mechanical models", which provide a popular method of describing linear viscoelastic behaviour. These onedimensional mechanical models consist of springs and dashpots so arranged, in parallel or in series, that the overall system behaves analogously to a real material, although the elements themselves may have no direct analogues in the actual material. The correspondence between the behaviour of a model and a real material can be achieved if the differential equation relating force, extension and time for the model is the same as that relating stress, strain and time for the material, i.e. this method is equivalent to writing down a differential equation relating stress and strain, but it has a practical advantage in that the main features of the behaviour of a material can often be inferred by inspection of the appropriate model, without going into the mathematics in detail. In mechanical models, Hookean deformation is represented by a spring (i.e. an element in which the force is proportional to the extension) and Newtonian flow by a dashpot (i.e. an element in which the force is porportional to the rate of extension) as shown in Fig. 3.2. The analogous rheological equations for the spring and the dashpot are (3.2) (with /30 = G) and (3.4) (with /31 = 11), respectively. The behaviour of more complicated materials is described by connecting the basic elements in series or in parallel. The Kelvin model results from a parallel combination of a spring and a dashpot (Fig. 3.3(a)). A requirement on the interpretation of this and all similar diagrams is that the horizontal connectors remain parallel at all times. Hence the extension (strain) in the spring is at all times equal to the extension (strain) in the dashpot. Then it is possible to set up a balance equation for the forces (stresses) acting on a connector. The last step is to write the resulting equation in terms of stresses and strains. Hence, for the Kelvin model the total stress (J is equal to the sum of the stresses in each element. Therefore
(3.7)
1 (0)
(b)
Fig. 3.2 Diagrammatic representations of ideal rheological behaviour: (a) The Hookean spring; (b) The Newtonian dashpot.
3.3]
The Kelvin and Maxwell models
41
1
h
G
(a)
(b)
Fig. 3.3 The simplest linear viscoelastic models: (a) The Kelvin model; (b) The Maxwell model.
in the obvious notation, and using eqns. (3.2) and (3.4) (with have (J
= Gy
+ 1]Y.
/30 =
G and
/31 =
1]) we
(3.8)
This is identical to eqn. (3.5), which was a very simple case of the general linear differential equation (3.1). It is readily seen from the diagram of the Kelvin model that after sudden imposition of a shear stress 0, the spring will eventually reach the strain given by 0/ G, but that the dashpot will retard the growth of the strain and, the higher the viscosity, the slower will be the response. Another very simple model is the socalled 'Maxwell model' *. The differential equation for the model is obtained by making al and /31 the only nonzero material parameters, so that
(3.9) where we have written a 1 = 7"M and /31 = 1]. If a particular strain rate y is suddenly applied at subsequent times, we can show that, for t > 0,
t =
0 and held at that value for
(3.10) which implies that on startup of shear, the stress growth is delayed~ the time constant in this case is 7"M' On the other hand, if a strain rate which has had a constant value y for t < 0 is suddenly removed at t = 0, we can show that, for t ~ 0, (3.11) Hence the stress relaxes exponentially from its equilibrium value to zero (see Fig. 3.4). The rate constant 7"M is called the' relaxation time'. * Recall the discussion in ยง1.2 concerning the influence of J.e. Maxwell on the introduction of the concept of viscoelasticity in a fluid.
Linear viscoelasticity
42
[Chap. 3
JO
OL....Time
Fig. 3.4 Decay of stress where 00 = 11,(Âˇ
0
following the cessation of steady shear at time t = 0 for a Maxwell model,
The pictorial Maxwell model is a spring connected in series with a dashpot (see Fig. 3.3(b)). In this case, the strains, or equally strainrates, are additive; hence the total rate of shear y is the sum of the rates of shear of the two elements. Thus (3.12) which leads to d
(J
1'=+G 11
(3.13)
or, after rearrangement, (3.14) in which 'TM has been written for 11/G. This equation is the same as eqn. (3.9) which arose as a special case of the general differential equation. The next level of complexity in the linear viscoelastic scheme is to make three of the material parameters of eqn. (3.1) non zero. If aI' /31 and /32 are taken to be nonzero we have the" Jeffreys model". In the present notation, the equation is (3.15) which has two time constants 'TM and 'TJ â€˘ With a suitable choice of the three model parameters it is possible to construct two alternative springdashpot models which correspond to the same mechanical behaviour as eqn. (3.15). One is a simple extension of the Kelvin model and the other a simple extension of the Maxwell model as shown in Fig. 3.5. We note with interest that an equation of the form (3.15) was derived mathematically by Frohlich and Sack (1946) for a dilute suspension of solid elastic spheres in a viscous liquid, and by Oldroyd (1953) for a dilute emulsion of one incompressible viscous liquid in another. When the effect of interfacial slipping is taken into account in the dilute suspension case, Oldroyd (1953) showed that two further nonzero parameters (a2 and /32) are involved.
3.4]
The relaxation spectrum
(0)
43
(b)
Fig. 3.5 Springdashpot equivalents of the Jeffreys model. The values of the constants of the elements are given in terms of the three material parameters of the model (eqn. 3.15).
~3l:fJ_
S=J ~,
1
(0)
(b)
Fig. 3.6 The Burgers model: (a) and (b) are equivalent representations of this 4parameter linear model.
Finally, in this preliminary discussion of the successive buildup of model complexity, we draw attention to the socalled "Burgers model". This involves four simple elements and takes the mechanicallyequivalent forms shown in Fig. 3.6. In terms of the parameters of the Maxwelltype representation (Fig. 3.6(b)), the associated constitutive equation for the Burgers model has the form (3.16) In this equation the AS are time constants, the symbol A being almost as common as 'T in the rheological literature. 3.4 The relaxation spectrum It is certainly possible to envisage more complicated models than those already
introduced, but Roscoe (1950) showed that all models, irrespective of their complexity, can be reduced to two canonical forms. These are usually taken to be the generalized Kelvin model and the generalized Maxwell model (Fig. 3.7). The generalized Maxwell model may have a finite number or an enumerable infinity of Maxwell elements, each with a different relaxation time.
Linear viscoelasticity
44
(Chap. 3
(b) Fig. 3.7 Canonical springdashpot models: (a) Distribution of Maxwell relaxation processes; (b) Distribution of Kelvin retardation processes.
Bya suitable choice of the model parameters, the canonical forms themselves can be shown to be mechanically equivalent and Alfrey (1945) has given methods for computing the parameters of one canonical form from those of the other. In the same paper, Alfrey also showed how a linear differential equation can be obtained for either of the canonical forms and vice versa. In other words, the three methods of representing viscoelastic behaviour (the differential equation (3.1) and the two canonical forms of mechanical model of Fig. 3.7 are equivalent and one is free to choose anyone of them as a basis for generalization to materials requiring a continuous infinity of parameters to specify them. In order to generalize from an enumerable infinity to a continuous distribution of relaxation times, we choose to start with the simple Maxwell model, whose behaviour is characterized by the differential equation (3.9) or what is equivalent
(J (
I)
f
= ~ ~ 00 exp [  ( I  If) /
T]
i' ( If) d If,
(3.17)
where we have dropped the subscript M in T M to enable us to generalize eqn. (3.17) without introducing a clumsy notation. * (See p. 144 for definitions of I and If). Considering next, a number, n, of discrete Maxwell elements connected in parallel as in Fig. 3.7(a), we can generalize eqn. (3.17), with the aid of the * The integral equation (3.17) techniques.
IS
obtained by solving the differential equation (3.9) by standard
3.4]
The relaxation spectrum
45
superposition principle, to give n
o(t) =
i~l
f~oo exp[ 
:;
(t  t')/T;] yet') dt',
(3.18)
where 11; and T; now correspond to the ith Maxwell element. The theoretical extension to a continuous distribution of relaxation times can be carried out in a number of ways. For example, we may proceed as follows. The "distribution function of relaxation times" (or "relaxation spectrum") N( T) may be defined such that N( T) d T represents the contributions to the total viscosity of all the Maxwell elements with relaxation times lying between T and T + d T. The relevant equation then becomes (on generalizing (3.18))
1o N ( T) ft 00
o ( t) =
T
exp [  (t  t') / T] Y( t ') d t' d T,
(3.19)
00
and if we introduce the" relaxation function" </>, defined by </>(t_t')=l
OON
o
(T) exp[(tt')/T] dT,
(3.20)
T
eqn. (3.19) becomes o(t)
=
ft 
</>(t  t')y(t') dt'.
(3.21)
00
We remark that we could have immediately written down an equation like (3.21) on the basis of Boltzmann's superposition principle. It is also possible to proceed from eqn. (3.18) by introducing a distribution function H( T) such that H( T) d T represents the contribution to the elasticity modulus of the processes with relaxation times lying in the interval T and T + d T. Further, other workers have used a spectrum of relaxation frequencies H(log F) where F = 1/(2 ']7'T). The relationships between these functions are (N(T)/T) dT=H(T) dT=H(log F) d(log F).
(3.22)
In a slow steady motion which has been in existence indefinitely (i.e. y is small, and independent of time) eqn. (3.21) reduces to 0=
110Y,
where
(3.23)
Linear viscoelasticity
46
[Chap. 3
in which ~ has been written for the time interval (t  t'). The variable ~ is the one which represents the timescale of the rheological history. It is also easy to show from eqns. (3.19), (3.21) and (3.22) that
00 N(r) dr= 100rH(r) dr= foo00 H(log F) 27TF
1
110= 0
0
d(log F).
(3.24)
We see from eqn. (3.23) that 110 can be identified with the limiting viscosity at small rates of shear, as observed in steady state experiments. Thus, the equations in (3.24) provide useful normalization conditions on the various relaxation spectra. It is also of interest to note that 110 is equal to the area under the N( r) spectrum, whilst it is equal to the first moment of the H( r) spectrum.
3.5 Oscillatory shear It is instructive to discuss the response of viscoelastic materials to a smallamplitude oscillatory shear, since this is a popular deformation mode for investigating linear viscoelastic behaviour. Let
yet') = Yo exp(iwt'),
(3.25)
where i = Ff, w is the frequency and Yo is a strain amplitude which is small enough for the linearity constraint to be satisfied. The corresponding strain rate is given by
yet') = iwyo exp(iwt'), and, if this is substituted into the general integral equation (3.21), we obtain a (t) = iwyo exp(iwt) ~oo cf> (~) exp( 
iw~) d~.
(3.26)
In oscillatory shear we define a 'complex shear modulus' G *, through the equation
aCt) = G*(w)y(t)
(3.27)
and, from eqns. (3.25), (3.26) and (3.27), we see that
G*(w)
=
iw ~oocf>(~) exp( iw~)
d~.
(3.28)
It is customary to write G*
=
G' + iG"
(3.29)
3.5]
Oscillatory shear
47
and G' and G" are referred to as the 'storage modulus' and 'loss modulus', respectively. G' is also called the dynamic rigidity. If we now consider, for the purpose of illustration, the special case of the Maxwell model given by eqn. (3.9) or eqn. (3.14) (with 7"M = 7") we can show that G*=
lWTJ
,
1 + iW7"
or alternatively
G*
=
iW7"G , 1 + iW7"
(3.30)
and
(3.31) G" =
TJW2 2' l+w7"
or alternatively
(3.32)
To some readers, the use of the complex quantity exp(iwt) to represent oscillatory motion may be unfamiliar. The alternative procedure is to use the more obvious waveforms represented by the sine and cosine functions, and we now illustrate the procedure for the simple Maxwell model. Let
(3.33)
Y = Yo coswt.
Thus, the strain rate is
y = YoW sinwt,
(3.34)
and if this is substituted into the equation for the Maxwell model, a first order linear differential equation is obtained, with solution a
=
TJWYo
.
2( W7" coswt  smwt). (1 + W 27" )
(3.35)
The part of the stress in phase with the applied strain is obtained by putting sinwt equal to zero and is written G' y. The part of the stress which is out of phase with the applied strain is obtained by setting coswt equal to zero and is written (G" / w) y. Hence
(3.36) (3.37) in agreement with (3.31) and (3.32) as expected.
Linear viscoelasticity
48
[Chap. 3
Returning now to the more convenient complex representation of the oscillatory motion, we remark that as an alternative to the complex shear modulus, we can define 'complex viscosity' 1]*, as the ratio of the shear stress a to the rate of shear y. Thus
oCt) =1]* yet),
(3.38)
and it follows that, for the general integral representation, 1]*(W) =
~oo</>(~)
exp( iw~)
d~.
(3.39)
We now write
(3.40) noting that 1]' is usually given the name 'dynamic viscosity'. The parameter 1]" has no special name but it is related to the dynamic rigidity through G' = 1]"w. It is also easy to deduce that G" = 1]'w. It is conventional to plot results of oscillatory tests in terms of the dynamic viscosity 1]' and the dynamic rigidity G'. Figure 3.8 shows plots of the normalized dynamic functions of the Maxwell model as functions of w 'T, the normalized, or reduced, frequency. The notable features are the considerable fall in normalized 1]' and the comparable rise in normalized G' which occur together over a relatively narrow range of frequency centred on W'T = 1. The changes in these functions are virtually complete in two decades of frequency. These two decades mark the viscoelastic zone. Also, in the many decades of frequency that are, in principle, accessible on the low frequency side of the relaxation region, the model displays a viscous response (G'  0). In contrast, at high frequencies, the response is elastic (1]'  0). From Fig. 3.8, the significance of 'T as a characteristic natural time for the Maxwell model is clear. }路o
G/G
}路o
0 log WT
Fig. 3.8 The Maxwell model in oscillatory shear. Variation of the normalized moduli and viscosity with normalized frequency (T = 1JIG).
3.5]
Oscillatory shear
49
In the literature, other methods of characterizing linear viscoelastic behaviour are to be found. For example, it is possible to define a 'complex shear compliance' J *. By definition (3.41)
yet) =J*(w)o(t)
in an oscillatory shear, with (3.42)
J*=J'iJ".
It is important to note that, although J * = I/G *, the components are not similarly related. Thus J' =1= I/G' and J" =1= I/G".
The second alternative method of characterizing linear viscoelastic response is to plot G' and the 'loss angle' 8. In this method, it is assumed that for an applied oscillatory strain given by eqn. (3.25), the stress will have a similar form, but its phase will be in advance of the strain by an angle 8. Then, a ( t)
= 00
exp [i( wt + 8)] .
(3.43)
It is not difficult to show that tan 8 = G" I G' .
(3.44)
Figure 3.9 shows how 8 and G'IG (where G = 7"1J) vary with the normalized frequency for the Maxwell model. At high values of the frequency, the response, as already noted, is that of an elastic solid. In these conditions the stress is in phase with the applied strain. On the other hand, at very low frequencies, where the response is that of a viscous liquid, the stress is 90 0 ahead of the strain. The change from elastic to viscous behaviour takes place over about two decades of frequency. This latter observation has already been noted in connection with Fig. 3.8. In Fig. 3.10, we show the waveforms for the oscillatory inputs and outputs. Figure 3.10(a) represents an experiment in the viscoelastic region. Figure 3.10(b) represents very high and very low frequency behaviour where the angle 8 is 0 0 or 90 0 , respectively. JO 26/71:
o log
WT
Fig. 3.9 The Maxwell model in oscillatory shear. Variation of the normalized storage modulus and phase angle with normalized frequency.
Linear viscoelasticity
50
[Chap. 3
wt 21r
I
10
I I
I
I
(a)
f:~1 2n:
10 7/70
T
a/ao
05,.""
0
,
10
wt 21r 10
av
(b) Fig. 3.10 Waveforms for oscillatory strain input and stress output: (a) Solid line ( ) strain according to eqns. (3.25) and (3.33); dashed line (     ) stress in advance by angle 8, according to eqn. (3.43); (b) Solid line ( ) strain input and also stress output for elastic behaviour; dotted line ( ) stress output for viscous behaviour.
Note that although the stress is 90 0 in advance of the shear strain for the viscous liquid, it is in phase with the rate of shear. 3.6 Relationships between functions of linear viscoelasticity In previous sections we have introduced a number of different functions which can all be used to characterize linear viscoelastic behaviour. These range from complex moduli to relaxation function and spectra. They are not independent, of course, and we have already given mathematical relationships between some of the functions. For example, eqn. (3.28), which is fairly typical of the complexities involved, relates the complex shear modulus G * to the relaxation function cp. Equation (3.28) is an integral transform and the determination of cp from G * can be accomplished by inverting the transform. There is nothing sophisticated, therefore, in determining one viscoelastic function from another: although this is a statement "in principle", and much work has been carried out on the nontrivial problem of inverting transforms when experimental data are available only over a limited range of the variables (like frequency of oscillation). The general problem of determining one viscoelastic function from another was discussed in detail by Gross (1953) and practical methods are dealt with by, for example, Schwarzl and Struik (1967). Nowadays most experimental data from linear viscoelasticity experiments are presented in the form of graphs of components of the dynamic parameters (such as
3.7]
Methods of measurement
51
complex modulus) and are rarely transformed into the relaxation function or the relaxation spectrum.
3.7 Methods of measurement Two different types of method are available to determine linear viscoelastic behaviour: static and dynamic. Static tests involve the imposition of a step change in stress (or strain) and the observation of the subsequent development in time of the strain (or stress). Dynamic tests involve the application of a harmonically varying strain. In this section we shall be concerned with the main methods in the above classification. Attention will be focussed on the principles of the selected methods and none will be described in detail. The interested reader is referred to the detailed texts of Walters (1975) and Whorlow (1980) for further information. An important point to remember is that, whatever the method adopted, the experimenter must check that measurements are made in the linear range; otherwise the results will be dependent on experimental details and will not be unique to the material. The test for linearity is to check that the computed viscoelastic functions are independent of the magnitude of the stresses and strains applied. 3.7.1 Static methods The static methods are either 'creep' tests at constant stress or relaxation tests at constant strain (see Figs. 3.11 and 3.12). In theory, the input stress or strain, whether it is an increase or a decrease, is considered to be applied instantaneously. This cannot be true in practice, because of inertia in the loading and measuring systems and the delay in transmitting the signal across the test sample, determined by the speed of sound. As a general rule, the time required for the input signal to reach its steady value must be short compared to the time over which the ultimate varying output is to be recorded. This usually limits the methods to materials which have relaxation times of at least a few seconds. A technique for estimating whether apparatus inertia is influencing results is to deliberately change the inertia, by
o''~:'_
to
t,
Time. t
Fig. 3.11 Typical creep curve of strain '( plotted against time t. A constant stress was applied at t = to and removed at t = t l â€˘ The strain comprises three regions: instantaneous (0 to '(I); retardation ('(I to '(2); constant rate ('(2 to '(J). In linear behaviour the instantaneous strains on loading and unloading are equal and the ratio of stress to instantaneous strain is independent of stress; the constantrate strain ('(2 to '(J) is not recovered.
Linear viscoelasticity
52
t> G 2
[Chap. 3
Time. t
IIlOr~~+::=====~III CII
~
~
l
V)
Fig. 3.12 Typical relaxation curve of stress (1 plotted against time t. A constant strain was applied at = to and reversed at t = t 1â€˘ In linear behaviour the instantaneous changes of stress from 0 to (11 and (12 to (13 are equal and the ratio of instantaneous stress to strain is independent of strain. The incomplete relaxation at t = t 1 may indicate either that further relaxation would occur in a longer time, or, that the material at very low deformation behaves like a Hookean solid and a residual stress would persist indefinitely.
t
adding weights for example, and checking the effect on the derived viscoelastic functions. The basic apparatus for static tests is simple. Once the shape and means of holding the specimen have been decided upon, it is necessary to apply the input signal and measure, and record, the output. It is easier to measure strain, or deformation, than stress. Hence, creep tests have been much more common than relaxation tests. The geometry chosen for static tests depends largely on the material to be tested. For solidlike materials, it is usually not difficult to fashion a long slender specimen for a tensile or torsional experiment. Liquidlike material can be tested in simple shear with the concentriccylinder and cone andplate geometries and constantstress rheometers are commercially available for carrying out creep tests in simple shear. Plazek (1968) has carried out extensive experiments on the creep testing of polymers over wide ranges of time and temperature. 3.7.2 Dynamic methods: oscillatory strain The use of oscillatory methods increased considerably with the development of commercial rheogoniometers, and a further boost was given when equipment became available for processing the input and output signals to give inphase and outofphase components directly. With modern instruments it is now possible to display automatically the components of the modulus as functions of frequency. A general advantage of oscillatory tests is that a single instrument can cover a very wide frequency range. This is important if the material has a broad spectrum of relaxation times. Typically, the frequency range is from 10 3 to 10 3 Sl. Hence a time spectrum from about 10 3 to 10 3 s can be covered. If it is desired to extend the limit to longer times, static tests of longer duration than 3 hr (10 4 s) would be
3.7]
Methods of measurement
53
r;F==~O Output transducer
Fig. 3.13 Representation of the coneandplate apparatus for oscillatory tests. The specimen is positioned between the input motion and the output stress.
needed. The lower relaxation time limit of oscillatory methods can be extended by wavepropagation methods (see Â§ 3.7.3). The conventional oscillatory methods involve the application of either free or forced oscillatory strains in conventional tensile and shear geometries. An advantage possessed by the free vibration technique is that an oscillator is not required and the equipment can be fairly simple. On the other hand, the frequency range available is no more than two decades. The reason for this is that a change of frequency relies on a change in moment of inertia of the vibrating system and the scope for this is limited. The method is readily adaptable to torsional deformation with solidlike materials. The wide frequency range quoted above is achieved with forced oscillations. We show in Fig. 3.13 the most common example of the forcedoscillation experiment, although the geometry could equally well be a parallelplate or concentriccylinder configuration. The test material is contained between a cone and plate, with the angle between the cone and plate being small ÂŤ 4 0). The bottom member undergoes forced harmonic oscillations about its axis and this motion is transmitted through the test material to the top member, the motion of which is constrained by a torsion bar. The relevant measurements are the amplitude ratio of the motions of the two members and the associated phase lag. From this information it is relatively simple to determine the dynamic viscosity TI' and the dynamic rigidity G', measured as functions of the imposed frequency (see Walters 1975 for the details of this and related techniques).
3.7.3 Dynamic methods: wave propagation A number of books are available which describe in detail the theory and practice of wavepropagation techniques. Kolsky (1963) has dealt with the testing of solids, Ferry (1980) has reviewed the situation as regards polymers and Harrison (1976) has covered liquids. The overall topic is usefully summarized by Whorlow (1980).
Linear viscoelasticity
54
[Chap. 3
Basically, the waves are generated at a surface of the specimen which is in contact with the wave generator and the evaluation of the viscoelastic functions requires the measurement of the velocity and the attenuation through the specimen. One significant advantage of wavepropagation methods is that they can be adapted to high frequency studies: they have been commonly used in the kHz region and higher, even up to a few hundred GHz. This is invaluable when studying liquids which behave in a Newtonian manner in other types of rheometer. Such liquids include, as a general rule, those with a molecular weight below 10 3 . They include most of the nonpolymeric liquids. Barlow and Lamb have made significant contributions in this area (see, for example, Barlow et al. 1967). 3. 7.4 Dynamic methods: steady flow In the oscillatory experiments discussed above, instrument members are made to oscillate and the flow is in every sense unsteady. A relatively new group of instruments for measuring viscoelastic behaviour is based on a different principle. The flow in these rheometers is steady in the sense that the velocity at a fixed point in the apparatus is unchanging. (Such a flow is described in fluid dynamics as being "steady in an Eulerian sense".) However, the rheometer geometry is constructed in such a way that individual fluid elements undergo an oscillatory shear (so that the flow is "unsteady in a Lagrangian sense"). A typical example of such an instrument is the Maxwell orthogonal rheometer which is shown in Fig. 3.14 (Maxwell and Chartoff 1965). It comprises two parallel circular plates separated by a distance h, mounted on parallel axes, separated by a small distance d. One spindle is rotated at constant angular velocity D. The other is free to rotate and takes up a velocity close to that of the first spindle. The components of the force on one of the plates are measured using suitable transducers. In the interpretation of the data it is assumed that the angular velocity of the second spindle is also D. It can then be readily deduced that individual fluid elements are exposed to a sinusoidal shear and that the components of the force on each plate (in the plane of the plates) can be directly related to the dynamic viscosity and dynamic rigidity. The Maxwell orthogonal rheometer and other examples of the steadyflow viscoelastic rheometers are discussed in detail by Walters (1975).
I h
1
Fig. 3.14 Arrangement of rotating plates in a Maxwell orthogonal rheometer. Plate separation h; axis displacement d. One spindle rotates at constant velocity Q and the second spindle takes up (nearly) the same velocity.
CHAPTER 4
NORMAL STRESSES
4.1 The nature and origin of normal stresses We have already stated in §1.5 that, for a steady simple shear flow given by (4.1) the relevant stress distribution for nonNewtonian liquids can be expressed in the form O'xy
i'1J( i'), O'yy = N} ( i' ),
= 0' =
O'xx 
O'xz
=
O'yy 
O'yz
=
O'zz
0,
}
(4.2)
= N2 ( i' ).
The variables 0', N} and N 2 are sometimes called the viscometric functions. A useful discussion of the importance of these functions is given by Lodge (1974, p. 212). In this chapter, we shall be concerned with the normal stress differences N} and N 2 or, equivalently, the socalled normal stress coefficients '1'} and '1'2' where
(4.3) In principle, it is possible for a nonNewtonian inelastic model liquid to exhibit normalstress effects in a steady simple shear flow. The so called ReinerRivlin fluid, which is a general mathematical model for an inelastic fluid (see §8.4), can be used to demonstrate this. However, all the available experimental evidence is that the theoretical normal stress distribution predicted by this model, viz. N} = 0, N 2 =i= is not observed in any known nonNewtonian liquid. In practice, normalstress behaviour is always that to be expected from models of viscoelasticity, whether they be mathematical or physical models. The normal stress differences are associated with nonlinear effects (cf. §1.3). Thus, they did not appear explicitly in the account of linear viscoelasticity in Chapter 3. In the experimental conditions of smallamplitude oscillatory shear, in which linear viscoelasticity is demonstrated and the parameters measured, the three normal stress components have the same value. They are equal to the ambient pressure, which is isotropic. Similarly, in steady flow conditions, provided the flow is slow enough for secondorder terms in i' to be negligible, the normal stresses are
°
55
Normal stresses
56
[Chap. 4
again equal to the ambient pressure. As the shear rate is increased, the normal stress differences first appear as secondorder effects, so that we can write
N2 =
2
+ o( y4),} B 2y 2 + o( y4),
NI = A 2 y
(4.4)
where A 2 and B 2 are constants and, as implied, the normal stress differences are even functions of the shear rate y. (The mathematicallyminded reader may confirm this expectation by undertaking a simple analysis for the hierarchy equations given in Chapter 8 (eqns. 8.238.25), which are argued to be generally valid constitutive equations for sufficiently slow flow). From a physical point of view, the generation of unequal normal stress components, and hence nonzero values of N I and N 2 , arises from the fact that in a flow process the microstructure of the liquid becomes anisotropic. For instance, in a dilute polymeric system, the chain molecules, which at rest occupy an enveloping volume of approximately spherical shape, deform to an ellipsoidal shape in a flow field. The molecular envelope before and during deformation is shown in Fig. 4.1. The droplets in an emulsion change shape in a similar way. In the polymeric system at rest, entropic forces determine the spherical shape whilst the requirement of a minimum interfacial freeenergy between an emulsion droplet and the surrounding liquid ensures practically spherical droplets in the emulsion at rest. It follows therefore that restoring forces are generated in these deformed microstructures and, since the structures are anisotropic, the forces are anisotropic. The spherical structural units deform into ellipsoids which have their major axes tilted towards the direction of flow. Thus the restoring force is greater in this direction than in the two orthogonal directions. The restoring forces give rise to the normal stress components of eqns. 4.2. It can be appreciated, from this viewpoint of their origin, why it is that the largest of the three normal stress components is always observed to be (Jxx' the component in the direction of flow. According to the principles of continuum mechanics, the components can have any value, but it would be an unusual microstructure that gave rise to components whose relative magnitudes did not conform to N I ?: 0, i.e. (Jxx?: (JyY' It is conceivable that a stronglyorientated reststructure, as found in liquid crystals, might produce such unusual behaviour in certain circumstances.

AT REST

UNDER SHEAR
Fig. 4.1 The molecular envelope before and during shear deformation.
4.2]
Typical behaviour of N1 and N}
57
10 2 .            .            r          , 1 03 1% POLYACRYLAMIDE SOLN.
0
Q.
"
<:..Q)"
u
~ .... Q)
0
Q.
"b
::::
lI)
10 2
~ 10' .... ...... lI)
....
1:i lI)
~ ......
lI)
0
o
N,
Q)
.c:
~
V)
o
c:
...... ~
100 '
'
100
10'
:'10' ~ 10 3
1.:
10 2
Shear ra te, ; /
5"
Fig. 4.2 Viscometric data for a 1% aqueous solution of polyacrylamide (E1O grade). 20 0 C. Note that, over the shearrate range 10 2 to 10 3 S I, N1 is about ten times larger than 0. 10' r..,10 5
x
POLYMER MEL T
o
Q.
"b lI)"
~ ......
â€˘
103
lI)
.... oQ)
6i
o ~ o c:
a
N,
10 2 '   : :             '   :  10' 100 Shear ra te,
J 10 3
10'
i /5"
Fig. 4.3 Viscometric data for a polypropylene copolymer. 230 0 C. Note that, over the shearrate range 10 0 to 10 1 S  1, N 1 is comparable in magnitude with o.
4.2 Typical behaviour of N 1 and N 2
In view of the discussion in the previous section of the thermodynamic origin of the normal stresses, we expect N1 to be a positive function of shear rate 1'. All reliable experimental data for elastic liquids are in conformity with this and show positive values of N1 for all shear rates. Figures 4.2 and 4.3 show typical examples for a polymer solution and polymer melt, respectively. Note that N1 may have a
Normal stresses
58
[Chap. 4
3
10 r     ,          .     r _   , D2 RHEOGONIOMETER DATA
~
•
'
0
<E"
6
<b
•
g /02
20·C 30·C 40·C 50·C
~
~l:J
/00'_":
/0'
L:
...J
/0)
Shear stress. a/Po
Fig. 4.4 A plot of In N) against In a at various temperatures for the polymer solution D2, which is a 10% wjv solution of polyisobutylene (Oppanol B50) in dekalin (cf. Lodge et al. 1987).
powerlaw behaviour over a range of shear rates, and we could write (cf. the related discussion concerning the shear stress CJ in §2.3.2)
(4.5) where A and m are constants, with m being typically in the range 1 < m ~ 2. As with the shear stress, the powerlaw region cannot extend to very low shear rates (unless m = 2). It is clear from Fig. 4.2 that the normal stress difference N1 , in this case, is higher than the shear stress CJ and such an observation is not unusual. The ratio of N1 to CJ is often taken as a measure of how elastic a liquid is; specifically N1 /(2CJ) is used and is called the recoverable shear. It follows that recoverable shears greater than 0.5 are not uncommon in polymeric systems. They indicate a 'highly elastic' state. For polymeric systems, it is often found that a plot of In N1 against In CJ for a range of temperatures results in a unique relationship which is a reasonably straight line of slope near 2 (see also §6.10 and Fig. 6.12). Figure 4.4 gives an illustration of such behaviour for a polymer solution. A straight line of slope 2 is expected at low shear rates in the socalled secondorder region but there is no fundamental justification for the line to be independent of temperature. Nor is there any fundamental justification for this unique relationship to apply, as it often does, outside the secondorder regime. It is generally conceded that the second normal stress difference N 2 is small in
4.2]
Typical behaviour of N, and N}
59
BOGERFLUlD
3000
&
2000
"
VI VI
~
Vi
!OOO
a
N]
olI;;J~C
TOo
~~~
TO' Shear ra fe. ; /
5 1
Fig. 4.5 Viscometric data for a Boger fluid: 0.184% polyisobutylene in a mixture of kerosene and polybutene (B.P. Hyvis 30). 25 0 C.
comparison to N1 • Indeed, for a socalled Boger fluid *, the second normal stress difference has been found to be virtually zero (see, for example, Fig. 4.5 and Keentok et al. 1980). We also remark that in the early days of normal stress measurement (c.1950) N 2 = was known as the Weissenberg hypothesis, and, within the limitations of the firstgeneration rheometers, experimental results on a number of systems were found to be in reasonable agreement with the hypothesis; the first such test being made by Roberts (1953) with a prototype version of the Weissenberg rheogoniometer. It is also noteworthy that some of the simpler microrheological models for polymeric systems predict N 2 = (d. Chapter 6). With N1 > 0, N 2 = 0, we note that the resulting normal stress distribution is equivalent to an extra tension along the streamlines, with an isotropic state of stress in planes normal to the streamlines. Modem rheometers are capable of determining N 2 with a reasonable degree of precision, although the level of tolerance is not as high as that associated with the determination of (] and N1 • Nonzero values of N 2 can now be detected and measured in many systems, but the ratio of I N 2 I to N1 is usually small (~0.1). Present reliable data on polymeric systems all show N 2 to be zero or negative: Fig. 4.6 shows the viscometric functions for a 2% solution of polyisobutylene in decalin (the socalled D1Iiquid). A comprehensive" roundrobin" series of experiments was carried out on D1 and the findings are given by Walters (1983) and Alvarez et al. (1985). In this roundrobin work, different types of instrument were used as well as different observers. The excellent agreement between the results shows that with
°
°
* A Boger (1977(a» fluid is a very dilute solution (  0.1 %) of a high molecularweight polymer in a very viscous solvent. Although the solution does, in fact, display shearthinning, the fall in viscosity is very small compared to the zeroshear value, and for practical purposes the viscosity appears to be constant (see also §7.2),
Normal stresses
60 1000
[Chap. 4
N,
Dl
500
500 10'
10 2 Shear ra te, ; /
s,
Fig. 4.6 Viscometric data for the polymer solution Dl, which is a 2% wjv polyisobutylene (Oppanol B200) solution in dekalin. 25Â°C (d. Alvarez et al. 1985).
modem instruments it is possible to obtain consistency and accuracy m the measurement of normal stress components.
4.3 Observable consequences of N 1 and N 2 Normal stresses are responsible for a number of effects of laboratory interest and of commercial importance. Those included here by way of examples are observable with the aid of relatively simple equipment. Perhaps the most well known and certainly the most dramatic effect is the rodclimbing phenomenon, usually referred to as the 'Weissenberg effect'. It is produced when a rotating rod is dipped into a squat vessel containing an elastic liquid. Whereas a Newtonian liquid would be forced towards the rim of the vessel by inertia, and would thus produce a free surface that is higher at the rim than near the rod, the elastic liquid produces a free surface that is much higher near the rod, as shown in Fig. 4.7. The observed rise of the surface is independent of the direction of rotation. The Weissenberg effect may be viewed as a direct consequence of the normal stress 0u' which acts like a hoop stress around the rod. This stress causes the liquid to "strangle" the rod and hence move along it. The reaction of the bottom of the vessel, which should not be sited too far from [he end of the rod, adds to the rise of the surface up the rod. If the geometry of the rodclimbing experiment is changed by adding a flat disc to the end of the rod and aligning the disc to be close to, and parallel with, the bottom of the vessel, we have the configuration of one of a set of instruments used for measuring N l and N 2 â€˘ Such instruments will be described later. Suffice it to say here that it can be shown that the strangulation caused by the first normal stress
4.3]
Observable consequences of N} and N}
61
Fig. 4.7 The Weissenberg effect shown by a solution of polyisobutylene (Oppanol B200) in polybutene (B.P. Hyvis 07). Reproduced by permission of Shell Research Ltd.
difference exerts a force between the bottom of the vessel and the disc, tending to push them apart. The measurement of this force can be used to yield normal stress information. If the rod is replaced by a tube, open at both ends and with the disc (with a hole in the middle) still in place, the Weissenberg effect causes the elastic liquid to flow up the tube (Fig. 4.8). Flow will continue until the normal force is balanced by the gravitational force, provided there is enough liquid in the vessel. This is the principle of the "normal force pump", which is probably more of a novelty than a practical means of dispensing highlyelastic liquids. Another phenomenon which can be reproduced with simple equipment, but yet has important consequences in manufacturing processes, is 'die swell', sometimes
Normal stresses
62
[Chap. 4
    '"/C
   
 

~
c
~
.
•• • b..
Fig. 4.8 The normalforce pump.
known as postextrusion swelling. When an elastic liquid is extruded from a die or flows from the exit of a tube, it usually swells to a much greater diameter than that of the hole, as shown in Fig. 4.9. In fact, Newtonian liquids can also show die swell, but only at low rates of flow (with about a 13% swelling at negligibly small Reynolds numbers), and as the flow rate increases the swelling decreases, eventually becoming a contraction. In contrast, die swell of an elastic liquid increases as the
Fig. 4.9 Die swell shown by a solution of 1% polyacrylamide in a 50/50 mixture of glycerol and water.
4.3]
Observable consequences of N} and N}
63
flow rate increases. A swelling of up to two or three times the hole diameter is not unusual. A convenient way of visualizing the origin of die swell is to consider the elastic liquid flowing towards the orifice as a bundle of elastic threads stretched by the CTxx normal stress component and when they emerge they are free to relax. The relaxation causes the threads to shorten in length, hence the bundle increases in diameter. An important commercial process which is affected by die swell is the manufacture of rods, tubes and sheets of polymeric material. These articles are made by extrusion of molten polymer, which is an elastic liquid. Die swell causes problems in the control of the final thickness of the articles. The phenomenon is sensitive to the molecularweight distribution of the polymer and such processing variables as flow rate and temperature. Increasing the length of the entry to the nozzle and reducing the angle of convergence to it are practical ways of reducing swelling, although at the expense of an increased pressure drop. However, die swell cannot be completely suppressed, so the satisfactory manufacture of a uniform product requires close control of the conditions. Finally, we should mention that the measurement of the equilibrium amount of die swell produced under fully~controlled experimental conditions forms the basis of another method of measuring normal stress differences. There is a close link between this method and the method known as jetthrust. In the latter, the force exerted by the emerging jet (of a necessarily mobile liquid), either directly onto an intercepting transducer or as a reaction on the flow tube, is related to the die swell and therefore also to normal stress levels (see, for example, Davies et aI., 1975, 1977). Normal stress effects are also important in those laminar mixing processes which involve disc impellers and may occur to some extent with other types. The flow pattern for a relatively inelastic liquid results from the interaction between viscous and inertial forces and comprises a radial outflow from the central impeller and return flows distant from the impeller as shown in Fig. 4.10. However, for a highly elastic liquid, the direction of flow can be completely reversed. There are intermediate cases when both types of flow pattern coexist. In this situation, the flow pattern characteristic of the elastic liquid and generated by the normal stresses hugs the impeller whilst the inelasticliquid pattern is found in regions remote from the impeller. Examples are given in Fig. 4.10. Obviously, liquid contained in the one pattern will not mix very well with liquid in the other. Which type of flow pattern is obtained in a given situation depends on the ratio of the elastic forces to the inertial forces. This ratio is a dimensionless group which is given by the ratio of the Weissenberg number to the Reynolds number (~/Re) *. The dual flow pattern is to be found at intermediate values of this ratio.
*
The 'Weissenberg number' We may be defined as the ratio of the first normal stress difference to the shear stress in a steady simple shear flow.
Normal stresses
64
cr" ~
Newtonion
~
(~
~,
(
[Chap. 4
J "
,
c_ r<~ ~
Mixed
()()
( )( )
( )( )( )( ) c""" ~
~
/ \
Elostic dominoted
~\ (.J
(
.J". "\
Fig. 4.10 Normalstress effects in mixing; showing how the form and direction of the circulation are affected by increasing elasticity.
Although the second normal stress difference N2 is generally of far less practical significance than the first normal stress difference N}> it is important to point out that in some situations N 2 is very important. For example, it is the function N 2 (y) which determines whether or not rectilinear flow in a pipe of noncircular cross section is possible (see, for example, Townsend et al. 1976). A related problem is wire coating, and the importance of N2 in this practical problem has been stressed by Tadmor and Bird (1974). Such examples of the importance of N2 are rare and apart from those who are directly concerned with the situations cited, most practitioners in nonNewtonian fluid mechanics tend to confine attention to N1 , especially in view of the relative difficulty of measuring N2 â€˘ 4.4 Methods of measuring N 1 and N 2
As a generality, the ideal method of measuring normal stress differences would involve an uncomplicated shear geometry, which could be easily made, be amenable to an exact mathematical analysis, and would enable the normal stress differences to be measured separately from shear and inertial forces. It is not possible to achieve the ideal, but the methods outlined below are the nearest to it.
4.4]
Methods of measuring N j and N;
65
We have already stated that N1 is large in comparison to N2 and that the latter is the more difficult to measure. For these reasons, it is customary to give greater emphasis to methods for N1 determination, and, in routine laboratory work, to confine measurements to N1 . The simplest flow is that shown in Fig. 1.1. in connection with Newton's postulate. It can be generated by sliding two parallel plates over each other ('plane Couette flow'). There has been a limited number of attempts to use this method, but it has practical limitations. Mobile liquids may run out of the gap, and it is impossible to maintain a continuous shear for very long; hence the method is restricted to extremely viscous liquids or (for lessviscous liquids) to very narrow gaps, hence high shear rates. In this form of the parallelplate apparatus, Dealy (see, for example Dealy and Giacomin 1988) uses flow birefringence as the means of measuring normal stress and he inserts a flushmounted transducer into the surface of one plate to measure the shear stress, free from edge effects. In view of the limitations of apparatus constructed for generating the primitive simple shear, it is not surprising that a detailed search has taken place for flows which are equivalent to steady simpleshear flow in a welldefined mathematical sense. These 'viscometric flows' include 'Poiseuille flow' (i.e. steady flow under a constant pressure gradient in a pipe of circular cross section), 'circular Couette flow' (i.e. steady flow between coaxial cylinders in relative rotation), torsional flow (i.e. steady flow between parallel plates, one of which rotates about a normal axis) and the corresponding coneandplate flow, which will figure prominently in the following discussion. This list is not meant to be exhaustive and the reader is referred to Walters (1975), Dealy (1982) and Lodge (1974) for other examples and greater detail. The proof that all these flows are equivalent to steady simpleshear flow (with the stress distribution expressible in terms of (1, N1 and N 2 ) is nontrivial and has been approached from different standpoints by Lodge (1974), Coleman et aI. (1966), Bird et al. (1987(a) and (bÂť and Walters (1975). 4.4.1 Coneandp/ate flow It is probably true to say that the coneandplate geometry is the most popular for determining the normal stress differences. The basic geometry is shown schematically in Fig. 4.11 (see also Chapter 2). The test liquid is contained between a
Fig. 4.11 Basic geometry for coneandplate flow.
Normal stresses
66
[Chap. 4
rotating cone and a flat stationary plate. (Alternatively the plate is designed to rotate with the cone stationary, with a small advantage as regards alignment). With respect to suitably chosen spherical polar coordinates, the physical components of the velocity vector at any point in the liquid are assumed to be (see Fig. 4.11) V(r) =
0,
V(8) =
0,
VCl() =
r sin8 .Q( 8),
(4.6)
with the boundary conditions that the angular velocity is zero at the plate surface and .Q1 at the surface of the cone, i.e.
(4.7) where 80 is the gap angle. It can be shown that the flow represented by eqn (4.6) is equivalent to a steady simpleshear flow with shear rate y = sin8 d.Q/d8, and that, when the stress equations of motion are taken into account, we obtain for the shear stress (J (see, for example, Walters 1975, Chapter 4): (4.8) and, for the normal stress differences, 2
. 2
d.Q
2pr sm 8 .Q d8
=
d [N (Y .) d8 1
+ 2N2 ( Y. )] ,
(4.9)
where p is the density and A is a constant to be determined from the boundary conditions. Equations (4.8) and (4.9) are in general incompatible (in the sense that a solution to (4.8) will not be a solution to (4.9) and vice versa), unless we make the following assumptions: (i) inertial effects are negligible, which means setting p
=
0 in (4.9);
(ii) the angle between the cone and the plate is small enough to allow us to set
cosec 2 8 = 1 in (4.8), which in practical terms means restricting the gap angle 80 to be no greater than 4 0 â€˘ With assumptions (i) and (ii), we have (4.10) i.e. there is a constant shear rate throughout the sample and it is independent of the form of the viscometric functions. Equations (4.8) and (4.9) are now compatible. It is easy to show that the torque C acting on the stationary plate of radius a is given by (cf. Chapter 2) C=
27Ta 3 3(J( y),
(4.11)
4.4]
Methods of measuring NJ and N}
67
and that if p is the pressure on the plate at a radius r, in excess of that due to atmospheric pressure, then (4.12) i.e. there is a logarithmic dependence of p on r and the slope of the (p, In r) curve can be used to yield N} ( y) + 2 N2 ( Y). Further, if the pressure is integrated over the plate, we obtain the total normal force F on the plate and it can then be shown that (Walters 1975, Chapter 4) (4.13) This force acts in the direction of the axis of rotation and pushes the cone and plate apart. It is essentially the same force that produces the Weissenberg rodclimbing effect. The above analysis tells us that the measurement of the rotational speed will give the shear rate and that measurement of the torque on the stationary plate will give the shear stress. As regards the normal stress differences, there are two alternatives. First, the force F gives N}; secondly the radial distribution of pressure gives N} + 2N2 â€˘ Hence, in principle, the two normal stress differences can be obtained if these two alternatives are both used. There is a basic conflict in the normal force measurement, since the force F tends to separate the cone from the plate. The consequence of such a separation, if it were allowed, is to upset the condition of uniform shear rate throughout the sample and to reduce the mean value of shear rate. The ideal measuring system should be rigid to axial forces. For systems which are not rigid, a servomechanism is used to maintain the coneplate gap. Various potential sources of error have to be borne in mind when performing experiments in the coneandplate geometry. The more important are enumerated below and we refer the reader to the texts of Walters (1975) and Whorlow (1980) for further details.
I Inertial effect The origin and nature of the effect of inertia has already been mentioned. It gives rise to the socalled "negative normal stress effect", whereby the plates are pulled together and the measured value of the force F is smaller than the true value. The reduction in the force F is given by (Walters 1975) (4.14) This formula is used to correct experimental values: it can be seen that it is sensitive to the rotational speed and very sensitive to the plate radius.
68
Normal stresses
[Chap. 4
II Holepressure error A major source of error which can arise when the pressuredistribution method is used is known as the holepressure error (Broadbent et al. 1968). Any method of measuring pressure which relies on the use of a hole in the bounding surface gives a low result with elastic liquids owing to the stretching of the flow lines as they pass over the hole. The reduction is directly related to N1 and is in fact used as a means of measuring N1 â€˘ This method is described later in this chapter, where a more detailed description is given. The error is avoided by the use of stiff, flushmounted pressure transducers. II I Edge effects "Shear fracture" places an upper limit on the usable shear rate range for highly elastic materials like polymer melts. It is observed as a sharp drop in all stress components, and at the same time a change in shape of the free surface can be seen, as well as a rolling motion in the excess liquid around the rim of the plates. A horizontal free surface forms in the test sample at the rim and grows towards the centre, hence reducing the sheared area. The limiting shear rate can be quite low, depending on the liquid and the cone dimensions. Expressed as a critical normal stress N1(c), the limit is given by
(4.15) where c is a constant of the liquid. For a given liquid, shear fracture is minimized if the cone radius and gap angle are small. The name "shear fracture" was given to the effect by Hutton (1965) owing to its similarity t.o 'melt fracture', which limits the occurrence of steady flow of polymer melts in tubes. Tordella (1956) made the first systematic study of melt fracture and noted that when the effect is severe the stream of melt breaks up with an accompanying tearing noise. Another edge effect, also pointed out by Hutton (1972) is ascribable to changes in contact angle and/or surface tension of the test liquid brought about by shear. The effect is of potential importance when the test liquid possesses only small normal stresses. IV Miscellaneous precautions The alignment of the cone axis to be coincident with the rotational axis, the setting of the cone tip in the surface of the plate, and the minimizing of, or correction for, viscous heating are other important matters to be taken into account in accurate work. 4.4.2 Torsional flow Torsional flow is shown schematically in Fig. 4.12 (see also Chapter 2). Clearly, commercial instruments which are designed to work in a coneandplate mode can be easily adapted to the parallelplate geometry and vice versa.
4.4]
Methods o/measuring NJ and N 2
69
Statianary plate
Fluid
4 ,.
h
I I
t
I
'T'
Fig. 4.12 Basic geometry for torsional flow.
In this case, with respect to suitably defined cylindrical polar coordinates, the velocity distribution can be taken to be V(r)
= 0,
V(8)
= rw (z),
V(z) =
(4.16)
0,
subject to the boundary conditions at the two plates
w(O)=O,
w(h)=.Q],
(4.17)
where h is the gap between the plates. Taking into account the fact that eqn. (4.16) is equivalent to a steady simpleshear flow, the stress equations of motion are satisfied, with the shear rate given by (4.18) provided
dw
2pr dz
=
(4.19)
O.
Equation (4.18) implies that the shear rate is independent of the viscometric functions: it depends on radial distance r, but is constant across the gap for fixed r. This time, we see from eqn. (4.19) that we have to neglect inertia for compatibility and there is no essential restriction on the gap h, except of course that this must not be too large that edge effects in a practical rheometer become important. The edge effects mentioned in connection with the coneandplate instrument apply here. After some routine mathematics, it is possible to show that the viscosity function can be determined from measurements of the torque C through the equation (d. Chapter 2): 11(YJ=2
3C ( 1 din C) 3路 1+3dlny , 7Ta Ya a
where Ya is the shear rate at the rim (r (N]  N2 ) 1'1 a
2F (1 + 21 ddinI F) . ,
= 2
7Ta
n Ya
(4.20) = a).
It can also be shown that (4.21)
Normal stresses
70
[Chap. 4
where F is again the total normal force on the plates. We see that totalforce data yield the combination N 1  N2 at the shear rate Ya at the rim. Clearly, total force measurements taken in the coneandplate and parallelplate geometries can be combined to yield N 1 and N2 separately. However, since N2 is small and two separate experiments have to be performed, significant scatter in the final data can be anticipated unless there is very refined experimentation. Of interest is the fact that, in principle, relatively high shear rates can be attained with small gaps h. This has been utilized in the socalled "torsional balance rheometer" of Binding and Walters (1976) to obtain normal stress data at shear rates in excess of 10 4 s 1. In this form of the instrument, a predetermined external normal force is applied to the upper plate and the separation h is allowed to vary until this force balances the normal force generated by the liquid. Gap h is measured and eqns. (4.20) and (4.21) applied. 4.4.3 Flow through capillaries and slits
A consistent theory for normal stress measurement in flow through a capillary is available (cf. Walters 1975, Chapter 5), but this depends critically on the flow being "fully developed" at the exit to the capillary, by which we mean that the Poiseuille flow generated away from the influence of end effects should be maintained right up to the capillary exit with no rearrangement of the velocity profile. Furthermore, the experimental results have to be carried out with flushmounted pressure tranducers to avoid the holepressure error problem, and this is difficult on the curved walls of a capillary. Therefore, the use of the potentially attractive exitpressure measurement technique of determining normal stress data is controversial (cf. Boger and Denn 1980). The associated jetthrust technique for low viscosity elastic liquids and high shear rates is also based on the assumption of fully developed flow at the capillary exit (cf. Davies et al. 1975, 1977). In the Lodge (1988) stressmeter, which uses pressuredriven flow through a slit, the holepressure error mentioned above is turned to good use in the measurement of N 1 . As liquid flows past the hole under an applied pressure gradient, streamlines adjacent to the boundary wall are deviated into and then out of the hole, as shown in Fig. 4.13. For an elastic liquid the deviation is viewed as a stretching by the normal stress component acting along the streamlines. The net result is a lowering of the pressure in the hole. The holes in the stressmeter are a pair of slots set across the flow direction as shown in Fig. 4.13. The reduction in pressure J.p is measured TI
â€˘
"
,
. ~
11 T3
..
"
~
'11"


~
T2
Fig. 4.13 Schematic diagram of the Lodge stressmeter for normal stress and shear stress measurement. The dotted lines represent the tension in the streamlines resulting in a lowered pressure in the holes.
4.5]
Viscometric functions and linear viscoelastic functions
71
(as PI  P2) between the bottom of the hole beneath one of the slots and a flushmounted transducer whose diaphragm forms the boundary wall on the opposite side of the slit. The difference in pressure in the two slots (P2  P3) gives the shear stress. It has been shown theoretically that .1 P is given by (cf. Tanner and Pipkin 1969) (4.22) for a secondorder simplefluid model (which will be shown in ยง8.5 to be a valid slowflow approximation for a general class of elastic liquid). The generalization of eqn. (4.22) embodied in the so called HPBL equation is used to interpret results for flows which are certainly outside the "slowflow" regime. The interpretation of results is accordingly based on what must be seen as an empirical equation, with no theoretical justification except at low shear rates. However, it appears to work well, judged by recent comparative studies with other instruments (Lodge et al. 1987), and shear rates as high as 10 6 S1 have been reached with multigrade motor oils with this technique. 4.4.4 Other flows Tanner (1970) has proposed that the free surface shape in gravitydriven flow down an open tilted trough can be used to calculate the second normal stress difference N 2 โข In general terms, if the free surface rises near the centre, N 2 is negative and, if it falls, N2 is positive. The interpretation of data is not trivial, but the technique provides a convenient method of determining estimates of N 2 at low shear rates. Circular Couette flow between rotating cylinders is popular in the determination of the viscosity of nonNewtonian liquids (cf. ยง2.4). Attempts have also been made to employ the flow to determine normal stress information from pressure readings (Broadbent and Lodge 1972). The fact that the technique has not been popular with experimentalists since the original paper is probably an indication of the difficulty of using the technique, or it at least points to the fact that much easier methods are available in rotational rheometry using, for example, coneandplate flow.
4.5 Relationships between viscometric functions and linear viscoelastic functions Earlier in this chapter we argued that normal stress differences in a simpleshear flow were a direct consequence of viscoelasticity. We recall from ยง3.5 that viscoelasticity can also be studied through a smallamplitude oscillatoryshear flow, the resulting stress distribution for an elastic liquid being expressible in terms of the dynamic viscosity r/ and the dynamic rigidity G'. Now, since the departure from a Newtonian response in the viscometric functions 'TI, N 1 and N 2 and in the dynamic functions 'TI' and G' can be ascribed to viscoelasticity, we should not be surprised to find that there are relationships between the various rheometrical functions. In fact,
Normal stresses
72
[Chap. 4
lO'r, 01
6
6 6 6
0
6
I11*(W) I 11 (;)
66 6 66 6 III 6% 6
6
&
6
~
...
6
000
0
Q
0 0 0 0 0 0 0 0 0
I
I
10'
10
2
;/5' or w /5'
10
3
10
1
Fig. 4.14 The CoxMerz rule applied to the polymer solution D1, which is a 2% w/v polyisobutylene (Oppanol B2(0) solution in dekalin. 25 0 C.
it is not difficult to deduce the exact relationships in the lower limits of frequency and shear rate: (4.23) 
'1'1 ( y) 2
(4.24) y,O
The former relationship states that the viscosity measured in oscillatory shear in the zerofrequency limit is equal to the low shear viscosity measured in steady shear. Equation (4.24) is a relationship between the limiting values of dynamic rigidity and first normal stress difference. In many cases, it is easier to carry out dynamic measurements than steady shear measurements and (4.23) and (4.24) provide a means of estimating the levels of TI and '1'} (and hence N}) from measurements of TIl and G I. We note that in view of eqn. (4.23) and the fact that both TI and TIl are usually monotonic decreasing functions of y and w, respectively, various attempts have been made to develop empirical relationships between TI and TIl at other than the lower limits of shear rate and frequency. The most popular, and most successful in this respect, certainly for polymeric liquids, is the socalled CoxMerz (1958) rule, which proposes that TI should be the same function of y as I TI* I is of w, where I TI* I is the modulus of the complex viscosity, i.e. (4.25)
4.5]
Viscometric functions and linear viscoelastic functions
73
/00r, o
03 o o o o o
o
...o
'"
Ii}
~
t.. /02 ~
;E
o
o o
o
o o
Fig. 4.15 A test of the relationship of eqn. (4.24) showing the asymptotic approach of the oscillatory and steady shear parameters. Steady shear and dynamic data for the polymer solution D3, which is a 1.5% wIv polyisobutylene (Oppanol B2(0) solution in dekalin. 20 0 C.
In Fig. 4.14 we provide an example of the application of the CoxMerz rule to a polymer solution. In view of (4.24) and the fact that both G' and N1 are monotonic increasing functions of wand y, respectively, we might be led to expect that a relationship analogous to the CoxMerz rule will hold between G' and N1 (see, for example, ยง6.10 and cf. AIHadithi et al. 1988). The limiting relationship (4.24) has been confirmed many times and Fig. 4.15 provides just one example of this for a polymeric liquid, where we see that the values of N1/2 y 2 and G' /w 2 coincide at low values of y and w.
CHAPTER 5
EXTENSIONAL VISCOSITY
5.1 Introduction
The subject of 'extensional' (or 'elongational') flow received scant attention until the mid 1960s. Up to that time rheology was dominated by shear flows. In the last twenty years or so the situation has changed dramatically with the dual realization that extensional flow is of significant relevance in many practical situations and that nonNewtonian elastic liquids often exhibit dramatically different extensional flow characteristics from Newtonian liquids. Accordingly, interest in the subject has mushroomed and much effort is now expended in trying to measure the extensional viscosity of nonNewtonian liquids, whether they be "stiff' systems like polymer melts or "mobile" systems like dilute polymer solutions, suspensions and emulsions. The general subject is covered in the book by Petrie (1979) entitled" Elongational Flows". Petrie's book requires more than a passing acquaintance with mathematics to be fully appreciated, but there is sufficient general detail in the book to make it important reading for anyone requiring a thorough knowledge of the subject. The works of Dealy (1982), Cogswell (1981), Meissner (1983, 1985), Mlinstedt and Laun (1981, 1986) are also important sources of information for those whose direct concern is polymer melts. Unlike the situation in steady simple shear and oscillatory shear (see Chapters 24) where the subjects are mature, the study of extensional flow is still evolving. This is reflected in the slightly different style of the present chapter. For the velocity field (see Fig. 5.1(a))
ux=i.x,
vy = i.y/2,
(5.1)
vz = iz/2,
where i is a constant extensional strain rate, the corresponding stress distribution can be conveniently written in the form On
=
0xy 
0yy _ 0xx 0xz 
=
0yz 
0zz
= iTlE ( E), }
(5.2)
O.
where TlE is the (uniaxial) extensional viscosity. In general, it is a function of the extensional strain rate i, just as the shear viscosity is a function of shear rate y (ยง2.3). However, we shall see that the behaviour of the extensional viscosity function 75
Extensional viscosity
76
(b)
(0) BIAXIAL EXTENSION
UNIAXIAL EXTENSION
[Chap. 5
olII~
(c) PLANAR EXTENSION
Fig. 5.1 The three different types of extensional flow fields are shown by the arrows: (a) Uniaxial; (b) Biaxial; (c) Planar.
is frequently qualitatively different from that of the shear viscosity. So, for example, highly elastic polymer solutions that possess a viscosity that decreases monotonically in shear (showing shearthinning) often exhibit an extensional viscosity that increases dramatically with strain rate. A fluid for which 'i1 E increases with increasing i. is said to be 'tension thickening', whilst, if 'i1E decreases with increasing i, it is said to be 'tensionthinning'. Experimentally, it is often not possible to reach the steady state implied in (5.1) and (5.2). Under these circumstances, it is convenient to define a transient extensional viscosity l1E(t, i), which is clearly a function of t as well as i. This arises from the obvious analogue to (5.2) given that the extensional flow field (5.1) is initiated at time t = 0 and maintained thereafter. In some respects this is a disappointing admission of difficulties which certainly do not normally occur in the measurement of the shear viscosity 'i1( Y). However, a study of l1E(t, i) can still throw considerable light on the rheological response of nonNewtonian liquids. It is also not without its industrial relevance, since in many practical situations liquids are exposed to extensional flow fields over a limited period of time only (see, for example, Bird et al. 1987(a) and Laun and Schuch 1988). Another type of extensional deformation is the socalled biaxial extension, given by (see Fig. 5.1(b))
v7
=
2iz ,
(5.3)
where i is a constant. This type of extension is equivalent to stretching a thin sheet of material in two orthogonal directions simultaneously, with a corresponding decrease in the sheet thickness. It is found (approximately) when a circular free jet impinges on a flat plate or in a lubricated squeezefilm flow (see, for example, Soskey and Winter 1985) and when a balloon is inflated. The stress field corresponding to (5.3) can be written in the form
(Ju
~ (Jxx
(Jxy 
_
(JX7 
(Ju
~ (Jyy =
(JY7 
0,

i'i1 EB ( i), }
(5.4)
5.2]
Importance of extensional flow
77
where l1EB is the biaxial extensional viscosity. It can be shown that (Walters 1975, p. 211) (5.5) Finally, a twodimensional planar extensional flow given by (see Fig. 5.1(c))
vz = i.z ,
(5.6)
where i. is a constant, yields a planar extensional viscosity l1Ep: (5.7) This type of extension is equivalent to stretching a thin flat sheet of material in one direction only (the x direction), with a corresponding contraction in its thickness in the z direction, but with no change in the width of the sheet. Planar extensional flow can be shown to be equivalent to that generally known as "pure shear" (see, for example, Walters 1975, Chapter 7). In the present book, our general concern will be the uniaxial extensional viscosity l1E and its comparison to the equivalent shear viscosity. Fuller details about subjects not enlarged on here are provided in the texts of Petrie (1979), Walters (1975), Tanner (1985) and Bird et al. (1987(a) and (b)).
5.2 Importance of extensional flow
In polymer processing (see ยง6.11.1), a case can be made out that some operations involve a significant component of extensional flow, with the obvious conclusion that the measurement of extensional viscosity may sometimes be as important as the determination of the shear viscosity. This will become increasingly so as manufacturers attempt to further increase production rates. Any reasonably abrupt change in geometry in a processing operation will generate a flow with an extensional component and, in particular, flows through a sudden contraction or out of an orifice often lead to flow characteristics which cannot be predicted on the basis of shear viscosity alone. The polymer engineer must, therefore, have a working knowledge of extensional flow and must, if possible, know whether the materials he is processing are tensionthinning or tensionthickening. Certainly, the' spinnability' of a polymeric liquid can be very dependent on its extensional viscosity behaviour. To illustrate this, consider the fibrespinning process shown schematically in Fig. 5.2. It is clearly important for the process, which is dominated by extensional flow, to be stable and for the threadline not to snap. The tension along the threadline is obviously chosen to prevent fracture under normal operating conditions and the main concern is with the propagation and magnification of small disturbances, which are to some extent unavoidable in a physical process of this sort.
Extensional viscosity
78
[Chap. 5
From the
spinnerette
/ /
/
......
To the
windup device Fig. 5.2 The filamentnecking imperfection in fibre spinning.
The stability of a spinning threadline is a vast area of study (see, for example, Petrie 1979) and we shall do no more than isolate one possible cause for concern. Let us speculate that for some reason a change in diameter occurs. From simple continuity considerations we would expect the narrower part of the filament to move faster than the rest of the threadline. Put in another way, the extensional strain rate will now be higher in the narrow part. If the polymeric liquid is tensionthinning, the resistance to extension is reduced in the narrow part and motion in this part of the threadline is further accelerated. It becomes thinner and may ultimately break. If, on the other hand, the polymeric liquid is tensionthickening, the resistance in the narrow part of the filament will now be increased. The flow in the filament will slow down, the radius will increase and may be expected to return to that of the remainder of the threadline. Tensionthickening is therefore a stabilizing influence in this process. Other examples of the importance of extensional viscosity in polymer processing could be cited. Certainly, the polymer engineer needs to be aware of the fact that two polymeric liquids which may have essentially the same behaviour in shear can show a different response in extension. Later in this chapter we shall see that there is sufficient theoretical and experimental evidence available to support the view that very dilute solutions of flexible polymers can have extremely high extensional viscosities. Certainly, these can be orders of magnitude higher than those expected on the basis of Newtonian theory. This has important consequences in a number of practically important situations. For example, it may significantly affect the pressure losses encountered in polymer flooding in "enhanced oil recovery" (EaR) (see ยง6.11.3). Further, it may be the cause of the phenomenon known as "drag reduction". When small concentrations
5.2]
Importance of extensional flow
79
Fig. 5.3 The 4roll mill experiment. Schematic representation of the fluid velocities for: (a) A Newtonian liquid; (b) A highly elastic liquid, for which high extensional stresses at A and B reduce the inflow.
(of the order of a few partspermillion) are added to a Newtonian solvent like water, there is often a substantial reduction in drag in turbulent flow (Tanner 1985, p. 423). Drag reduction is of potential importance in many spheres. For example, small quantities of polymer may be injected into sewers during heavy rain to upgrade flow and so prevent flooding. Many different mechanisms have been proposed to account for the phenomenon of drag reduction, but it may be linked to extensional viscosity and in particular to the suppression of the rollwave motion and vortex stretching in the sublayer by the high extensional viscosity. The potential importance of extensional viscosity effects in such processes as calendering and paper coating is suggested by the fourroll mill experiments discussed by Metzner and Metzner (1970) (see Fig. 5.3). When the fourroll mill is immersed in a Newtonian liquid, the expected flow regime shown in Fig. 5.3(a) is observed. However, in the case of some dilute polymer solutions, the flow shown in Fig. 5.3(b) more adequately reflects the observations. The flow at A and B is too" strong" to permit substantial amounts of fluid to enter as in Fig. 5.3(a). Specifically, the anticipated flow has a high extensional component which results in high extensional stresses. The shear stresses generated by the rotating rollers are not strong enough to overcome the large extensional stresses and a reversed flow results at A and B. Further examples of anomolous flow characteristics caused by high extensional viscosities are given in ยง5.6.
80
Extensional viscosity
[Chap. 5
Finally, we remark that extensional flow experiments can be viewed as providing critical tests of any proposed constitutive equations. Indeed, the historical convention of matching only shear flow data with theoretical predictions in constitutive modelling may have to be rethought in those areas of interest where there is a large extensional contribution. It may be more profitable to match any extensional viscosity data which may be available, even if this means that the resulting constitutive model loses some of its predictive value so far as shear data are concerned.
5.3 Theoretical considerations Continuum mechanics is able to provide some useful insights into the extensionalviscosity behaviour of nonNewtonian liquids. For example, the following limiting relations between extensional and shear viscosities are true (cf. Walters 1975, Petrie 1979) (5.8) (5.9) We note that these relationships are valid for all values of i. and y in the case of Newtonian liquids. In particular, for Newtonian liquids, (5.10) a result obtained by Trouton as early as 1906. Accordingly, rheologists have introduced the concept of the 'Trouton ratio' T R defined as (5.11) Elastic liquids are noted for having high Trouton ratios, but the definition as given in eqn. (5.11) is somewhat ambiguous, since it depends on both i and y, and some convention has therefore to be adopted to relate the strain rates in extension and shear. To remove this ambiguity and at the same time provide a convenient estimate of viscoelastic effects, Jones et al. (1987) have proposed the following definition, based on a simple analysis for an inelastic nonNewtonian fluid: (5.12) i.e., in the denominator, the shear viscosity is evaluated at the shear rate numerically equal to 13 i. Jones et al. show that if the fluid is inelastic and isotropic, T R is 3 for
5.3]
Theoretical considerations
81
all values of i. They argue that any departure from the value 3 can be associated unambiguously with viscoelasticity, so that the definition (5.12) not only removes the ambiguity in the definition of the Trouton ratio, but also provides a convenient means of estimating viscoelastic response. Variable (shear) viscosity effects are accommodated in the analysis of Jones et aL, which illustrates convincingly that a fluid that is shearthinning must also be expected to be tensionthinning in extension, if viscoelastic effects are negligible or very small. Continuum mechanics also supplies a limiting relationship between the extensional viscosity TI E and the normal stress coefficients '1'1 and '1'2 as determined in shear flow. A simple analysis for the socalled secondorder model (which is argued in ยง8.5 to provide a general description of nonNewtonian behaviour in sufficiently slow flow) leads to the following relation:
(5.13) Available experimental evidence from shearflow rheometry (cf. ยง4.2) would indicate that '1'1 ~ 0, '1'2 ~ 0, } o ~ 1'1'21 < 0.2'1'}>
(5.14)
so we expect (5.15) for nonNewtonian elastic liquids. This is important, since it indicates that the extensional viscosity TIE must be an increasing function of i for very small values of i, i.e. initial tensionthickening must be anticipated for all elastic liquids satisfying (5.14), whatever the response at higher values of i may be. Bird (1982) has made the interesting observation that it is usually easier to calculate theoretically the extensional flow characteristics of molecular models than the corresponding shear flow functions. He has also provided a useful summary of the TIE predictions for various molecular models of polymeric liquids. Many of them predict infinite extensional viscosities at a finite value of the extensional strain rate (d. the predictions in Table 8.3). Partly to overcome this problem, Phan Thien and Tanner (1977) proposed a model which allows TI E to pass through a maximum rather than take infinite values. For general and future interest, we show in Fig. 5.4 schematic TIE and TlEP curves computed for the socalled PTT modeL Interestingly, although the initial values of TIE and TlEP are different at low strain rates, in agreement with eqns. (5.8) and (5.9), they are indistinguishable at high strain rates. The general observation concerning the relative ease of carrying out theoretical work on the extensional flow characteristics of molecular models is also illustrated
Extensional viscosity
82
[Chap. 5
"0 c
.~J I ~E
..... ~o
~
o
j . .3.L71_         Strain ra te. f:
Fig. 5.4 Showing how the planar, l1EP' and uniaxial, l1E' extensional viscosities vary with strain rate i for the PhanThienTanner (P'IT) model.
by the important work of Batchelor (1970, 1971) on suspensions of slender particles. He showed that the extensional viscosity for such systems can be very high, depending on the aspect ratio of the particles. 5.4 Experimental methods 5.4.1 General considerations It is generally agreed that it is far more difficult to measure extensional viscosity than shear viscosity, this being especially so for mobile liquids. There is therefore a gulf between the strong desire to measure extensional viscosity and the likely expectation of its fulfilment. Concerning experimentation, we remark that, in the case of stiff systems, the basic problem is not one of exposing the sample to a uniaxial extensional flow, but rather of maintaining it for a sufficient time for the stress (in a controlled strainrate experiment) or the strain rate (in a controlled stress experiment) to reach a steady state, thus enabling the steady extensional viscosity TIE to be determined. This is nowhere better illustrated than in the careful experimentation on the LDPE sample commonly referred to as IUPAC A (see, for example, Meissner et al. 1981, and Fig. 5.12). Extensive early work up to Hencky strains * of 5 or 6 seemed to indicate that an equilibrium had been reached, thus permitting the calculation of TIE' However, further experiments involving strains of up to 7 have indicated that the "equilibrium" was in fact a "turning point" and the ultimate equilibrium value of TI E' if it exists, must be lower than the original (overshoot) value (see, for example, Meissner et al. 1981, Meissner 1985). However, the new data do not point unam~ biguously to a new equilibrium value and Bird et al. (1987(a), p. 135) stress the * The Hencky strain length is L o.
â‚Ź
is defined as In( L / L o) where L is the final length of the sample whose original
5.4]
ExperifinentalfinethodS
83
general difficulty of reaching a steady state in extension for many polymer melts, questioning whether a meaningful extensional viscosity exists for some materials and conditions. Fortunately, a knowledge of the transient function 1idt,i) may be sufficient (or at least very useful) in many practical applications (cf. Bird 1982, Laun and Schuch, 1988). When it is realized that the Hencky strain of 7 reached in the Meissner experiments corresponds to stretching the sample to 1100 times its original length, the difficulties involved in extensional rheometry become selfevident. The problems of determining the extensional viscosity of mobile liquids are even more acute, but they are of a different type from those experienced for stiff systems. With mobile liquids, severe difficulties arise in trying to achieve a continuous extensional flow field which approximates that given in eqs. (5.1). The most that one can hope for is to generate a flow which is dominated by extension and then to address the problem of how best to interpret the data in terms of material functions that are rheologically meaningful. Fortunately, for many mobile elastic liquids, the extensional viscosity levels are so high (and potentially important) as to justify such an approach. This fact has spawned a number of extensional rheometers in recent years and most of them are able to capture the high extensional viscosities which are known to exist. The main outstanding problem is to assess critically the" viscosities" arising from the various methods and to see whether a concensus emerges. This is under active consideration (Walters 1988). 5.4.2 Homogeneous stretching method The homogeneous stretching method, illustrated in Fig. 5.5, was the first to be used to determine the extensional viscosity. A major (unavoidable) disadvantage of this method is that, in order to attain a constant extensional strain rate in the sample, the velocity of the movable block must vary exponentially with time. In principle this can now be accomplished very easily with the most recent electroniccontrol techniques, but the accelerating motion of the clamp places a severe constraint on the strain rates which can be attained, given the requirement that the motion must be sustained for a sufficient time for the stress (which is measured at either the stationary or the moving block) to reach a steady value. For practical reasons the overall deformation is clearly restricted in the conventional stretching method of Fig. 5.5. The Meissner (1972) apparatus shown in Fig. 5.6 goes some way to overcoming this problem (see also Laun and Mlinstedt 1978). Instead of end loading, constant stretching is provided by two sets of toothed wheels
I
\~'\'''~ ~
'\ Stationary block
Sample under test
\ Movable block
Fig. 5.5 Schematic diagram of the homogeneous stretching method.
Extensional viscosity
84
[Chap. 5
~

Fig. 5.6 Schematic diagram of the Meissner apparatus for attaining high strains (see, for example, Meissner 1972). Note that the stretched specimen is supported by a suitable liquid.
which rotate with constant angular velocity. The stress can be measured by the deflection of a spring F, associated with one pair of rollers. Using this method on polymer melts, Meissner (see, for example, Meissner 1985) has been able to reach Hencky strains as high as 7. A further recent development has involved the use of a series of clamps in the form of a ring. In this way other modes of (multiaxial) extensional deformation can be generated (Meissner 1985). The homogeneous stretching method is clearly restricted to highviscosity systems. 5.4.3 Constant stress devices The instruments shown schematically in Figs. 5.5 and 5.6 are of the constant strainrate type. An alternative technique, first introduced by Cogswell (1968) and developed later by Mtinstedt (1975, 1979) utilizes a constant stress, which is brought about by applying a force to the movable block in Fig. 5.5, the force decreasing in proportion to the crosssectional area of the extending specimen. Cogswell exployed this method using a cam to apply a programmed load, together with a convenient means of measuring the length of the sample as a function of time. It is interesting to note that as a general rule the constant stress devices reach the steadystate elongational flow regime at smaller total deformations than the constant strainrate devices. For example, Laun and Schuch (1989) quote that a strain of 3.5 was required to reach equilibrium in a constant stress experiment on an LDPE melt whereas a strain of 4.5 was required in the comparable constant strainrate experiment. The constant stress devices are also clearly restricted to highviscosity systems. 5.4.4 Spinning It is selfevident that fibre spinning involves a significant extensionalflow component. At the same time, it is extremely difficult (if not impossible) to interpret
5.4]
I
Experimental methods
85
Res1rvoir
'~~I
._l
I
Die swett I
Test section
i'L
Wind  up or suction device Fig. 5.7 Schematic diagram of the spinline rheometer.
the data unambiguously in terms of the extensional viscosity 11 E defined in eqns. (5.2). The problem is that, although the flow may be steady in an Eulerian sense (in that the velocity at a fixed distance down the threadline does not vary with time) it is unlikely to be steady in a Lagrangian sense (since the strain rate experienced by a given fluid element will generally change as it moves along the threadline). Furthermore, even when the strain rate is constant over a portion of the threadline (so that a given fluid element is exposed to a constant strain rate for a limited period of time) that element may still "remember" conditions experienced in the reservoir in the case of highly elastic liquids. Certainly, there is ample evidence that a change of conditions in the spinnerette can significantly affect the response along the threadline under some conditions. The fibrespinning experiment (Fig. 5.7) is therefore a typical illustration of the dilemma facing rheologists who are interested in extensionalviscosity measurement. It is relatively easy to perform, the general kinematics can be determined with relative ease, and a suitable stress variable can be obtained from force measurements on the reservoir or the takeup device (see, for example, Hudson and Ferguson 1976, Jones et aL 1987). However, a consistent quantitative interpretation of the experimental data in terms of the extensional viscosity 11 E defined in eqns. (5.2) is not possible. One can certainly define an extensional viscosity by dividing the measured stress by (say) an average value of the strain rate (Jones et aL 1987). Given the difficulties encountered in measuring extensional viscosity and the scale
Extensional viscosity
86
[Chap. 5
of the viscoelastic response in such a flow, the proposed course of action can be justified and may be all that is required in many circumstances. The spinning technique can be used for polymer melts (see, for example, Laun and Schuch 1989) and for low viscosity liquids (Jones et al. 1987). In the commercial spinline rheometer (see, for example, Ferguson and EITawashi 1980) the windup device is a rotating drum. A variant of this for very mobile liquids is to use a suction device (Gupta and Sridhar 1984). 5.4.5 Lubricated flows A schematic diagram of the lubricateddie rheometer is given in Fig. 5.8. The shape of the test section is so designed that the flow is equivalent to steady extensional flow if there is perfect slip at the walls. To facilitate this, lubricant streams of low路viscosity Newtonian liquids are employed. Pressure measurements provide the relevant stress input. This would seem to be a convenient technique for eliminating the unwanted shearing induced by the rheometer walls, thus providing a flow close to the desired extensional flow. However, the interface boundary condition between the sample and the lubricant is dependent on the rheological properties of the sample. The interpretation of experimental data is therefore not without its problems and the technique itself is far from easy to use (see, for example, Winter et al. 1979, Williams and Williams 1985, Jones et al. 1987). A similar technique has also been used by Winter (see, for example, Soskey and Winter 1985) to study biaxial extensional flows of polymer melts. In this case uniform discs of the sample are placed between two parallel circular plates, both of
I I
I I
r I
I
/
Pressure measurement on wolf Lubricant
:.;
_ +,~u_id_ ~_::~?::_ ~=~ ~:;::::::;r::::::::::::;;::s::::r
Fig. 5.8 Schematic diagram of the lubricatedconvergingflow rheometer; the shape of the channel walls is chosen such that the flow is equivalent to a pure extensional flow if the lowviscosity lubricant streams are able to bring about" perfect slip" at the walls.
5.4]
Experimental methods
87
which are coated with a lowviscosity lubricant. The plates are then squeezed together. The relationship between applied load and rate of squeezing is interpreted in terms of the biaxial extensional viscosity 1JEB' Again, data interpretation is difficult and the technique itself is not easy to use.
5.4.6 Contraction flows The contractionflow method of determining extensional properties can be applied equally well to polymer melts and to more mobile systems like dilute polymer solutions. Indeed, in the case of polymer melts, the socalled Bagley (1957) correction (or a suitable variant of it) must be used to interpret correctly shear viscosity data from a capillary rheometer (cf. 搂2.4.9). The Bagley correction can be immediately utilized to yield extensionalviscosity information on the melt, as we shall see. Specifically, in capillary rheometry where the test fluid is forced to flow under pressure from a barrel into a capillary of much smaller radius, one technique is to measure the pressure in the barrel for fixed capillary diameter D and varying length L (d. Chapter 2 and Fig. 5.9). At a fixed flow rate, a plot of pressure as a function of LID provides sufficient information to facilitate shearviscosity determination: in particular, the pressure drop for fully developed Poiseuille flow along a capillary of a given length can be determined. Often, just two experiments are carried out in capillary rheometry: one for a capillary of a reasonable length (LID;> 20) and the other for so路called orifice flow (i.e. L = 0). It is this last experiment (and by implication the Bagley correction) which is of potential importance in the determination of extensionalviscosity characteristics. In general, a contraction geometry is simply two capillaries of different diameters with an abrupt contraction between them. In some experiments, as we have indicated, flow through an orifice is an alternative. Usually, but not always, the flow consists of a central core and a vortex region (see Fig. 5.10). The kinematics are determined by the flow rate and the shape of the central core region, whilst the relevant stress is obtained from the pressure drop required to force the test fluid through the contraction. There is no doubt that the
o
L/D
Fig. 5.9 The Bagley correction. The pressure drop (for a fixed flow rate and fixed capiIlary diameter) is measured for various values of capillary length. .
Extensional viscosity
88
[Chap. 5
NEWTONIAN
111 '0 Region of high â‚Ź
VISCOELASTIC
1 11
VORTEX ENHANCEMENT
Fig. 5.10 Contraction flow. In the case of highly elastic liquids, vortex enhancement usually occurs.
contractionflow experiment is relatively easy to perform and has many attractive features. An approximate analysis of the contractionflow problem has been developed by Binding (1988). This extends and reinterprets the early analysis of Cogswell (1972(a) and (bÂť. The Binding analysis is based on the assumption that the flow field is the one of least resistance; it includes both shear and extension in its formulation. The theory successfully predicts the phenomenon of vortex enhancement, which is often observed in axisymmetric contraction flows, and provides estimates of the extensional viscosity. 5.4. 7 Opensyphon method The opensyphon technique is shown schematically in Fig. 5.11. Fluid from the reservoir is drawn up through a nozzle by a vacuum pump and the nozzle is then raised above the level of the liquid in the reservoir. With some liquids the upward flow continues. This is the opensyphon effect. The flow rate and the dimensions of the fluid column yield the relevant kinematical information and the stress is provided by force measurements made at the top of the liquid column (see, for example, Astarita and Nicodemo 1970, Moan and Magueur 1988). In general terms, the opensyphon technique suffers from the same general disadvantages as the spinning experiment, so far as data interpretation is concerned. However, the former may have advantages in the case of structured materials like gels. In the spinning experiment the structure is often changed by shear in the delivery pipe. In contrast, the test material in the opensyphon technique is in its
5.5]
Experimental results
89
f "
','
"
:~~
"""
"'",'
f:~i
Fig. 5.11 The opensyphon technique for studying extensional flow. Liquid is sucked up from the reservoir into a tube, and the downward pull on the tube is measured.
rest state before being exposed to a sudden extension and one is therefore determining what is essentially a measure of the extensional properties of the virgin gel. 5.4.8 Other techniques Numerous other techniques have been suggested for the study of the extensional behaviour of mobile elastic liquids. These include the socalled triplejet technique (Oliver and Bragg 1974), the droplet techniques of SchUmmer and Tebel (1983) and Jones and Rees (1982), the elongation of radial filaments on a rotating drum (Jones et al. 1986) and stagnationpoint devices such as the opposingjet techniques of Odell et al. (1985), Keller and Odell (1985) and Fuller et al. (1987).
5.5 Experimental results Typical transient extensionalviscosity data for a polymer melt are given in Fig. 5.12 (cf. Meissner 1985, Bird et al. 1987(aÂť. It will be seen that as the strain rate i. is increased, the experimental results depart from "Trouton behaviour" *, increasing abruptly with time. This is called "strain hardening". There then follows the maximum in 1iE(t, i) already referred to in Â§5.4.1. In view of the extreme difficulty * Trouton behaviour, in this context, is obtained from linear viscoelasticity theory.
Extensional viscosity
90
[Chap. 5
10 6 ,        ,       , ,         ,     .       , 0,01 0,001
/
Trouton line
10' 10°
10' Time. t /5
Fig. 5.12 Extensional viscosity growth llE(t, i) as a function of time t for a lowdensity polyethylene melt. 423 K (see, for example, Meissner 1985).
of obtaining data at relatively high strains, rheologists nowadays often simply quote the maximum values of 1i E (t, i) (which were, of course, once thought to be the equilibrium values l1E( i)). When this is done, one obtains the type of. result shown in Fig. 5.13 for four polymer melts. The data are consistent with the requirements of eqs. (5.8) and (5.15). There is a clear indication of a maximum in l1E with strain rate for the polyethylenes. If the extensional viscosity and shear viscosity are plotted as functions of stress, 6
10
1
~
105t::::~
!.JOsf .c
=:::E.' ===
'Vi 10 7 o U
'!!! :..
oC
10 6 HDPE 2
o 'Vi C 105 '_....L..._'_ _....L..._'_ _J._...J
~L
J06~SZ, ~ 10'
102 Strain rate,
10°
€ /5 7
Fig. 5.13 Extensional viscosity data for four polymer melts (after Laun and Schuch 1989). LDPEIowdensity polyethylene; HDPEhighdensity polyethylene; PSpolystyrene.
5.5]
Experimental results
91
III
t1. 10' ~ III
o
U
III
:;:
LOPE
10 3
IUPAC A
10 2 '         '         '         '     . 1 . . .       ' 10' 10 2 10 3 10' 10 5 10 6 Stress. Pa
Fig. 5.14 Extensional viscosity and shear viscosity as functions of stress for the lowdensity polyethelyne designated IUPAC A. 423 K (ct. Fig. 5.12) (see, For example, Laun and Schuch 1989).
rather than strain rate, the response shown in Fig. 5.14 is obtained for a typical lowdensity polyethylene melt. In Fig. 5.15 we show extensionalviscosity data obtained from a spinline rheometer on a solution of polybutadiene in dekalin (Hudson and Ferguson 1976). Here there is a further and substantial increase in "lE after the tensionthinning region. The data in Figs. 5.13 and 5.14 do not extend to sufficiently high values of i to indicate whether the ultimate tensionthickening trend occurs also for stiff polymeric systems. We have already indicated that the accurate determination of "lE for mobile elastic liquids is very difficult, perhaps impossible, but the evidence to hand indicates that the extensional viscosities which have been measured can be very high indeed. For example, in Figs. 5.16 and 5.17 we show shear and extensionalviscosity III
t1.
"Iu
2路0
I':"
~ III 8 .!!l ::.
10
"0 c:
.~
III
c:
QJ
~
05 10
0
10'
10 2
Strain rate.i/s 1
Fig. 5.15 Extensional viscosity curve determined .with a commercial spinline rheometer for a 6.44% solution of polybutadiene in dekalin (cf. Hudson and Ferguson 1976).
Extensional viscosity
92
la' .,.
[Chap. 5
,.,.10 4
'
oQ.I
...c:::
V)
....III 10'
10' Sheaf rate,
'
G::
i / s'
Fig. 5.16 Viscometric data for aqueous solutions of polyacrylamide (1175 grade) (Walters and Jones 1988). Note that viscosity decreases and normal stress increases with shear rate.
10 4 .       . . . . . . . .  ,              ,         ,
III
~
~ 10
3
.b ..... III
o
U
.~
..e:.~~~
/\~
10' '
...1...
10'
10째 Strain fate,
'
10'
'
10 2
i/s'
Fig. 5.17 Extensional viscosity data obtained from a spinline rheometer for the aqueous polyacrylamide solutions of Fig. 5.16 (Walters and Jones 1988). Note that whereas shear viscosity decreased with shear rate, extensional viscosity increases with extensional rate.
5.5]
Experimental results
10'
x
VI
X
"I:'"
X
10 3
x
71
~
93
..
~
'iii 100
x
0
Q.
N,
"
~
iii u
c:
N,
..
III
....
Ql
':::::
1)
10 2
0
u
.~
VI VI Ql
.... .....
:::.
VI
.... 0
0
Ql
E ....
65
0
c:
... X
..... VI ....
2% POLYACRYLAI>4IDE SOLN. 3% XANTHAN SOLN,
10' ':"Ll.....Jl0' 10° 10' 10 2 Shear ra te. ; /5'
i:L
Fig. 5.18 Viscometric data for a 2% aqueous solution of polyacrylamide (E10 grade) and a 3% aqueous solution of Xanthan gum. Note the very different values of N l for solutions with almost the same viscosi ties.
104
,
,
,
10 4 r         r     
(a)
, (b)
2% POLYACRYLAMIDE 2% POLYACRYLAMIDE
/
3% XANTHAN
3% XANTHAN
10' ~l:"_J 10° 10' Strain rate. g/SI
Fig. 5.19 (a) Extensional viscosity data obtained from a spinline rheometer for the polymer solutions investigated in shear flow in Fig. 5.18; (b) Trouton ratios obtained from Figs. 5.18 and 5.19(a). Note that although the Xanthan gum solution is tensionthinning (Fig. 5.19(a», the associated Trouton ratios increase with strain rate and are still significantly in excess of the inelastic value of 3.
94
Extensional viscosity
[Chap. 5
data for a series of very dilute aqueous solutions of a very high molecularweight polyacrylamide designated 1175 (Walters and Jones 1988). It is not difficult to deduce that the Trouton ratios are as h.igh as 10 4 â€˘ We now refer to the rheometrical behaviour of two polymer solutions with almost identical shear viscosity behaviour (see Figs. 5.18 and 5.19). One is a 2% aqueous solution of polyacrylamide (E10 grade) and the other a 3% aqueous solution of Xanthan gum. We note that polyacrylamide is a more flexible polymer than Xanthan gum which is rodlike. The corresponding extensionalviscosity data obtained from a spinline rheometer show that the polyacrylamide solution is strongly tensionthickening, whereas the Xanthan gum solution is tensionthinning over the
Fig. 5.20 An illustration of the opensyphon effect for a 0.75% aqueous solution of polyethylene oxide.
5.6)
High extensional viscosity behaviour
95
range studied. However, when the Trouton ratios are calculated on the basis of eqn. (5.12), we see that even the Xanthan gum solution has T R values that are significantly higher than the Newtonian value of 3 over most of the range. Finally, we note that available evidence would indicate that the Trouton ratios for nonpolymeric colloidal liquids are much lower than those for polymeric liquids showing similar behaviour in smallamplitude oscillatoryshear flow.
5.6 Some demonstrations of high extensional viscosity behaviour We conclude this chapter by referring to some easily reproduced situations in which the dramatic effects of high Trouton ratios are clearly in evidence. Some of these can be readily performed in the laboratory with quite standard equipment. We have already referred to the opensyphon technique for measuring extensional viscosity (d. ยง5.4.7). We remark that the use of a 0.75% aqueous solution of polyethylene oxide WSR 301 grade (or similar polymer solution) will enable the experimenter to operate a conventional syphon several centimetres above the level of the reservoir liquid. The opensyphon effect is even more dramatically demonstrated when the polymer solution is transferred from one full container to a lower empty container. All that is normally required to (almost) empty the container is to start the flow by slightly tilting the top container. The initial flow will be sufficient to empty the bulk of the liquid from the top container (see Fig. 5.20). The opensyphon phenomena can be directly attributed to the very high Trouton ratios exhibited by the polymer solution. These and other dramatic demonstrations of high extensionalviscosity behaviour are illustrated in the film "NonNewtonian Fluids" produced by Walters and Broadbent (1980) *. Our final example of visual extensionalviscosity phenomena is provided by flow past cylindrical obstructions placed asymmetrically in a parallel channel (d. Walters and Jones 1988). The flow is basically twodimensional and may be considered to be made up of narrow channels and wide channels formed by the offset positioning of the circularcylinder barriers (Fig. 5.21). The behaviour of the Newtonian liquid is unspectacular with as much liquid going through the narrow channels as one would expect. This behaviour may be contrasted with that for the relatively inelastic Xanthan gum solution. In this case, a substantial flow finds its way through the narrow channels, clearly on account of the shearthinning viscosity. Finally, we note the qualitative difference in the behaviour of the highly elastic shearthinning polyacrylamide solution. In this case, extensional viscosity consider* The film is available in Video or 35mm form from the Department of Mathematics, University College of Wales, Aberystwyth, UK.
96
Extensional viscosity
[Chap. 5
Fig. 5.21 Flow visualization pictures for: (a) a Newtonian liquid; (b) a Xanthan gum solution; (c) a polyacrylamide solution. They show the dominant effects of shearthinning in the Xanthan gum solution and tensionthickening in the polyacrylamide solution (see, for example, Walters and Jones 1988).
ations are all important and virtually no liquid finds it way into the narrow channels. There is a relatively fastmoving stream in the wide channels and virtually stagnant regions elsewhere (d. the fourroll mill situation in Fig. 5.3).
CHAPTER 6
RHEOLOGY OF POLYMERIC LIQUIDS
6.1 Introduction The rheological literature is dominated by discussions of polymer rheology. The reasons for this are not difficult to determine; the subject is extremely important industrially and much money and many resources are expended in carrying out the relevant research. Also, polymeric liquids exhibit a wide range of rheological phenomena and can often be tailormade to facilitate fundamental rheological research. Indeed, it should not have escaped the reader that most of the examples used in earlier chapters to illustrate various rheological phenomena were obtained with polymeric liquids. The dominance of polymer rheology is also reflected in the number of books either devoted to the subject or strongly influenced by it. We shall have cause to mention some of these in the course of this chapter, but at this point we refer especially to the texts of Bird et aI. (l987(a) and (bÂť) which contain a thorough study of "the dynamics of polymeric liquids" and together are recommended as an (almost) encyclopaedic treatise on the subject. The fact that there are so many detailed and expert texts on polymer rheology and that the subject itself is very broad in scope suggests that, in the present introductory text, we should do no more than attempt an overview of the subject, pointing the interested reader to the preferred texts on matters of detail.
6.2 General behaviour The generic term U polymeric liquids" can be viewed as including a spectrum of possibilities, ranging from mobile systems like very dilute polymer solutions, through the concentrated solution regime to stiff systems like polymer melts. All the rheological properties introduced in earlier chapters can be demonstrated to occur in suitably chosen polymer systems. The wide diversity of observed phenomena is attributable to the long chain molecules, which are a unique characteristic of polymers. The length of the chain is the main factor determining the rheology, although many other factors are also influential, as we shall indicate. A long chain will occupy a great deal of space compared to its atomic dimensions. The possibility of polymer molecules linking together, either temporarily by intermolecular forces or more permanently by chemical cross linking (as in the 97
Rheology of polymeric liquids
98
[Chap. 6
IOJ.,.,""T""".r~ 10 5 0 RHE(JO(JNlo,.,~rER
~ ...0
r.jJ
AANGE CA.ptLI.~FI'1'
RA,IiGE
,
• a'l' : ........ "
IO'~
"c:.
I1J
qj
c:i
u
Cl..
(;
10 J ~
. 10'
~ .;;n
~ ii
o
'"
.!!,! ::::..
""""<II
10~ ~
III
'I
•
0
~ c:
0
10' '...&...:;::~...l.....::__~=__JL.J TO' .... III TOO 10' W2 IO J 10' 10 5 ~ Shear rote. i/~I Dr Strain rDte. i/5 1
Fig. 6.1 Steady shear and extensional viscosity data for a concentrated solution of a semirigid polymer of modest molecular weight. 25 0 C. Full lines ( ) steady shear data obtained with a rheogoniometer and a capillary rheometer (points not shown). Crosses (X X X) and broken line (_.  . ) extensional viscosity from the spinline rheometer and contraction flow respectively. Triangles (..........) predictions based on the CoxMen rule for viscosity. Squares (•••) NI derived from IGe I as described in §6.10.
vulcanization of rubber) increases still further the space over which the influence of an individual molecule is felt. If the polymer chain is long enough, the intermolecular association known as entanglement occurs. The entangled polymer, whether in the molten state or in nondilute solution, gives rise to the effects of high elasticity, such as normal stresses and high extensional viscosity. 10 1,
, IOJ
IrI
ti
0
a..
Q...
"'
,",
l:l
I:"
~
'~
~ 10'
101~
,~
u .l!'!
...
~
.~
E
.~
0
~ 0
c::
cS
~ 10°""'"":'"':~....L...Jl0'
TO J
10 0
Frequency. Hz
TO'
102
Fig. 6.2 Oscillatory data for the polymer solution of Fig. 6.1 obtained with a rheogoniometef. 25 Q C.
6.2]
General behaviour
99
The vast majority of polymeric liquids exhibit shearthinning in a steady simpleshear flow (d. §2.3.2). Figure 6.1 contains a typical example, for a concentrated solution (30%) of a stiffchain polymer of moderate molecular weight ( 20,000). Such behaviour may be viewed as being of modest proportions and it is certainly possible to generate more severe shearthinning by, for example, increasing the molecular weight of the polymer. However, the data in Fig. 6.1 clearly demonstrate the existence of a first (lower) Newtonian region followed by the shearthinning zone. Figure 6.2 contains the corresponding dynamic data obtained from a smallamplitude oscillatoryshear flow (cf. §3.5). When the CoxMerz rule lie is applied to the dynamic data, we see from Fig. 6.1 that the shear viscosity behaviour is predicted very well over the available range of the da tao In some circumstances, because of experimental limitations, it is not possible to reach the second (upper) Newtonian region, and it is even more difficult to reach sufficiently high shear rates to check on the existence or otherwise of the ultimate (shearthickening) upturn in viscosity mentioned in §2.3.3. However, recent studies have demonstrated that shearthickening, sometimes accompanied by antithixotropy, can be obtained in dilute polymer solutions beyond a critical set of conditions (see, for example, Jackson et al. 1984). Figure 6.1. also contains first normal stress data for the polymer solution. The normal stress level is also modest and it is certainly possible to obtain much higher normal stresses in polymeric liquids. N 2 data are not available for this polymer solution, but from the discussion of §4.2 we would anticipate N 2 to be negative and much smaller than N 1• Extensionalviscosity results for the polymer solution are also included in Fig. 6.1. These were obtained from the spinline rheometer and a contraction flow device (d. §5.4.6). 'I'IE is seen to be relatively constant over the range of the experiments. Since 7](Y) falls as y increases, it is evident that the resulting Trouton ratios are greater than 3 over much of the experimental range. The extensionalviscosity behaviour of polymeric liquids is maybe the one area where it is possible to distinguish qualitatively between the behaviour of dilute polymer solutions and polymer melts. We have already alluded to this in §5.5, where we showed that the general viscosity behaviour of dilute polymer solutions and polymer melts was similar to that shown schematically in Fig. 6.3. In the former, l1E rises abruptly with strain rate i after some critical strain rate f c ; l1E can reach very high values indeed. In constrast, for a polymer melt, 'ijE is usually a weak function of i, by which we mean that the magnitude of 1JE does not change very much as i. is varied. Note, however, the indication that, even in the case of polymer melts, 'ijE may ultimately rise sharply with increasing i.. Arriving at a firm conclusion on this matter is hindered by the difficulty of obtaining consistent experimental data at
... The empirical Cox.Men. (1958) rule slates that the shear viscosity l'J should be the same function of shear rate i' as 1'1*1 is of frequency w, where 1l'J*1 =[('Pl')2+(G'lw)~11/2. 'Pl' and 0' being the dynamic viscosity and dynamic rigidity, respectively (see Chapter 3 and §4.5).
Rheology ofpolymeric liquid.'i
100
[Chap. 6
(bl
(a'
I /
I
"" 3710
"'
Slroin role
Fig. 6.3 Schematic representation of typical shear viscosity "l and extensional viscosity (a) A dilute polymer solution; (b) A concentrated polymer solution or polymer melt.
7j E
behaviour for:
sufficiently high strain rates, but recent molecular theories are not inconsistent with such a trend (Marrucci 1988). Note that for all polymeric liquids, the Trouton ratio is expected to be always greater than or equal to 3, with the value 3 only attained at vanishingly small strain rates (cf. Chapter 5). We make passing reference to the one type of highly elastic polymer solution which does not exhibit measurable shear thinning. We refer to the socalled Boger (1977(aÂť fluids, which are very dilute solutions of a high molecularweight polymer in a solvent with a high viscosity TIs' The dissolved polymer only contributes a small proportion (say 5%) to the final zeroshear viscosity Tlo of the polymer solution. This means that the viscosity is essentially confined to lie between Tlo and TIs' so that the shearthinning is constrained to be at most 5% and, in practical terms, it appears from conventional rheometry that the polymer solution has a constant viscosity. At the same time, the presence of the high molecularweight polymer, even at very low concentration levels, can result in substantial normal stresses and high extensional viscosities, and the polymer solution may be (loosely) regarded as being a highly elastic constantviscosity liquid .... Examples of such a liquid include very dilute solutions ( 0.1 %) of polyacrylamide in a maltose syrup/water base and very dilute solutions (0.1 %) of polyisobutylene in a mixture of kerosene and low molecularweight polybutene (see, for example, Prilutski et al. 1983). Boger fluids have proved to be popular test fluids in the study of viscoelastic effects in complex flows (see, for example, Binding et al. 1987).
... Some experimental evidence would suggest that N.. 1980).
=0 for Boger fluids (see Fig. 4.5 and Keentok et a1.
6.3)
Effecl of temperature On polymer rheology
101
6.3 Effect of temperature on polymer rheology It is now instructive to consider the changes which can occur in a given polymer system when a variable parameter is scanned over a range. As a first example, we take a thermoplastic polymer and change the temperature (see also Â§2.2.2 and d. Tanner 1985, Chapter 9). At temperatures well above the melting point Tm , the polymer is a liquid with a measurable (shearthinning) viscosity. It is possible to observe normal stresses in simple shear flow and also relatively high extensional viscosities, which indicate that the melt is viscoelastic. As the temperature is reduced the viscosity increases rapidly and the elasticity becomes more evident. In this state the melt displays a pronounced elastic recovery from any deformation. It is this ability to recover from large deformations that justifies the description of the behaviour as 'highly elastic'. At still lower temperatures, some polymers crystallize and the freezing point is a firstorder transition which involves latent heat. Polyethylene is an example of a crystallizing polymer. The semicrystalline solid polymers have a shear modulus of about 1 GPa. This value is about 10 4 times higher than the modulus of a typical unhardened rubber but is lower than that for a metal. The polymer in this state can in general undergo larger deformations than metals without fracturing. Other polymers do not crystallize but continue to increase in viscosity, eventually to form a glass. Polystyrene is an example of a noncrystallizing polymer. The glass transition is not a welldefined change of state and depends on the method of measurement. It is not accompanied by a latentheat change. Some liquidstate theories associate the glass transition temperature Tg with the attainment of a particular value of the free volume. Since free volume and viscosity are closely related at high viscosities, Tg has also been associated with the attainment of a TABLE 6.1 Transition temperatures and operating temperatures for some common polymers Tm{Â°C}
Tg (0C)
Normal meltprocessing temperatures ( C C)
140
100
160240
I.sotactic polypropylene (PP)
165
15
180240
Polyethylene terephthalate (PEl)
265
70
275290
Nylon66
265
40
275290
Polystyrene
n/a
100
180240
High density
}
polyethylene (HDPE) Low density polyethylene (LDPE)
Rheology of polymeric liquids
102
[Chap. 6
certain viscosity, which has a value of about 10 12 Pa.s. Since polymers do not crystallize readily, it is reasonably easy to prevent crystallization by rapid cooling or by introducing a degree of chain branching into the molecules. Table 6.1 contains Tm and ~ va~ues for some conunon polymers (from White 1980; see also Tanner 1985 p. 351).
6.4. Effect of molecular weight on polymer rheology
The second example illustrating general rheological behaviour of polymer systems is provided by a series of polymers at a given temperature but covering a range of molecular weights. 1 J 3 "
poly' r/im.'hybsilor,,,,. J poly {~u 'odj',n. J pr)ly fm.,hylm"hocryIQ',} poly {8'yr.n.J
o
J 2 3 I. log (Mw ) + const,
5
6
Fi8. 6.4 Varialion of uroshear melt viscosity wilh molecular weighl. The data have been scaled using constant factors in order .that the change in slope should occur at the same position and the curves should be separ.ated. To the left of the transition the slope is 1.0, whilst to the right lhe slope is 3.4 (from Ferry 1980, p. 244).
6.5]
ElfteJ of concentration
103
The monomer, and molecules containing just a few monomer units, are indistinguishable (rheologica1ly) from smallmolecule liquids, but at and above a certain length, the molecules become polymeric. In very high~frequency oscillatory experi· ments, Lamb and his coworkers (see for example, Gray et al. 1977) found no evidence of polymeric modes of motion in chains of polystyrene and other monomers less than eleven monomer units long. In samples of greater chain length than this, they observed polymeric behaviour. The zeroshear viscosity 110 of the melt increases (initially) as M1.0, where M is the molecular weight. With a further increase in M, 1)0 varies as M 3 .4. The change in the slope of the (110, M) curve is reasonably sudden and can be identified with a critical molecular weight denoted by Me. Some representative graphs taken from the extensive work of Berry and Fox (1968) and quoted by Ferry (1980, p. 244) are shown in Fig. 6.4. The melts in the region above the critical molecular weight are highly elastic. It is thought that the change in Mdependence is the result of the formation of entanglements between molecules. Entanglements are not merely the overlapping of adjacent molecules, since overlapping occurs at quite low molecular weight. Rather, entanglements are strong couplings, whose details are largely unresolved, but which act in a localized manner like chemical crosslinks between molecules. l
6.5 Effect of concentration of the rheology of polymer solutions We now consider the example of a polymer in solution. The polymer and solvent chosen are such that, at very low concentrations, there is no strong interaction between polymer molecules. In this region, physical properties change in direct proportion to the concentration c. As the concentration is increased, the increment in viscosity over that of the solvent increases at a faster rate. Ultimately there may be a change to a regime in which the viscosity varies as c 3 or even higher powers. The example given in Fig. 6.5 shows an increase in slope from 1.5 to 4. The transition is associated with the formation of entanglements, as happens in a melt above Me. It follows that this polymer in solution must be capable of forming entanglements, hence the molecular weight must be higher than Me for the strong concentrationdependence to occur. In this region the solution properties are very similar to those of the melt, namely strongly viscoelastic. A useful parameter which has been found helpful when making comparisons between different polymers in solution is the socalled "reduced concentration". This is the product of concentration and •intrinsic viscosity', c[ 11 J, and is therefore dimensionless. * Elastic effects achieve prominence when c[ 'lJ] attains a value in the range 5 to 10, and develop very rapidly with further increases in the parameter. * Note: in polymer rheology [1'J] usually has the dimensions of volume per unit mass (i.e. a reciprocal concentration); whereas in suspension rheology, since concentration is expressed as a volume per unit volume, [1'j] is dimensionless (see §7.2.3). Of course, the product c(71) is always dimensionless.
Rheology ofpolymeric liquids
104
[Chap. 6
;; 0 ci 0... " I .....
.
~
I
I':""
2
'=<;;;
~  3 4
1
0 1 2 fog fc/gllOOmO
3
Fig. 6.5 Zeroshear viscosity of solutions of polystyrene in benzene showing the change from a 1.Spower dependence On concentration to a 4power dependence. 'lib is the solvent viscosity (from Vinogradov and Malkin 1980, p. 187).
It should be understood that the three examples discussed in ยง6.3 to ยง6.5 are of specific rheological behaviour displayed by typical polymer systems; there are a number of variants. Thus, the details can be strongly influenced by such factors as molecularweight distribution, chain branching, polarity, copolymerization, polymer mixtures (blends), suspended solid particles, solventpolymer interactions and chain rigidity (see, for example, Brydson 1981, Vinogradov and Malkin 1980, Cogswell 1981, Nielsen 1977, White 1980, Laun and Schuch 1989). It is not appropriate for us to go into these in any detail, but two variants are worthy of special mention. These are polymer gels and polymeric liquid crystals.
6.6 Polymer gels A polymer gel is generally a solution in which the chains are crosslinked by a
more permanent means than mere physical entanglements. The crosslinks may be chemical bonds of the type used to vulcanize or harden rubbers. Alternatively, they may be crystalline regions linked by chains which pass through more than one of these regions. The latter process is the same as that which occurs in solid semicrystalline polymers. A rather different form of gel structure is obtained by adding high concentrations (say 20% vIv or more) of small solid particles such as carbon black to a polymer melt or concentrated solution. In such systems, the structure is formed by chains of the particles. although the formation of polymer bridges by adsorption on adjacent particles is an additional possibility. A gel can be formed in solution in two ways: either by contacting the crosslinked solid with a suitable solvent, which is then taken up by the solid by the process of swelling, or by crosslinking molecules already in solution. Many natural products, such as gelatine, form gels of the latter type.
6.7]
Liquid crystal polymers
105
Gels may be regarded as â€˘soft solids' with a wide range of elastic modulus depending on the extent of crosslinking. It is of interest that the particlefilled polymer gel, although having a high shear viscosity at low shear rates may have a relatively low extensional viscosity. The book by Glicksman (1969) contains useful background information on polymer gels. 6.7 Liquid crystal polymers Liquid crystals are formed in solutions of polymers which have a rigid backbone. Rigidity is conferred by introducing bulky groups such as benzene rings into the backbone structure. As the molecular weight is increased, chain entanglement begins at a critical value, as with flexible polymers. However, the concentration relationship for polymers above Me is very different. Initially, the viscosity increases rather rapidly with concentration beyond the entanglement point, but there then occurs a second critical point beyond which the viscosity decreases markedly. The phenomenon is shown in Fig. 6.6. The transition is a sharp one. It signals the formation of a strongly orientated polymer structure. Since orientation can be induced by shear, the position of the transition moves to lower concentrations as the shear rate increases. Liquid crystals are also formed in melts of rigidbackbone polymers. The rheological behaviour of the liquid crystalline state is dependent on the orientation vector and its relation to the flow direction. This has led to the prediction of strange effects and may account for the observation of a negative first normal stress difference and zero, or negative, die swen in some liquid crystalline polymer melts, which in other respects are highly elastic. For further information on this class of materials, the book edited by Chapoy (1985) is recommended. 30 ,
}
""jOe}
3
;JI.'JO'J ~9.00()
"
~ III
ma!_wtlighl 'O.oOr}
3
o
\J
$
10
Fig. 6.6 Dependence of viscosity on concentration for solutions of poly(pbenzamide) in dimethyl ac::elamide at 20 CI C. The liquidcrystalli.ne state occurs 10 the right or the maxima in the curves (Crom Vinogradov and Malkin 1980, p. 196).
106
Rh.twlogy 01 polym~,ic liquids
[Chap. 6
6.8 Molecular theories
6.8.1 Basic concepts Viscoelastic phenomena in a polymeric liquid are due, primarily, to intramolecular forces which arise from the orientation of chemicalbond vectors in the polymer chains and, in particular, from changes In orientation caused by the deformation of the liquid. A molecule possesses a minimumenergy state (or rest state), in which the bond vectors are distributed in essentially a random configuration, and elastic recovery is a consequence of the return to this state. Therefore, the kinetic theory of rubber elasticity (see, for example, Treloar 1975) is basic to the physics of polymeric liquids. The presence of other molecules, whether polymer or solvent, delays the reorientation process and gives rise to the viscous component of the rheological effect. Starting from these fundamental ideas, molecular theories of polymer liquids follow two main branches. One branch is entitied beadspring and the other network. They will be considered separately, although historically they were developed concurrently and are still being improved. For detailed treatments the reader is referred to Tanner (1985) and especially Doi and Edwards (1986) and Bird et al. (1987(bÂť. 6.8.2 Beadspring models: the RouseZimm linear models In beadspring models, viscous behaviour is specifically introduced by considering the molecule to be acted on by frictional drag according to Stokes' equation (see. for example, Bird et aI. 1987(b)) or more elaborate forms of it. The beadspring models, of which there are many, consider the sites of fluid friction to be represented by small spheres, or beads, which are connected by a length of polymer chain, which is itself considered to be frictionless. Figure 6.7 illustrates how the beads are imagined to be distributed along a chain. The chains between beads are equal in length and are sufficiently long for them to obey Gaussian statistics and thus for the chain elements to be entropic springs.
v
I
... ..
...
Fig. 6.7 The necklace model. Equal lengths of Gaussian chain (above) are represented by equal (below) joined by equalsized beads which account for the drag experienced in Ihe veloclty field.
spri~
6.8]
Molecular theories
107
Two cases have been considered: the dumbbell models in which two beads are placed at the extremities of one spring and the more realistic but more complicated neck/ace models, in which (N + 1) beads are connected by N equal lengths of spring. The simple Stokesdrag law was used by Rouse (1953) in a notable paper on the necklace model. Zimm (1956) extended the theory to account for socalled hydrodynamic interaction. The RouseZimm theories apply to conditions of smallamplitude oscillatory shear flow and hence to linear viscoelastic behaviour (cf. Chapter 3). Specifically, the RouseZimm treatment leads to linear viscoelastic models which are equivalent to distributed Maxwell elements, (see Fig. 3.7 (a» with an interpretation of the model parameters in terms of molecular characteristics. In passing, we remark that the constantviscosity restriction implied in the linear theories of Rouse and Zimm is relaxed in the Bueche (1954) treatment. In this, shear thinning is predicted in steady simple shear flow. Specifically, 11 is predicted to vary as yO.5. This rate of shearthinning is reasonable for moderately concentrated polymer solutions but is low compared with most experimental results for concentrated solutions and melts. The Bueche treatment is criticized in Bird et a11987 (b) P 161.
6.8.3 The GiesekusBird nonlinear models We turn now to the advanced kinetic theories of principally Giesekus, and Bird and coworkers (d. Giesekus 1985, Bird 1985, Bird et al. 1987(b». It was the intention of these researchers to develop models which predict nonlinear rheologi· cal effects, not just the linear ones as in the RouseZimm treatment. In order to do this, it was necessary to use the dumbbell approximation (see Fig. 6.8). At first sight it seems to be a retrograde step to adopt the dumbbell approximation when the beadspring necklace is intuitively a much better model of a real polymer chain. A major reason for making this step, and for its successful outcome, is that the longer relaxationtime processes are more influential than the short ones in conferring viscoelasticity, and the longest such p!ocess corresponds to the dumbbell. The relevant theories lead to constitutive equations of the upper convected Maxwell and Oldroyd B type (cf. §8.6). Specifically, the steady shear viscosity" is a constant, the first normal stress coefficient 'V1 is a positive constant and the second normal stress coefficient 1f'2 is zero (d. Chapter 4, eqs. 4.2 and 4.3). Numerous developments of the basic dumbbell model have been made and these are discussed in detail by Bird et al. (1987(b». Typical of these is the socalled
Fig. 6.8 The dumbbell approximation. The elastic behaviour is represtmted by a spring and the sites of the frictional drag are located at the ends of the spring.
l08
Rheology ofpolymeric liquids
[Chllp.6
FENEdumbbell model * which predicts shear.tllinning and a first normal stress coefficient which decays with shear rate. It also predicts stress overshoot in the startup of shear flow.
6.8. 4 Network models The essential difference between the kinetic theory of rubberlike elasticity and the network models of polymer solutions and melts is that the pennanent crosslinks between molecules in the rubber are replaced by transient junctions in the network. The concept of transience is that, at any instant, junctions are sufficiently "permanent" for the network to behave like a rubber but they break after a short lifetime and reform elsewhere, hence the system is capable of flow. Since the total concentration of junctions always remains constant, the elastic properties are constant. The original idea of the transient network was published by Green and Tobolsky (1946). It was extensively developed by Lodge (1956, 1964) and is often associated with his name. In a steady simpleshear flow, the Lodge rubberlike liquid predicts a constant viscosity 11, a positive (constant) 'l'1 and zero 'l'2' It seems to be a coincidence that the Lodge theory leads to very similar predictions to the simpler versions of the GiesekusBird theories, especially since the molecular concepts are quite different in the two cases. Numerous attempts have been made to modify the network theory by employing more realistic molecular modelling and sometimes by adding further ad hoc assumptions (see, for example, Kaye 1966, Tanner 1969, Acierno et a1. 1976, Johnson and Segalman 1977, Phan路Thien and Tanner 1977, Giesekus 1982, Leonov 1987). These attempts have been reasonably successful and it is now possible to predict, amongst other things, a second nonnal stress coefficient 'l'2 of the correct form (see, for example, the predictions for the JohnsonSegalman and PhanThienTanner models in Chapter 8). 6.8.5 Rep/ation models The entanglement theory of rubber elasticity of Edwards (1967) introduced a new physical concept which has had an influential impact on later developments in the molecular theory of polymer systems. The concept is of an equivalence between a chain constrained by entanglements, and/or crosslinks, and a relatively free chain constrained in a tube and unable to escape through its sides. Figure 6.9 represents the equivalence pictorially. A related concept for uncrosslinked polymers introduced by de Gennes (1971) has revolutionized ideas on the mechanism of permanent deformation, or flow, of the entangled molecules. This concept is that the only way a molecule can escape from its tube~ and hence allow flow to occur, is by diffusion along the tube. It is a wriggling, snakelike motion and the process has the aptly descriptive name of reptation. The detailed application of these concepts to polymer systems has been developed by de Gennes (1979), Doi and Edwards (1986) and
... FENE stands for "finitely extensible, nonlinear elastic".
6.9]
The method of reduced variables
•
•
•
• •
•
•
109
•
•
• •
• •
• •
Fig. 6.9 The DoiEdwardsde Oennes tube concept can be visualised by first placing the molecule on a plane (this page). Neighbouring molecules will intersect this plane at the points (see lefthand part or the figure). The nearest points define a tube which prevents major penetration by the molecule (!lee righthand part).
Curtiss and Bird (see Bird et al. (1987(b)). The DoiEdwards theory (with the additional "independentalignment" assumption) leads to a constitutive equation similar to the socalled KBKZ model (see Chapter 8, eqn. 8.35). However, this statement simply indicates the broad general form of the constitutive equations arising from the simpler reptation theories and should be read in conjunction with the recent papers of Marrucci who has shown the limitations of the independent alignment assumption (Marrucci and Grizzuti 1986, Marrucci 1986). There is no doubt that substantial progress has been made in deriving constitutive equations for polymeric liquids using •microrheological' concepts. The interested reader is referred to the detailed texts of Tanner (1985 Chapter 5), Doi and Edwards (1986) and Bird et al. (1987(b)) for fuller details.
6.9 The method of reduced variables In many cases it is important to study the full range of rheological properties for varying temperature and pressure (and in the case of polymer solutions, concentration as well). Such a study is facilitated by a suitable "normalization" procedure. The aim of such a procedure is to plot experimental results on a pair of axes using normalized variables, such that a unique curve is obtained whatever the temperature or pressure (or concentration). The socalled ~'method of reduced variables" is one way of accomplishing this. The method is fully described by Ferry (1980 p. 266), one of its originators, and it will be sufficient here to refer to the •timetemperature superposition' principle only, although the additional variables, pressure and concentration, are also accommodated in the full method. The method is basically empirical but is guided by reference to molecular theory. Timetemperature superposition depends on the principle that all the relaxation times in a spectrum have the same temperature dependence provided there is no phase change of the polymer within the temperature range considered. Hence (6.1 )
Rheology of polym~Tic liquids
110 9
[Chap. 6
10
.....
o 8
9 ~
Q.
~
~
"7 c" '3' 15' Cl.
I
"3 ......
8
" "cf'
7
"i '
0 .. ~
~
6
\~ ......
t:) .....

6 ~ I.
L..''.l.._
o
2
I.
___''_"'''_'_L_I.......J5
6
8
JO
12
II.
log (war /5')
Fig. 6.10 Results of the application of timetemperature superposition to data for an unvulcanized rubber. Reference temperature To::lll 298K. Shift factors aT were determined empirically by horizontal adjustment of individual Curves (from Whorlow 1980, p. 417). Note thaI p is the density.
where suffix T refers to temperature T and suffix 0 refers to the reference temperature To. An example where the empirical shift process has been used for an unvulcanized rubber is shown in Figs. 6.10 and 6.11. The curves of G and Gil obtained at different temperatures (and not shown here) have been successfully reduced to two single composite curves by introducing a common temperature of 298K. The procedure in this case has resulted in values of G and G" covering some 16 decades of frequency at 298K. Empirically it is found that 1
I
(6.2)
6
o 2 4
';"':;::~~~:~....J~l_.:::::::.J
1.0
20
0 20 ITT.J/I<
40
60
80
Fig. 6.11 Variation of shift factor ar for the rubber of Fig. 6.10 compared with the curve (solid line) predicted by the WLF equation CT.. "" 248K, Cl "" 8.86 and c1 "'" 101.6K).
6.11]
Practical applications
111
in which c1' C2 and ~ (a reference temperature) are constants. This form of the Q T function has become known as the WilliamsLandelFerry or WLF equation. A test of the WLF equation is given in Fig. 6.11 which contains a graph of the shift factors used to produce Fig. 6.10. For measurements of shear stress and normal stress in steady shear flow, the same principles apply with the reduced shear rate becoming aTi'. In the case of a given polymer solution at varying concentration and temperature, it is often possible to construct a master curve by plotting 1J/1Jo against 1JoY, where 1Jo is the relevant zeroshear viscosity. Examples of such a procedure are provided by Vinogradov and Malkin (1980, p. 207) who also discuss possible extensions and limitations of the procedure.
6.10 Empirical relations between rheological functions
We have already referred to the CoxMen: rule which provides a useful empirical correlation between the steady shear viscosity function 1J( y) and the dynamic data (1J'(w) and G'(wÂť in the case of polymeric liquids (see Â§4.5). A corresponding correlation between the first normal stress difference Nt (y) and the dynamic data has also been attempted (see, for example, Laun 1986, AIHadithi et al. 1988). Figure 6.1 for a concentrated polymer solution contains the relevant correlation based on the empirical formula of AlHadithi et al. (1988), viz.
IG I = c
+ ')G' )1 / 2 ( G' 1 + 1Jo 1J ( 2W(1J,)2
(6.3)
These authors proposed (as the CoxMen equivalent) that N 1 /2 should be the same function of y as I Gc I is of frequency w. Another useful empiricism is to plot the first normal stress difference Nt as a function of shear stress CJ on logarithmic scales. Often, a master curve is obtained which is independent of temperature. The data usually lie on a reasonably straight line even in the shearthinning region. Figure 6.12 contains an example of this procedure for a polymerthickened oil (see also Fig. 4.4).
6.11 Practical applications 6.11.1 Polymer processing Nowadays there is no need to emphasize the importance of plastics to modern life: it is regarded as self evident. Polymers are now used as primary materials of construction and have become indispensible. Specialized texts on rheological aspects of polymer processing have been written by Han (1976), Middleman (1977), Cogswell (1981) and Pearson (1985). Further,
Rheology o{polymeric liquifb
112
[Chap. 6
JO~ r~;____.
POLYMER THICKENED OIL T£f04P.
• c•
'c
0 s 20
~
JrJ
•
1.0
'0 E ...o c
Fig. 6.12 Plot of N1 against a for a polymerthickened oil. The data for different temperatures fall approximately on the same straight hne. The slope is 1.59.
many standard rheological texts have important chapters on the subject (see, for example, Tanner 1985). In the main, processing is carried out on the melt, although in some cases, such as in the formation of films and fibre of heatsensitive polymers, a solution is processed. The extruder is the most important melt processing machine and it incorporates a number of subprocesses, such as melting and mixing, prior to that of forming into rods, tubes or films. Extruders are also attached to moulds if the required final shape is more complicated. The process is then either injection moulding for "solid" objects or blow moulding when an extrudate sheet is forced by air pressure against a cooled mould surface. Extruded films and fibres are stretched to achieve their final thickness and molecular orientation. The process of drawingdown film extruded in the form of a tube or bubble is called film blowing, whilst the drawingdown of fibre is called spmrung. Pearson (1985) points out that in many processes the molten polymer can be considered to be an inelastic non~Newtonian liquid and the powerlaw model is often adequate in process modelling. This view is justified by the fact that many processing flows are characterized by a narrow dimension normal to the direction of flow and the socalled "lubrication approximation" can be employed (see also Tanner 1985). Under these conditions, it is not difficult to argue that shear viscosity is the dominant rheological influence. However, there are some important processing situations, e.g. film blowing, spinning and flow through a contraction, where extensional viscosity is clearly the rheological function of importance (cf. Chapter 5). Not surprisingly, therefore, the
6.11]
Practical applications
113
measurement of the extensional viscosity of polymeric liquids is viewed as a study of industrial importance. Melt flow instabilities such as "sharkskin" and •melt fracture' can occur in extrusion and these effectively place upper bounds on operating conditions. A review of such instabilities is provided by Petrie and Denn (1976). There is recent evidence that the materials used to construct processing equipment can have a significant effect on the critical conditions for the onset of melt flow instabilities thus indicating that interfacial as well as viscoelastic effects are important (Ramamurthy 1986).
6.11.2 Polymers in engine lubricants For more than 40 years, polymers have been used to make the socalled multigrade oils. The motivation is to reduce the large variation of viscosity with temperature and to thereby maintain good hydrodynamic lubrication at high temperatures, without incurring excessive frictional losses at low temperatures. The viscosity level of an automotive oil is specified by a grade number. By the use of polymer, it has become possible to formulate oils which meet the requirements of more than one grade, something which is impossible with ordinary lubricating·oil fractions. Hence the tenn "multigrade". The polymer additives are known as ViscosityIndex (or VI) improvers. The thickening effect of the VI improvers depends on the grades required, but in modem oils it can amount to more than a tripling of the baseoil viscosity. The blends show shearthinning behaviour, which does not become significant until shear rates exceed about lOS s 1. Since engine bearings can operate at shear rates two orders of magnitude higher than this. shearthinning must be accommodated in the design of a lubricant. Normal stresses and other viscoelastic effects can be measured in multigrade oils and evidence is accumulating that viscoelasticity, together with the increased viscosity, may help in carrying the bearing load. These and many other aspects of the rheology of lubrication were reviewed by Hutton (1980) although, at that time, viscoelasticity was thought to have a relatively minor role to play in journal bearings. 6.11.3 Enhanced oil recovery Unlike a water reservoir, a crude oil reservoir is located in the pores of sedimentary rock and the extraction of oil is not easy. A newly tapped deposit is held under earth pressure which will drive a proportion of the oil to the receiving bore holes. When this begins to fail, the secondary recovery process is initiated. This involves pumping water down holes set in a ring around the field. The water sweeps crude before it, but, since the water has the lower viscosity, the water/oil interface is unstable. When the instability occurs, water bypasses the oil in the form of "fingers" and reaches the receiving well first: any variation in the porosity of the oilbearing strata can exacerbate the fingering effect. Oil wells which have been
114
Rheology ofpolymeric liquids
IChap.6
abandoned .because of fingering may still contain as much as 50% of the original deposit. Hence t tertiary or enhanced oil recovery (EOR) is potentially important. Many proposed EOR methods are being researched. One method is known as polymer flooding. The principle is to stabilize the water/oil interface by using an aqueous polymer solution as the displacement fluid. Candidates for use in this connection are the relatively rigid Xanthan gum and the more flexible polyacrylamide. We have already shown in ยง5.5 that aqueous solutions of these polymers can behave similarly in shear flow but in a qualitatively different fashion in extensional flow. TIlls may be important in the relatively severe conditions near the well bore (see, for example, Walters and Jones 1988). 6. J 1.4 Polymers as thickeners of waterbased products
Many consumer products require the use of a polymer thickener. This might be for some technical reason such as the suspension of fine particles: typical are kaolin in medicines and abrasive particles in liquid abrasive cleaners. Although the amount of thickening is of paramount importancet the elasticity and the extensional viscosity are also relevant. The visual presence of "wobbliness" (which indicates high elasticity) and "stringinessu (which indicates a high extensional viscosity) are sometimes unacceptable to the consumer. It is of interest to note that polyacrylamide, one of the polymers of Figs. 5.18 and 5.19, is unacceptable in this respect because it forms solutions which have high elasticity and a high extensional viscosity. On the other hand the other polymer, Xanthan gum, forms solutions which are not so highly elastic and have a much lower extensional viscosity. ConsequentlYt on the basis of equal shear viscosity, Xanthan gum solutions are not wobbly or stringy in comparison with polyacrylamide solutions. Toothpastes and paints require the use of such "inelastic" polymer thickeners, whilst the food industry relies heavily on such materials for thickening sauces and soups. Polysaccharid~type polymers and natural gums are often used for this purpose (Glicksman 1969).
CHAPTER 7
RHEOLOGY OF SUSPENSIONS
7.1 Introduction The rheology of suspensions has been the subject of serious research for many years, mainly because of its obvious importance in a wide range of industrial applications (see, for example, Barnes 1981). Suspensions include cement, paint, printing inks, coal slurries, drilling muds and many proprietory products like medicines, liquid abrasive cleaners and foodstuffs. Examples of suspensions where the particles are deformable range from emulsions to blood. 7.1.1 The general form of the viscosity curve for suspensions The general viscosity/shear rate curve for all suspensions is shown schematically in Fig. 7.1. We could anticipate most of this behaviour from the general discussion of Chapter 2. The first Newtonian plateau at low shear rate is followed by the powerlaw shearthinning region and then by a flatteningout to the upper (second) Newtonian plateau. At some point, usually in this upper Newtonian region, there can be an increase in viscosity for suspensions of solid particles, given the appropriate conditions. In certain situations the first Newtonian plateau is sometimes so high as to be inaccessible to measurement. In such cases the lowshear rate behaviour is often described by an apparent yield stress. The factors controlling the details of the general flow curve in particular cases will now be considered. One point worth stressing here is that the relevant measure of the amount of material suspended in the liquid is that fraction of space of the
"".../
I
I I
Log shear rate
Fig. 7.1 Schematic representation of the flow curve of a concentrated suspension. 115
116
Rheology of suspensions
[Chap. 7
total suspension that is occupied by the suspended material. We call this the phase volume cp. This is the volumepervolume fraction, and not the weightperweight fraction that is often used in defining concentration. The reason why phase volume is so important is that the rheology depends to a great extent on the hydrodynamic forces which act on the surface of particles or aggregates of particles, generally irrespective of the particle density. 7.1.2 Summary of the forces acting on particles suspended in a liquid Three kinds of forces coexist to various degrees in flowing suspensions. First, there are those of colloidal origin that arise from interactions between the particles. These are controlled by properties of the fluid such as polarisability, but not by viscosity. These forces can result in an overall repulsion or attraction between the particles. The former can arise, for instance, from like electrostatic charges or from entropic repulsion of polymeric or surfactant material present on the particle surfaces. The latter can arise from the everpresent Londonvan der Waals attraction between the particles, or from electrostatic attraction between unlike charges on different parts of the particle (e.g. edge/face attraction between clay particles). If the net result of all the forces is an attraction, the particles flocculate, whilst overall repulsion means that they remain separate (i.e. dispersed or deflocculated). Each colloidal force has a different rate of decrease from the surface of the particle and the estimation of the overall result of the combination of a number of these forces operating together can be quite complicated. Figure 7.2 shows the form of some single and combined forces (see Hunter 1987 for a more detailed account of colloidal forces). Secondly, we must consider the everpresent Brownian (thermal) randomising force. For particles of all shapes, this constant randomisation influences the form of the radial distribution function (Le. the spatial arrangement of particles as seen from the centre of anyone particle), whereas for nonspherical particles, spatial orientation is also being randomised. The Brownian force is of course strongly sizedependent, so that below a particle size of 1 p.m it has a big influence. This force ensures that the particles are in constant movement and any description of the spatial distribution of the particles is a time average. Thirdly, we must take into account the viscous forces acting on the particles. The viscous forces are proportional to the local velocity difference between the particle and the surrounding fluid. Hence the way these affect the suspension viscosity enters via the viscosity of the continuous phase which then scales all such interactions. Thus an important parameter is the 'relative viscosity' 'riP defined as the suspension viscosity divided by the continuousphase viscosity. Clearly, the rheology measured macroscopically is strongly dependent on these microstructural considerations. For instance, the presence of isolated particles means deviation of the fluid flow lines and hence an increased viscosity. At higher concentrations, more resistance arises because particles have to move out of each other's way. When particles form flocculated structures, even more resistance is encountered because the flocs, by enclosing and thus immobilising some of the
7.1]
Introduction
117
\ ~
(a)
(b)
DISTANCE
! ~ ~
(.)
...."'1:~
L..
""
'
J
Fig. 7.2 Examples of the typical interaction forces between a pair of submicron particles: (a) van der Waals attraction (omnipresent); (b) Steric repulsion due to adsorbed macromolecules; (c) Electrostatic repulsion due to the presence of like charges on the particles and a dielectric medium; (d) A combination of (a) and (b); (e) A combination of (a) and (c); (f) A combination of (a), (b) and (c).
continuous phase, have the effect of increasing the apparent phase volume, thus again giving a higher than expected viscosity. 7.1.3 Rest structures When particles are introduced into a liquid at rest they usually assume a state of thermodynamic equilibrium which, when the Brownian motion dominates, corresponds to a random disordered state. When colloidal forces dominate, the particles form structures whose forms depend on whether the overall forces are attractive or repulsive. When they are attractive they form aggregates and when they are repulsive they form a pseudolattice. The particular shape of aggregates can vary from nearspherical floes to strings. The latter is sometimes referred to as a stringofpearls structure. Pigment dispersions form floes and silica dispersions can form the string structures. Pseudolattices are formed by overall repulsion, for instance in systems of particles carrying electrostatic charges of the same sign dispersed in a polar continuous phase. The particles then take up positions as far from each other as possible. If the charge on such particles is very large, movement of the particles is severely restricted and the structure can be visualised as a pseudocrystal: if the lattice spacing is comparable to optical wavelengths, interference effects occur and the suspension displays irridescence.
Rheology of suspensions
118
[Chap. 7
Any of the structures mentioned above can be modified by the adsorbtion of surfactant materials onto the surface of the particles. The structures formed by electrostatic charges can be modified by the addition of electrolytes. The structures discussed so far are formed by nearspherical particles. However, if the basic particle is itself anisotropic, very complicated structures can be formed. One example is an aqueous suspension of bentonite clay: the basic particle is platelike and it carries charges of opposite sign on the faces and edges. The aggregated structure is then like a house of cards with edges attracted to faces. Another example is a suspension of soap crystals. Soap can be made to crystallize in the form of long ribbons, which then intertwine to form an entangled structure, as in lubricating grease. A useful method for judging the importance of colloidal forces has been derived by Woodcock (1985). It gives the average distance Ii between first neighbours in terms of the particle size d and the volume fraction cf.> as follows:
(7.1)
This expression is plotted in Fig. 7.3 for four sizes of particle. The diagram also shows the range of action of typical colloidal forces. This diagram indicates for example that, for a suspension with a cf.> of 0.2 and particle size 0.05 .urn, electrostatic interactions will be very important. This will not be so if particles are larger or if the concentration is lower.
Sphere diameter, d/j.)m
0,05 ..  0,10 
0·50
   J·oo
01
0·2
03 O·{. 0·5 Solids volume frac tion
0·6
0'7
Fig. 7.3 Average interparticle separation as a function of concentration for monodisperse spheres (according to eqn. (7.1» plotted for four particle sizes. The horizontal lines show twice the distance over which various interparticle forces typically operate: (A) Electrostatic forces in aqueous suspensions with low salt levels; (B) Steric forces originating from adsorbed macromolecules; (C) Steric forces originating from adsorbed nonionic detergents.
7.2]
Solid particles in Newtonian liquids
119
7.1.4 Flowinduced structures We shall consider first, relatively unaggregated systems in which the Brownian forces dominate. When a concentrated suspension of this type flows at very low shear rates, the particles necessarily have to move around each other or "bounce off' each other for overall flow to occur. This involves a large resistance and the resulting viscosity is high. On the other hand, the distribution of particles remains essentially undisturbed because the effect of Brownian motion dominates the shear motion and restores the randomness of the reststate distribution. The viscosity remains essentially constant. At slightly higher shear rates, the imposed velocity gradient induces an orientation of the particle structure, which is not restored by the Brownian motion. However this orientation enables particles to move past each other more freely than at very low shear rates and hence the viscosity is lower. At even higher shear rates, the structure is so grossly orientated that the particles form layers separated by clear layers of the continuous phase. The viscosity is then at its minimum value. The suspension is shearthinning. The existence of particle layers has been confirmed by light diffraction. When shearing is stopped the flowinduced layered structure gradually disappears. If the shear stress is increased above a critical value, the layers disrupt and gradually disappear. Hence, the viscosity begins to rise again and it also increases with time of shearing. Flowinduced structures can also be formed by the more complicated clay and soap suspensions mentioned earlier. In these cases, flow causes the plates and ribbons to align in the direction of flow. This orientation can be detected by optical techniques. Examples of increased flocculation caused by flow are also known (see, for example, Cheng 1973).
7.2 The viscosity of suspensions of solid particles in Newtonian liquids 7.2.1 Dilute dispersed suspensions A considerable amount of progress has been made in predicting the viscosity of dilute suspensions (10% and less phase volume). All studies essentially extend the work of Einstein (1906, 1911) on spheres, so that particle shape, charge and the small amount of hydrodynamic interaction arising when anyone particle comes into the vicinity of another can all be taken into account. Einstein showed that single particles increased the viscosity of a liquid as a simple function of their phase volume, according to the formula 11
=
11 s(1
+ 2.5</Âť,
(7.2)
where 11 is the viscosity of the suspension and 11s is the viscosity of the suspending medium. We notice immediately that in eqn. (7.2) there is no effect of particle size, nor of
120
Rheology of suspensions
[Chap. 7
particle position, because the theory neglects the effects of other particles. When interactions between particles are included, the situation becomes more complicated. The presence of other particles is accounted for by higherorder terms in cp. However the only tractable theory is for extensional flow, because only in this type of flow can the relative position of the particles be accounted for analytically. Batchelor (1977) gives the viscosity in this case as
(7.3) where the viscosities must now to be interpreted as extensional viscosities (Chapter 5).
A number of experimental determinations of the term multiplying cp2 for shear flows have been made, but the range of values so obtained is large (varying from about 5 to 15). A great deal of work has been done and many reviews written (see, for example, Barnes 1981) on dilute suspensions, but almost all conclude that, apart from providing some limiting condition for the concentrated case, the work is of little relevance to suspensions of industrial importance. Dilute suspension theory covers the range below 10% phase volume, and this accounts for no more than a 40% increase in viscosity over the continuous phase. 7.2.2 Maximum packing fraction The influence of particle concentration on the viscosity of the concentrated suspensions is best determined in relation to the maximum packing fraction. There must come a time, as more and more particles are added, when suspensions "jam up", giving continuous threedimensional contact throughout the suspension, thus making flow impossible, i.e. the viscosity tends to infinity. The particular phase volume at which this happens is called the maximum packing fraction CPm' and its value will depend on the arrangement of the particles. Examples are given in Table 7.1. Maximum packing fractions thus range from approximately 0.5 to 0.75 even for monodisperse spheres. The maximum packing fraction, as well as being controlled by the type of packing, is very sensitive to particlesize distribution and particle shape (see, for TABLE 7.1 The maximum packing fraction of various arrangements of monodisperse spheres Arrangement
Maximum packing fraction
Simple cubic Minimum thermodynamically stable configuration Hexagonally packed sheets just touching Random close packing Bodycentred cubic packing Facecentred cubic/ hexagonal close packed
0.52 0.548 0.605 0.637 0.68 0.74
7.21
Solid particles in Newtonian liquids
121
example, Wakeman 1975). Broader particlesize distributions have higher values of epm because the smaller particles fit into the gaps between the bigger ones. On the other hand, nonspherical particles lead to poorer spacefilling and hence lower epm' Particle flocculation can also lead to a low maximum packing fraction because, in general, the flocs themselves are not closepacked. From the above considerations, we see that the ratio eplepm is a relevant normalized concentration. 7.2.3 Concentrated Newtonian suspensions The situation for concentrated suspensions, where we expect higherorder terms than ep2 to be important, is even more difficult to analyse from a theoretical point of view. The only methods available to tackle the problem are to introduce a technique for averaging the influence of neighbouring particles or alternatively to simulate the situation using computer modelling. One recent development, based on an averaging technique, is that of Ball and Richmond (1980) who essentially start from the assumption that the effect of all the particles in a concentrated suspension is the sum of the effects of particles added sequentially. Hence the Einstein equation can be written in a differential form
d TI
=
(5T112) dep,
(7.4)
where dTl is the increment of viscosity on the addition of a small increment of phase volume dep to a suspension of viscosity TI. The viscosity of the final suspension is then obtained by integrating the phase volume between 0 and ep, for which the viscosity is TIs and TI, respectively. Then TI = TIs
exp(5epI2).
(7.5)
Ball and Richmond point out that this omits the correlations between spheres due to their finite size. This means that when a particle is added to a relatively concentrated suspension it requires more space than its volume dep, due to packing difficulties. Therefore dep has to be replaced by dep/(1  Kep), where K accounts for the socalled "crowding" effect. Integration now yields
(7.6) From this equation we see that the viscosity becomes infinite when ep = 11K. Therefore, we can identify 11K with the maximum packing fraction epm' Ball and Richmond's expression is effectively identical to that of Krieger and Dougherty (1959). Krieger and Dougherty's theory also states that, in the general case, the 5/2 factor could be replaced by the intrinsic viscosity [TI]. * The value of 512 is the * Note: in suspension rheology [TIl is dimensionless, since the phase volume is also dimensionless (see eqn. (7.2Âť; whereas in polymer rheology the concentration is usually expressed as a mass per unit volume, thereby giving [TIl the dimensions of a reciprocal concentration (see Â§ 6.5).
Rheology of suspensions
122
50
[Chap. 7
~~
4o
~
~~301
r20          ~ 110 j 10 0 L.._'__'_ _ ' _ _....L.._J
o
02
0路4 06 08 Fraction of large particles
],0
Fig. 7.4 Effect of binary particlesize fraction on suspension viscosity, with total % phase volume as parameter. The particlesize ratio is 5: 1. P ~ Q illustrates the fiftyfold reduction in viscosity when a 60% v/v suspension is changed from a mono to a bimodal (50/50) mixture. P ~ S illustrates the 15% increase in phase volume possible for the same viscosity when a suspension is changed from mono to bimodal.
intrinsic viscosity for an ideal dilute suspension of spherical particles. Replacing it by [11] allows particles of any shape to be accounted for. The KriegerDougherty equation is (7.7)
Equations 7.6 and 7.7 both reduce to the Einstein equation (eqn. (7.2)) when ct> is small. The values of ct>m obtained from the empirical use of eqn. (7.7) are strongly dependent on the particlesize distribution. Thus, ct>m increases with increasing polydispersity (i.e. the spread of sizes). This is illustrated by Fig. 7.4 where the viscosities of mixtures of large and small particles are plotted as a function of the total phase volume. The large reduction in viscosity seen near a fraction of 0.6 of large particles is known as the Farris effect. The effect is very large at a total phase volume of more than 50%. Mixing particle sizes thus allows the viscosity to be reduced whilst maintaining the same phase volume, or alternatively, the phase volume to be increased whilst maintaining the same viscosity. Similar effects can also be shown for tertiary mixtures (d. Fig. 7.5). In the example shown in Fig. 7.5 the minimum relative viscosity is approximately 25 for the optimum tertiary mixture and is over 30 for the binary mixture. All these effects can be predicted using eqn. (7.7) by assuming, for instance, that the small particles thicken the continuous phase
7.2]
FINE
Solid particles in Newtonian liquids
7·0 0
0·7
0·2
0·3
0,4
0·5
0·6
0·7
0·8 O·g
123
0 7·0 COARSE
Fig. 7.5 Effect of particlesize distribution on trimodal suspension viscosity. Contours show values of the relative viscosity at 65% total solids (from the theoretical relationship of Farris (1968).
and the nextsizeup particles then thicken this phase; the result for a binary mixture being
(7.8) Most suspensions of industrial interest have a continuous distribution of particle sizes which often fit some empirical mathematical expression. However no information is available in the rheological literature on how the parameters of such a fit control eJ>m' Each system has therefore to be measured and eJ>m found by nonlinear curve fitting. Once eJ>m is found for any practical suspension, it is a useful parameter to assess the effect on viscosity of changing the dispersed phase concentration or the continuous phase viscosity. Thus far, we have concentrated on the effect of spherical particles on the viscosity of suspensions. However, particle asymmetry has a strong effect on the intrinsic viscosity and maximum packing fraction, and hence on the concentration/viscosity relationship. A number of studies have shown that any deviation from spherical particles means an increase in viscosity for the same phase volume. Figures 7.6 and 7.7 illustrate this point. It will also be seen that, generally speaking, rods have a greater effect than discs in increasing the viscosity. This is in accordance with theory, at least as far as it goes for dilute suspensions. Barnes (1981) provides simple empiricisms for the effect of very large axial ratio on the intrinsic viscosity [11]. These are discs: [11]
=
3 (axial ratio)/10,
(7.8a)
rods: [11]
=
7 [(axial ratio)5/3]/100.
(7 .8b)
Rheology of suspensions
124
[Chap. 7
50 Ul
& E:
"
I:'
1.0 30
b
"Vi 20 o u
':!!
:::. ]0
]0 20 30 Percentage volume concentration
t.O
Fig. 7.6 Dependence of the viscosity of differently shaped particles in water on concentration at a shear rate of 300s 1 (from Clarke 1967). (.) spheres; (0) grains; (e) plates; (0) rods. (See Table 7.2.)
5
00
]0 20 Percentage phase volume
30
Fig. 7.7 Dependence of the relative viscosity of glass fibre suspensions of various length/diameter ratios (L/ D) (d. Giesekus 1983). (......) spheres; (000) L/D = 7; (vvv) L/D = 14; (ITIJ) L/D = 21 (see Table 7.2).
Table 7.2 gives the values of [11] and <Pm obtained by fitting the results of a number of experimental investigations on suspensions of asymmetric particles using eqn. (7.7). The trend to higher [ 11] and lower <Pm with increasing asymmetry is clearly seen, but the product of the two terms changes little. This fact has practical value in making estimates of the viscosity of a wide variety of suspensions. The values of [11] are qualitatively in line with the predictions of eqns. (7.8a) and (7.8b).
7.2]
Solid particles in Newtonian liquids
125
TABLE 7.2 The values of [11] and ~ for a number of suspensions of asymmetric particles, obtained by fitting experimental data to eqn. (7.7) System
[11]
q.m
[11]q.m
Reference
Spheres (submicron) Spheres (40 J.Lm) Ground gypsum Titanium dioxide Laterite Glass rods (30 X 700 J.Lm) Glass plates (100 X 400 J.Lm) Quartz grains (5376 J.Lm) Glass fibres: axial ratio7 axial ratio14 axial ratio21
2.7 3.28 3.25 5.0 9.0 9.25
0.71 0.61 0.69 0.55 0.35 0.268
1.92 2.00 2.24 2.77 3.15 2.48
de Kruif et at. (1985) Giesekus (1983) Turian and Yuan (1977) Turian and Yuan (1977) Turian and Yuan (1977) Clarke (1967)
9.87
0.382
3.77
Clarke (1967)
5.8
0.371
2.15
Clarke (1967)
3.8 5.03 6.0
0.374 0.26 0.233
1.42 1.31 1.40
Giesekus (1983) Giesekus (1983) Giesekus (1983)
7.2.4 Concentrated shearthinning suspensions Although the theory described above (see eqn. (7.6)) was derived for the spherically symmetrical radial distribution function, i.e. the very low shear rate case, it has been found to work surprisingly well over a range of shear rates for which the structure is anistropic. It accommodates these situations by allowing [Til and cf.>m to vary with shear rate, thus accounting for shearthinning by the fact that the flow brings about a more favourable arrangement of particles. The tendency to form twodimensional structures rather than three is one such favourable rearrangement. Considering first the viscosityjphase volume relationships at very low and very high shear rates, it is found that they both fit the KriegerDougherty equation. 10 3 , . .                     ,
1),1路loc
~_L
OJ
~l
02
1
03
~~_'
Of. Phase volume, <P
_ _''
05
06
Fig. 7.8 Relative viscosity versus phase volume for monodisperse latices. Data points arc those of Krieger (1972) and de Kruif et at. (1985) combined. The upper line relates to the zero shearrate asymptotic relative viscosity, and is the best fit to the KriegerDougherty eq. (7.7) with q.m = 0.632 and [11] = 3.133. The lower line relates to the high shearrate asymptotic value of relative viscosity and is the best fit to eqn. (7.7), with q.m = 0.708 and [11] = 2.710.
Rheology of swpensions
126
[Chap. 7
Combining data from Krieger (1972) and de Kruif et al. (1985) (Fig. 7.8) the values of ct>m and [rll pertinent to the two situations are
ct>m(Y ~ 0) = 0.632, [11]( y ~ 0) = 3.13, ct>m( y
~
(0) = 0.708, [11]( y
~
(0) = 2.71.
Secondly, a number of workers have found that not only can viscosity be related to phase volume at the extremes of shear rate, but at intermediate values as well. However, it is usually necessary in this case to correlate values of viscosity measured at the same shear stress, not shear rate. A further reduction of data is possible following the suggestion of Krieger (1972). He recognised that although ct>m and [11] are stressdependent, they are independent of particle size. In order to relate the viscosity of different particlesize suspensions, he suggested that, instead of shear rate, a new variable be used, namely (7.9) where a is the particle radius, (J the shear stress and kT the usual unit of thermal energy. Krieger was able to show that for noninteracting suspensions, the viscosity/shear stress curves for submicron suspensions are reducible to a single curve (Fig. 7.9) whatever the particle size, temperature and continuous phase viscosity. The" Krieger variable" is dimensionless and is in fact a modified Peclet number *. Krieger realised that the viscosity of the suspension is more relevant than that of the continuous phase in accounting for concentrated suspensions. The shape of the curve of viscosity versus Pe in most cases follows the empirical Ellis model: 11  11':10 110  11':10
=
1 1 + b( Pe)P
,
(7.10)
where band p are dimensionless quantities (see §2.3.2 and the footnote on p. 18). 26,. • • 
... .22
r::
BENZYL ALCOHOL CRESOL WATER
~
'Vi
8 18
.!(l ~
~
:.:: o Qj Q::
14 10 "'''''_'_J 0·01 0'03 01 030 1'0 3·0 10·0 30·0
Peelef number.
Pe
Fig. 7.9 Composite curve of relative viscosity versus modified Peclet number (see eqn. (7.9». Points are for 0.10.5 J.Lm latex particles dispersed in two solvents; the solid line is for the samesized particles dispersed in water; the volume fraction is 0.50 (reproduced from Krieger 1972).
* The Pl:clet number is the ratio of the viscous force experienced by a particle to the Brownian force.
7.2]
Solid particles in Newtonian liquids
127
7.2.5 Practical consequences of the effect of phase volume I Weighing errors An examination of eqn. (7.7) will show that~ at phase volumes less than about 30% concentration~ the viscosity changes slowly with concentration~ and the viscosities at very low and very high shear rates~ respectively~ are essentially the same~ i.e. dilute suspensions are basically Newtonian. However~ at values of cj> around 0.5~ small changes in either cj> or cj>m give large changes in viscosity and alter the degree of shearthinning. Thus~ small errors in the weighing involved in the incorporation of the particles making up the suspension can give very large variations in viscosity~ (see~ for example~ Fig. 7.10). Also~ as is often the case in polymer latices after their manufacture, the absorption of small amounts of the suspending phase into the suspended phase can cause large changes in the viscosity of concentrated suspensions. Even half of one percent lost from the continuous phase to the suspended phase means an increase in the phase volume of one percent, which can, in the case of high phase volume, lead to a doubling or more of the viscosity! When it is realised that this is equivalent to the particle size increasing by about 0.2%~ and that particle size measurement techniques are nowhere near able to detect such small changes, we see that viscosity is a very sensitive variable in concentrated suspenSIOns. II Effect of phase separation Any sedimentation or 'creaming' of the particles in a viscometer will result in an increase in the indicated viscosity. At phase volumes above about 0.5 this effect is extremely pronounced. III Wall effect Yet another factor which must be taken into account in rheometry, as well as in industrial situations~ is known as the" wall effect". This term covers the phenomena
JOOtJJ",
o
J0 "L..o....l.....l...JJ.sL...J..L...l.~:!6o'":"rL.J
o
Percentage phase volume
Fig. 7.10 Relative viscosity versus nominal phase volume showing the effect of a 1 % error in phase volume.
Rheology of swpensions
128
[Chap. 7
which lead to a reduction in concentration of a suspension adjacent to the solid wall of the flow channel. One such phenomenon arises from the geometric impossibility of arranging particles near a wall in the same way as they are arranged in the bulk. Another is a particle migration from regions of high shear rate to regions of low shear rate. The hydrodynamic redistribution of particles demonstrated by Segre and Silberberg (1962) is yet another. A number of approaches have been attempted to account for the wall depletion. Most use the concept of a layer of continuous phase only at the wall and the normal dispersion everywhere else, with the thickness of the depleted layer being of the order of the radius of the particles. The result of the wall effect in tube viscometers is a reduction in the measured viscosity, the reduction increasing as the tube radius is decreased. Figure 7.11 illustrates these effects for lubricating greases. 7.2.6 Shearthickening of concentrated suspensions Given the correct conditions, all concentrated suspensions of nonaggregating solid particles will show shearthickening. The particular circumstances and severity of shearthickening will depend on the phase volume, the particlesize distribution and the continuous phase viscosity. The region of shearthickening usually follows that of the shearthinning brought about by twodimensional layering. The layered arrangement is unstable, and is disrupted above a critical shear stress. The ensuing random arrangement increases the viscosity. The effect has been studied using an optical diffraction system (Hoffman 1972). The result in terms of viscosity/shear rate for a range of particle concentrations is shown in Fig. 7.12. A number of studies have shown that the critical shear rate for transition to shearthickening varies little with phase volume when the phase volume is near 0.50. However, at phase volumes much higher than this, the critical shear rate decreases, whilst at phase volumes significantly below 0.5, the opposite is true (see Fig. 7.13). 10 3 ,                , CALCIUM BASED GREASE fa)
10'
10 2
Shear ra fe.
i
10 3 /5 1
Fig. 7.11 (a) and (b): Viscosity measurements for greases measured in axial flow between parallel cylinders (plunger viscometer) using various annular gaps. Gap/mm: (1) 0.624; (2) 0.199; (3) 0.042. The viscometersize effect disappears at higher shear rates away from the" yield stress" region. (Bramhall & Hutton 1960).
7.2]
Solid particles in Newtonian liquids
129
"
57%
...o
~ U) tl'l
Q .J
Log shear rate
Fig. 7.12 Schematic representation of viscosity versus shear rate for shearthickening systems. with phase volume as parameter (d. Barnes, 1989).
.~ ~
o... ...o
III
.c: U) .
o

.~
.i:: <...>
o
45
50
55
Percentage phase volume
Fig. 7.13 Schematic representation of the dependence of the critical shear rate for the onset of shearthickening i e • as a function of the phase volume of the dispersed phase cp. 2·4 22
c: . 2D
~
·S J·8 ~
~
... J6
~
& 1·4 J 2 '_ _L.._l_ _l_ _I._ _J
30
32 34 36 38 Percentage phase volume
40
Fig. 7.14 The powerlaw index n for the shearthickening region of starch suspensions (after Griskey and Green 1971).
Rheology ofsuspensions
130
[Chap. 7
10 5 r                         ,
• • •• • •
..., •• •..
; 10 3 III
"'l'."U
~
2
~ 10' 'o CIi
II•• : • ••
..c:
III
§...... 10' 8
• • •
••
• •
102 ~...J.I__:__'_:_l..l 102 10' 10° 10' 10 2 Particle size,
d/lJm
Fig. 7.15 Shear rate for the onset of shearthickening Ye , versus particle size for suspensions with phase volumes around 0.5 (Barnes, 1989).
The level and slope of the viscosity/shear rate curve above the transltlOn increases with increase in particle concentration (see Figs. 7.12 and 7.14). Evidence is accumulating that the viscosity decreases again at very high shear rates, although experiments are difficult to carry out at very high phase volume due to flow instability. The ultimate decrease is readily observed at lower phase volume. For any phase volume around 0.50, it is found that the effect of particle size on the value of the critical shear rate is quite large. In fact, it is approximately proportional to the inverse of the square of the particle size (see Fig. 7.15). The viscosity of the continuous phase is also very important, and an increase in this viscosity decreases the critical shear rate. This reflects the greater relevance of shear stress (rather than shear rate) for the onset of shearthickening, (see Fig. 7.16).
10"
102
10'
10°
10'
10 2
10 3
Continuous phase viscosity" shear rate. tl s .j/Pa
Fig. 7.16 Envelope of flow curves for latices dispersed in various solvents whose viscosities vary from 18 mPa.s to 14 Pa.s. (Redrawn from Hoffman 1972.)
7.3]
90,~
250 (a) III
200
&
III
~ 150 ~ 100
I::"
'Vi
8
:::.
70
&
~
I::"
.!!!
131
The colloidal contribution to viscosity
A/B 50
0/100
.c
.~
50
100/0
u
!!! 30
:::. 2.000
4,000
         50/50
6.000
Shear rate, 7/5/
I0
4
10 r(C)         . . . ,
L......'~~:l~:__l..I.J
20,000 4QOOO
6QOOO
Shear rate. j /5/
narrow p.5.d.
10 2 '7..L......_ _..l...._ _  I
WO
W' Shear rate.
W2
W3
7/5 1
Fig. 7.17 (a) Viscosity of clays A and B at different ratios as a function of shear rate at a solids content of 44% by volume (67% by weight). Clay A 9 Jlm, clay B 0.7 Jlm. (Alince and Lepoutre 1983); (b) Viscosity of calcium carbonate blends at 48% solids content by volume (71.4% by weight) as a function of shear rate. Clay A 12 Jlm, clay B 0.65 Jlm. (Alince and Lepoutre 1983); (c) Effect of particlesize distribution. (Redrawn from Williams et at. 1979).
The severity of shearthickening is often alleviated by widening the particlesize distribution (see Fig. 7.17).
7.3 The colloidal contribution to viscosity 7.3.1 Overall repulsion between particles Overall repulsion between the particles of a suspension is created if the particles carry electrostatic charges of the same sign. The particles then take up positions as far from one another as possible. For flow to occur, particles have to be forced out of their equilibrium positions and induced to move against the electric fields of neighbouring particles into nearby vacancies in the imperfect lattice. Goodwin
Rheology ofsuspensions
132
[Chap. 7
1O"'''....L.I 10'8 10'7 Jo'6 JO 5 /0" Particle radius, a/m
Fig. 7.18 Particle size versus viscosity for a suspension of charged particles, for various particle phase volumes and charge. The viscosity is the sum of the two contributions given by eqns. (7.7) and (7.11). The value of E * used here is the difference in potential energy between the particle reststate and the maximum potential it experiences as it "jumps" to the next reststate site. The particle arrangement is assumed to be facecentred cubic. The charge on the particle is characterised by the value of K which is the inverse of the doublelayer thickness. This is a measure of the distance over which the electrostatic potential acts, measured from the particle surface.
(1987) has given the following equation to evaluate the extra contribution of repulsion to the zero shear·rate viscosity over and above the usual KriegerDougherty contribution: h .d1] = 3 exp(E* /kT), b
(7.11)
where h is Planck's constant, b is the centre·to·centre particle separation and E * is the activation energy calculated for selfdiffusion. This expression predicts very large (but finite) viscosities compared to the viscous contribution alone, as accounted for by the KriegerDougherty expression, (see Fig. 7.18). The effects of particle size and concentration are very strong, the latter being accounted for in the E* factor. Goodwin also suggests that shearthinning in such systems will become significant at a shear stress of the order of kT/b 3 • At very high shear rates, twodimensional layering occurs and the electrostatic contribution loses its dominance. The viscosity decreases towards that given by the KriegerDougherty expression for noninteracting particles. The range of the electrostatic forces is greatly decreased if electrolyte is added to the solution, so screening the charges on the particles. This means that using electrostatic forces to thicken suspensions is limited to very pure systems, since slight electrolyte contamination can give a large decrease in viscosity. Repulsion can also arise from the entropic forces caused by the interaction of the chains of any polymer adsorbed onto the particle surfaces. Although not always
7.3)
The col/oidal contribution to viscosity
133
operating over great distances from the particle, they can affect the viscosity at high phase volumes. 7.3.2 Overall attraction between particles The formation of flocs traps part of the continuous phase, thus leading to a bigger effective phase volume than that of the primary particles. This gives an additional increase in the viscosity over and above that expected from the phase volume of the individual particles. When flocculated suspensions are sheared, the flocs rotate, possibly deform and, if the applied stress is high enough, begin to break down to the primary particles. Flocs sometimes take the form of chains which form networks throughout the liquid. The length of the strands is a function of the shear stress. All flocculated structures take time to break down and rebuild, and thixotropic behaviour is usually associated with flocculated suspensions; clay suspensions being classic examples. The driving force to rebuild the floc is Brownian motion, and since this increases with decrease in particle size, the rate of thixotropic change is a function of particle size. Thus, one expects systems of large particles to recover their viscosity slower than systems of small particles. Similarly largeparticle suspensions will break down faster under shearing. These considerations are important in the design of thixotropic products such as paints and printing inks. The attraction between particles can be reduced in a number of ways, including the adsorbtion of molecules onto the surface of the particles. Adding electrolyte to clay suspensions can reduce the differential charge effects. In all these cases, the viscosity is reduced substantially. Flocculated systems usually have very high viscosities at low shear rate, and are very shearthinning, often giving the impression of a yield stress (see Fig. 7.19). In many cases the Bingham model has been used to describe their behaviour. 15r
o
Q
"b Vl
~ Vl
~
<II
5
t5
2000
1.000 Shear rate.
6000
i /5"
8000
Fig. 7.19 Shear stress/shear rate curves for 1.5% byweight suspensions of bentonite Superge1 in water (0%), and with 0.2% and 1.5% sodium chloride additions. The corresponding curve for pure water is shown for comparison (Ippolito 1980).
Rheology of suspensions
134
[Chap. 7
7.4 Viscoelastic properties of suspensions Viscoelastic properties of deflocculated suspensions arise from particle interactions of all kinds. If these require a preferred arrangement of the particles at rest in order to fulfil some minimum energy requirement, there will always be a tendency for the suspension to return, or relax, to that arrangement. It is possible to make small perturbations about the preferred state by means of smallamplitude oscillatoryshear experiments. In this case the measure of elasticity is the dynamic rigidity G' (§ 3.5). Figure 7.20 shows a typical example of such behaviour. 160r~~~,/600 II)
o
o
Q..
Q..
." 120
1200 "
o
' ' '" 800
£ :g l> II)
~
400 .~
~
c
a
':;~~
102
/03
J:
';;
10 I
100
L:,
a S
la'
Osciffotory frequency. Hz
Fig. 7.20 Dynamic viscosity 1/' and dynamic rigidity G' as functions of frequency for polystyrene latex in 10  2 M NaCI aqueous solution ep = 0.35, particle radius = 0.037 Ilm. (J. Goodwin, private communication.) (a) II)
,
c:i
10 3 Q..
"""
~
102iij 0
U
~ /0' (b) I/)
"
....:.10·' Q>
! ~/O} o ~
o
Ql
Q: 10 3 '_ _"_ _L..,,_'_ _"_ _J
10}
10'
/00
10
'
102
Shear rate. ; /s'
Fig. 7.21 (a) Normal stress and viscosity versus shear rate for a PVC organosol (ep = 0.54) dispersed in dioctyl phthalate; (b) The relaxation time (defined as A = Nl!oy) plotted against the shear rate derived from the data in (a). (Willey and Macosko 1978).
7.5]
Suspensions of deformable particles
135
Elastic effects are also observa~le in a steady simpleshear flow through normal stress effects (cf. Chapter 4). This is demonstrated for a typical colloidal system in Fig. 7.21. In general, the normal stresses found in colloidal systems are lower than those in comparable polymeric liquids.
7.5 Suspensions of deformable particles Many dispersions are made from deformable particles, the most obvious examples being emulsions and blood. In dealing with the rheology of these systems, all the earlier factors like interparticle forces are relevant, but the effect of phase volume is not so extreme as with solids. The maximum phase volume is usually much higher than with solid particles since the particles deform to accommodate the presence of near neighbours. In this situation, the shape of the particles is polyhedral and the suspension resembles a foam in its structure. Maximum packing fractions of 0.90 and above are usual (Pal et al. 1986). Figure 7.22 shows the viscosity/shear rate profiles for typical emulsions. The familiar shape seen for solid dispersions is again apparent as is the increasingly nonNewtonian behaviour with increase in concentration. However, the asymptotic value of viscosity at high shear rate is generally much lower than that observed for a dispersion of solid particles at the same phase volume. This effect is ascribable to particle deformation in the emulsion (see, for example, Fig. 7.23 and compare Fig. 7.8). Whereas many model studies have been carried out on monodisperse solid particle dispersions, the usual mode of production of emulsions by droplet breakup means that making monodisperse dropletsize samples is difficult. Therefore, model studies have not always been able to distinguish between the relative effects of droplet size and the shape of the dropletsize distribution. What is clear however is 10 3 r                    ,
% OIL
~_
:
10 3
~
...... 75
~60
••• II
........• •
• 50
~
~J;O
X
0> 09>
~
0
30
L......I...._.J....>_....LL_'''::''
103
10" 10' Shear ra fe.
i / s"
10 3
105
Fig. 7.22 Viscosity versus shear rate for emulsions of silicone oil in water at various values of phase volume of oil.
Rheology of suspensions
136
[Chap_ 7
10 5 r           .
10'
.
I:'"
. 10 3 ~
"~
7:::100
rJ400
u
~ 10 2 Ql
'....
I
~
.!:? ~ 10'
10째 ~'~''' o 04 08 Phose volume. 4J
Fig. 7.23 The relative viscosity of a wideparticlesize emulsion (see Pal et al. 1986) for a range of shear rates. Note the onset of shearthinning is at ep  0.55 for this particular sample; cr. Fig. 7.22 where the emulsion is not so polydisperse and shearthinning begins at ep  0.4.
that a smaller droplet size and a more monodisperse droplet size both give an increase in viscosity. Since vigorous mixing of emulsions usually gives smaller and more monodisperse particles, increasing the energy input in emulsion manufacture always increases the viscosity. Theoretical work carried out by Oldroyd (1953) for very dilute emulsions showed that viscoelasticity results from the restoring force due to the interfacial tension between the continuous and disperse phases. The emulsion droplets at rest are spherical, but become ellipsoidal in shear, with a consequent increase in the surface area. Solid particles stabilised by adsorbed polymers can appear as deformable particles when the particle size is very small (say < 100 nm). In this case the deformable stabilising layer can form a considerable proportion of the real phase volume. The overall effect is that the viscosity is a decreasing function of nominal particle size, when evaluated at constant phase volume (based on uncoated particles). In this case however the phase volume must be adjusted to take account of the stabilising layer. This can be obtained by measuring the viscosity of very dilute suspensions and applying Einstein's equation (eqn. (7.2)). 7.6 The interaction of suspended particles with polymer molecules also present in the continuous phase There are at least four ways in which particles and polymer molecules interact: (i) Neutrally. That is, the polymer merely acts as a thickener for the continuous
7.7]
Computer simulation studies of suspension rheology
137
phase and the particles as inert fillers. The only overall effect is an increase in viscosity. Examples of this are found in various toothpastes. (ii) For specific polymers (e.g. block copolymers), some part of the polymer
molecule adsorbs onto the particle while the other protrudes into the liquid phase. This can have the effect of hindering any flocculation that might take place, especially with very small particles, and hence prevent any ensuing sedimentation or creaming. The interacting polymer chains of adjacent particles overlap and cause entropic repulsion because their local concentration is higher than the average. Emulsion and dispersion stabilisers such as Gum Arabic are examples showing this phenomenon. (iii) Certain polymers have the ability to anchor particles together. This is called
"bridging flocculation". They are usually very high molecularweight macromolecules with groups that attach to the particles by unlike charge attraction. These are deliberately introduced to cause flocculation in separation processes. An example is the use of the polyacrylamide family of polymers in waterclarification plants. The flocs formed by bridging flocculation are relatively strong and can withstand quite high stresses before breaking down. (iv) Some situations arise where polymers in the continuous phase can cause
flocculation of the particles. This "depletion flocculation" arises when polymer molecules, because of their finite size, are excluded from the small gap between neighbouring particles. The concentration difference thus caused between the bulk and the gap causes an osmotic pressure difference. This results in solvent leaving the gap, thus pulling the particles together. This in turn means that even more polymer becomes excluded and the effect grows. Eventually the particles are completely flocculated. The floc strength of such a system is relatively small, certainly as compared to (iii) above. There must always be a tendency for this to occur in any system, but the time scale of the particle movement and the level of the force makes it possible to ignore it in some circumstances.
7.7 Computer simulation studies of suspension rheology
The computer simulations of flowing suspensions have been reviewed by Barnes et al. (1987). The simulations are not dissimilar to computer simulations of simple liquids such as argon and chlorine. Both simulations use the Newtonian equations of motion and a LennardJones type of particleparticle interaction law. The main differences are that the interparticle forces are smaller and the hydrodynamic resistance to motion is much greater for the suspensions. The techniques of nonequilibrium molecular dynamics (NEMD) consider an assembly of particles which is given an initial set of positions in space and a set of
Rheology of suspensions
138
[Chap. 7
velocities. Assemblies of between one hundred and a few thousand can be dealt with. The NEMD calculation is the reevaluation of the positions and velocities over a succession of short intervals (see, for example, Reyes 1986). From this information the stress tensor can be calculated, hence the viscosity and the normal stress differences. Given the similarities of approach, it is not surprising that the main results for simple liquids and suspensions are similar. Following a lower Newtonian region the systems display shearthinning. At still higher shear rates the simulations predict shearthickening. Considerable support for the existence of flowinduced structures in the shearthinning region is provided by NEMD. The simulations show that suspensions of spherical particles form twodimensional layers which break up at the onset of shearthickening. The corresponding results in simple liquids are the formation of
10 '
(0)
III
0
a... 100 "l':"'
;,.,
'Vi 10 1 0
u
VI
s:
...0
10'2
DENSITY
Ql
.c:
a
•
IO'J
10 0
10"
& IO J ....
0
VI
c:
~
...Ql:::l
OJ OS Og
0
V)
10 2
J 1O' 10 2 10 Shear rate. ;/s',
DENSITY 0
OJ
"a v •
0,'
••
OS 0'/5 07 08
O·g
VI VI Ql
5..
1O'
~
0
Ql
U 0
~
100 1O"
10
0
2
1O' 10 Shear rate. ;/s"
10
J
10'
Fig. 7.24 Typical predictions from a computer simulation of a suspension in shear flow (see Barnes, Edwards and Woodcock 1987). Note: density is normalized using particle parameters. (a) Viscosity versus shear rate, showing the qualitative features of Fig. 7.1; (b) Shows the trace of the stress tensor. This osmotictype pressure results in particle migration to regions of lower shear rate.
7.7]
Computer simulation studies of suspension rheology
139
strings of molecules aligned in the direction of flow and, for diatomic and longer molecules, an additional alignment of the molecules. The normal stress components are unequal at shear rates in the shearthinning region and the differences increase with shear rate. The increase is slow compared with that predicted by polymer theory. Very little normal stress data have been obtained by NEMD and N} and N 2 generally show a considerable scatter. The results are often presented in terms of the trace of the stress tensor. This is also referred to as an osmotic pressure. Typical results are shown in Fig. 7.24 where the predicted osmotic pressure and viscosity of a dense suspension of submicron particles is shown as a function of shear rate. The technique of computer simulation is likely to become more important in the future, especially in its ability to study complicated but idealized systems.
CHAPTER 8
THEORETICAL RHEOLOGY
8.1 Introduction
An alternative title to this chapter could be "Constitutive equations and their uses" since it summarizes the vast majority of published work in theoretical rheology. The theoretician seeks to express the behaviour of rheologically complex materials through equations relating suitable stress and deformation variables. Such equations are of interest in themselves and continuum mechanics, which addresses such matters, is a respectable subject in its own right which occupies the attention of many theoreticians. The relevant equations, called constitutive equations or rheological equations of state, must reflect the materials' microstructure and one fruitful area of study concerns the search for relationships between microstructure and (macroscopic) constitutive equations. We have already touched on this subject in ยง6.8 and the reader is referred to the important books of Bird et al. (1987(b)) and Doi and Edwards (1986) for further details. Constitutive equations, which satisfy the basic formulation principles to be discussed in ยง8.2 and are constrained either by microstructure considerations or by the way the fluids behave in simple (rheometrical) flows, are also used by theoreticians to predict the way the relevant fluids behave in more complex flows of practical importance. Here, the constitutive equations are solved in conjunction with the familiar stress equations of motion and the equation of continuity, subject to appropriate boundary conditions. This is an important branch of nonNewtonian fluid mechanics and is discussed briefly in ยง8.7. Practical scientists and engineers may also look to constitutive equations for more modest reasons. For example, they may be interested in reducing experimental data to the knowledge of a small number of material parameters. This can be accomplished by comparing the forms of graphs relating, for example, viscosity/ shear rate and/or normal stress/shear rate with the corresponding predictions from likely constitutive equations. It is not difficult to make out a case for a detailed study of theoretical rheology and many books are either devoted to the subject (like that of Truesdell and Noll 1965) or have substantial sections dealing with it (e.g. Lodge 1974, Bird et al. 1987(a), Schowalter 1978, Tanner 1985, Astarita and Marrucci 1974 and Crochet et al. 1984). We have left the subject to the final chapter of the present book for 141
142
Theoretical rheology
[Chap. 8
specific reasons, which have already been alluded to in Â§1.5. The subject is a difficult one by common consent and newcomers to the field (especially those without a mathematical background) are often put off by the complexity of the mathematics. In previous chapters we have attempted to cover the various strands of rheology without involving ourselves with intricate modern continuum mechanics, but it is now time to address this important subject and to point the interested reader in the direction of the many detailed texts and authoritative works on the subject. At the same time, sufficient attention is given to the subject in the present chapter to indicate to the reader, by way of an overview, the most important features of presentday knowledge of continuum mechanics. For most readers this will be all that is required. For others, the growing list of available books on the subject is more than adequate for further detailed study. In this connection we recommend particularly the books by Bird et al. (1987(aÂť, Schowalter (1978) and Truesdell and Noll (1965). Particular backgrounds and tastes vary greatly and many readers will no doubt obtain significant benefit from the theoretical sections in the other texts mentioned above. The following discussion is limited to isotropic, timeindependent nonNewtonian fluids. Readers interested in anisotropic fluid behaviour should consult the papers of Ericksen and Leslie (see, for example, Leslie 1966, 1979, Jenkins 1978). Those interested in thixotropy and antithixotropy are referred to the review article by Mewis (1979). The amount of theoretical literature on timedependent materials is limited. The considerable conceptual difficulties in the subject are no doubt largely responsible for this deficiency.
8.2 Basic principles of continuum mechanics We seek equations for complex nonNewtonian fluids (with or without fluid memory). To facilitate this, we need to define suitable stress and deformation variables and consistent timedifferentiation and integration procedures. The relevant formulation principles required for this purpose are now welldocumented and are not controversial. However, a cursory glance at the literature may give the reader the mistaken impression that there are two distinct kinds of formulation principles, one associated with the names of Oldroyd, Lodge and their coworkers and the other with the names of Truesdell, Noll, Coleman, Green, Rivlin, Ericksen and their coworkers. Certainly, the way the formulation principles are expressed and applied varies between these groups, but there have been sufficient objective reviews in recent years to prove to the perceptive newcomer to the field that the formulation principles of continuum mechanics have an invariance which is independent of the researcher! They can be expressed in different ways, but there is no essential controversy concerning the two basic approaches referred to and Chapter 2 of the text by Crochet et al. (1984), as well as discussions in other books, should convince the reader of this fact (see also the paper by Lodge and Stark 1972).
8.2]
Basic principles of continuum mechanics
143
We may summarize the formulation principles as follows: Principle I. The constitutive equations must be independent of the frame of reference used to describe them. Expressing the equations in consistent tensorial form will ensure that this principle is automatically satisfied and, in a real sense, this principle is required of all physical theories. Principle II. The constitutive equations must be independent of absolute motion in space (Oldroyd 1950). Any superimposed rigid body motion cannot affect the basic response of the material *. Principle III. The behaviour of a material element depends only on the previous history of that same material element and not on the state of neighbouring elements (Oldroyd 1950). Expressed in an alternative waythe stress is determined by the history of the deformation, and the stress at a given material point is uniquely determined by the history of deformation of an arbitrarily small neighbourhood of that material point (see, for example, Astarita and Marrucci 1974). The basic feature of principle III is that "fluid memory" as a concept must be associated with material elements and not with points in space.
To illustrate how these principles (especially I and III) apply in situations already discussed, consider again the general integral equations of linear viscoelasticity which were introduced in ยง3.4. These can be written in the tensorial form * *
(8.1)
where T;k is the extra stress tensor; d ik the rateofstrain tensor; p is an arbitrary isotropic pressure; 8ik is the Kronecker delta, which takes the value zero for i =1= k
... Coleman and Noll et al. define a principle called "the principle of material objectivity", which requires that the frame indifference of principle I must also apply to a timedependent frame (see, for example, Truesdell and Noll 1965, Astarita and Marrucci 1974). In other words, it is principles I and II combined. ...... In this chapter we shall be forced to use general tensor analysis. We employ the usual notationcovariant suffices are written below, contravariant suffices above, and the usual summation convention for repeated suffices is assumed. The need to distinguish between covariance and contravariance is made dear in the detailed texts on theoretical rheology (e.g. Lodge 1974). In rectangular Cartesian coordinates, we note that it is not necessary to distinguish between covariant and contravariant components. For readers meeting tensor analysis for the first time, we recommend a study of Foster and Nightingale (1979, pp. 114) Spain (1960, pp. 811) and Bird et al. (l987(a), pp. 597606).
144
Theoretical rheology
[Chap. 8
and unity for i = k; t is the present time and t' an earlier time. ! stands for xl, x 2 and x 3 , the Cartesian coordinates of a fixed point in space. In the corresponding onedimensional version of (8.1) given in Chapter 3 (eqn. (3.21Âť, the dependence on ! was not made explicit, but it was implied. The reason for this was that the strains for which the linear theory applied were so small that the particles occupied essentially the same position in space throughout the deformation. If we attempt to use (8.1) under all conditions of motion and stress, we would arrive at the unphysical conclusion that the stress in the particle which is at the point! in space at the present time t is determined by the history of the rate of strain in all the particles which were at the same point at previous times t'. One simple (but incorrect!) way around this problem is to introduce the socalled displacement functions X,i (defined such that X,i (i = 1, 2, 3) is the position at time t' of the element that is instantaneously at Xi at time t) and to write (8.2) where d ik now relates to the position !'. This equation is certainly in sympathy with principle III since it relates "memory" to "particles" rather than "points in space", but eqns. (8.2) now equate a tensor at the point! with a tensor at the point !' and this violates principle I, so that the satisfaction of the formulation principles (and the above discussion refers to only two of them) is clearly nontrivial. The corresponding differential equations of linear viscoelasticity are also invalid under general conditions of motion and stress. Take, for example, the threedimensional form of the simple Maxwell model given by (8.3) The partial derivative, by definition, refers to the way the stress variable is changing with time at a particular point in space and, at the very least, this must be replaced by the convected (Lagrangian) time derivative D jDt of hydrodynamics, in order to accommodate changes in a fluid element, where
(8.4) vm being the velocity vector. However, yet again, the situation is not that simple and the correct application of principle II requires time derivatives of greater complexity than (8.4). These will be introduced later. Principles I to III are of fundamental importance in the formulation of rheological equations of state; however, we would also wish such equations to satisfy two further principles:
8.3]
Applications offormulation principles
145
Principle IV. In the case of elastic liquids, the deformation history of a material element in the distant past must be expected to have a weaker influence on the current stress response than the deformation history of the recent past. This is known as "the principle of fading memory". Principle V. The equations must be consistent with thermodynamic principles. Astarita and Marrucci (1974, p. 52) show that there are pitfalls in developing a purely mechanical rheological theory without due regard being paid to thermodynamics. For instance, the principle of "positive dissipation" can provide useful constraints on constitutive equations. At the same time, much of the literature which attempts to apply thermodynamics in a general way to continuum mechanics has not been too successful and much of it is controversial.
8.3 Successful applications of the formulation principles In his classic 1950 paper, Oldroyd sought to satisfy the basic principles of formulation by introducing a convected coordinate system embedded in the material and deforming continuously with it, so that a material element which is at ~j at one instant is at the same point (with respect to the convected coordinate system) at every other time. Oldroyd argued that, provided one works in a tensoriallyconsistent manner in the convected coordinate system, the basic principles IIII are automatically satisfied, since using (~\ ~2, t') as independent variables essentially satisfies the need to concentrate on fluid elements; thus moving away from the more usual "Eulerian" preoccupation with fixed points in space. coordinate system is unaffected by absolute (rigid body) motion in Further, the space and principle II is satisfied automatically (provided, of course, that operations like time differentiation and integration do not introduce any unwanted dependence on absolute motion in space). In this connection we note that a time derivative D /Dt holding convected coordinates constant is a convenient and valid differential operator. The metric tensor Yj/(~' t') of the ~j system was taken by Oldroyd as the fundamental deformation variable *, since, in the usual definition,
e
e,
e
(8.5) and Yj/(t t') clearly provides a convenient measure of the distance ds(t') between the parts of the arbitrary element at Oldroyd (1950) showed how his general theory could be used by means of some simple examples. One example was the socalled liquid A, which obeyed the
e.
* The contravariant metric tensor White 1964).
yJI
can also be used for this purpose (see, for example, Truesdell 1958,
Theoretical rheology
146
[Chap. 8
differential constitutive equation:
(8.6) where 'Ij/(t t) is the extra stress tensor in the convected coordinate system * and 11o, Al and A2 are material constants. Another example was the integral model called liquid 1\:
'Ij/
(ยง, t ) f =
t
</>
(
t t
')
DYjI ( ,) , Dt' ยง, t dt.
(8.7)
00
Having written equations in the convected coordinate system ~i, Oldroyd showed how to transform equations like (8.6) and (8.7) into the fixed laboratory coordinate system Xi. The relevant transformation rules for so doing were given by Oldroyd (1950). For example, the D IDt time derivative of the differential models in convected coordinates must be replaced by the "codeformational" derivative b/bt, where, for a symmetric covariant tensor bik , we have (8.8) and for a symmetric contravariant tensor b ik , the relevant form is (8.9) The derivative b/bt in eqns. (8.8) is often called the lower convected derivative and that given in eqns. (8.9) the upper convected derivative. The symbol fj. over the tensor being differentiated is usually employed for the lower convected derivative and the symbol \l for the upper convected derivative. Oldroyd (1950) also showed that terms like DYj/(~' t')/Dt' in integral models like (8.7) need to be replaced by their socalled "Eulerian fixed components". For example, Yj/(t t') has to be replaced in the fixed coordinate system Xi by G ik , where 
a ,m a ,r
G.=_X_~ lk
aX i
aX k
(x')
gmr 
(8.10)
,
* In his development, Oldroyd used, for consistency and convenience, Greek letters for tensor variables in the convected ~j system and Roman letters for tensor variables in the fixed
Xi
system.
8.3]
Applications of formulation principles
147
gik being the metric tensor of the Xi coordinate system. When the fixed coordinate system is Cartesian, we have gmr = 8mn the Kronecker delta, and hence
(8.11 ) The equivalent stress tensor in fixed laboratory coordinates for liquid A' is
( ) f ' ep (t  t
T;k :!, t = 2
00
I )
a
,m
a
Ir
X X , ,. a k d mr (:!' ,t I ) dt. ax x
(8.12)
We remark that the contravariant equivalents of (8.6) and (8.7) are called liquid B and B / , respectively, and are given in fixed coordinates by (8.13) and T ik ( :!, t )
=
2
.
k
f' ep (t  t ') aax,m a ax d x x l
Ir

mr( :!, I
t ') d t I ,
(8.14)
00
respectively. Oldroyd introduced models like the A and B series to illustrate the general theory, but their introduction gave the impression to some workers in the field that his formulation work was in some sense not completely general. This is now acknowledged to be a mistaken impression, but at the same time it is interesting to note that simple models like liquid B and liquid B' have figured prominently in modem developments in the numerical simulation of nonNewtonian flow (see, for example, Crochet et al. 1984). Some of the rheometrical consequences of Oldroydtype models are given later in Table 8.3. For an updated version of Oldroyd's work on formulation, the reader is referred to the review article published posthumously in a commemorative volume (Oldroyd 1984). The application of the formulation principles in the work of Coleman and Noll et al. takes a somewhat different path. Some general hypothesis is made on the relationship between stress and deformation. The formulation principles, applied within a Cartesian coordinate framework, are then used either to supply the resulting equations or at least to provide constraints on them. We shall refer to this procedure as "the formal approach". Occurring quite naturally in the development of Coleman and Noll et al. is the Eulerian fixed component equivalent of the tensor Yj/' given in Cartesian coordinates by (8.11) and called the CauchyGreen tensor. Also of importance is the
Theoretical rheology
148
[Chap. 8
series expansion of G ik in terms of the socalled RivlinEricksen (1955) tensors A(n).
ik .
G ik ( :!, t, t
')_ ;. (tt ' )i(l)i (j)  ~ ., A ik . , 0 J. J=
(8.15)
The RivlinEricksen tensors are related to the (lower convected) time derivative of Oldroyd through (8.16)
In a later development, White and Metzner (1963) derived the contravariant equivalents of the Rivlin Ericksen tensors involving the Finger tensor F ik in place of the CauchyGreen tensor G ik , where, in Cartesian coordinates, (8.17)
The resulting tensors have become known as the White Metzner tensors and have an obvious counterpart to (8.16) with the upper convected Oldroyd derivative given by eqns. (8.9) replacing that in eqns. (8.16) (see, for example, Walters and Waterhouse 1977). We may conclude that the basic framework of Oldroyd is matched in the developments of Coleman, Noll, et al. and any differences in the application of the various techniques result from the particular outlook adopted rather than from any fundamental disagreement. The variables and operations needed to construct rheological equations of state are now known and it is simply a matter of employing and applying these within the context of certain constitutive proposals. In these proposals there may be a preoccupation with generality or, alternatively, a search for simplicity. A compromise between the two is also a possibility. If our concern is with generality, we may write
~k ( t)
t
g;
= 
00
[Gjl (t ') 1'
(8.18)
which expresses mathematically the requirement that the stress at time t is determined in a very general way by the history of the deformation. g; is called a tensorvalued functional, and in the equation, the stress at time t is to be viewed as a function of the deformation measure, which is itself a function of the time variable t ' with  00 < t ' .:s;; t. The integrals in (8.12) and (8.14) are (simple) examples of a functional. When certain formal requirements of functional analysis are added to eqns. (8.18), we obtain the so called "simple fluid" of Coleman and Noll, which has had
8.4]
Some general constitutive equations
149
an influential impact on constitutive theory (see, for example, Truesdell and Noll 1965). On account of their generality, eqns. (8.18) have limited predictive utility in nonNewtonian fluid mechanics and, not surprisingly, simpler equations have been sought. These arise from three distinct approaches: I. One may relax the complete universality embodied in eqns. (8.18) but still make constitutive assumptions of some generality. Such developments are considered in ยง8.4. II. One may consider approximations arising from simplifications in the flow so that G jl in eqns. (8.18) has a relatively simple form. These approximations lead to general equations of state for restricted classes of flow. They are discussed in ยง8.5. I I I. One may consider special (usually very simple) choices of the functional g;. These lead to particular equations, which are nevertheless valid under all conditions of motion and stress. Examples of this sort are considered in detail in"ยง8.6.
8.4 Some general constitutive equations
The formal approach was used by Reiner (1945) and Rivlin (1948) in a search for the most general constitutive equations for inelastic nonNewtonian fluids. The resulting model, which has become known as the ReinerRivlin model, has constitutive equations of the form (8.19) where 12 and 13 are the two nonzero invariants of the strainrate tensor d ik . The behaviour of the Reiner Rivlin model in a steady simpleshear flow can be easily determined. Surprisingly for an inelastic model, it predicts normal stresses. However the resulting normal stress distribution (viz. N l = 0, N 2 =1= 0) is not of a form which has been found in any real nonNewtonian fluid. Consequently, any normal stress differences found experimentally in a steady shear flow can be viewed as manifestations of viscoelastic behaviour (cf. Chapter 4). A simplified version of the ReinerRivlin fluid given by
(8.20) where
(8.21 ) has been given significant prominence in the rheological literature. It is familiarly known as the "generalized Newtonian model". The form of the invariant 12 given in
Theoretical rheology
150
[Chap. 8
(8.21) is chosen such that it collapses to the shear rate y in a steady simpleshear flow. The generalized Newtonian model can account for variable viscosity effects, through the function 11(12 ), but not normal stress differences. Therefore, it has an obvious application to fluids which show significant viscosity variation with shear rate, but negligibly small normal stress differences, and also to flow situations where variable viscosity is the dominant influence (even though normal stress differences may be exhibited by the fluids under test). In an influential development, Rivlin and Ericksen (1955) used the formal approach to derive constitutive equations based on the general proposition that the stress is a function of the velocity gradients, acceleration gradients... (n  l)th acceleration gradients. The resulting RivlinEricksen fluid has equations of state of the form
.
/ [A(1) Ti k rt.. jt,
A(2) j t · ..
A(n)] jt
,
(8.22)
where / is a function of the RivlinEricksen tensors introduced in (8.15). Useful constraints on the form of the function / have been found using routine matrix theory (see, for example, Truesdell and Noll 1965). In a series of papers, Green, Rivlin and Spencer (1957, 1959, 1960) developed integral forms of eqns. (8.18), the lowerorder approximations being essentially the same as the integral equations discussed in §8.5 (d. eqns. (8.26)(8.28». The socalled GreenRivlin fluids can be thought of as arising from a procedure analogous to the Taylorseries expansion of an analytic function (cf. Pipkin 1966) or, alternatively, from a direct application of the StoneWeierstrass theorem (d. Chacon and Rivlin 1964).
8.5 Constitutive equations for restricted classes of flows
There is no doubt that the simple fluid of Coleman and Noll has been the most influential application of the formal approach. The resulting equation is (8.18), with a suitably chosen function space and accompanying norm. In the original development, the function space(s) chosen by Coleman and Noll had certain limitations which were highlighted by Oldroyd (1965), who argued that the Newtonian fluid was not a special case of the simple fluid except in the limit of very slow flow. This, and related objections, have been overcome in the more recent work of Saut and Joseph (1983). Notwithstanding the original limitations mentioned above, the basic simple fluid hypothesis was studied to good effect by Coleman and Noll, who developed simplified constitutive equations for special classes of flows. Their most influential
8.5]
151
Restricted classes offlows
contribution applies to socalled "slow flow", which to be precise requires the flow not only to be slow but also" slowly varying" *. The Coleman and Noll (1960) work on the slow flow of fluids with fading memory leads to a set of approximate equations (ordered by some convenient measure of "speed of flow"), the first three being expressible in the form Tik 
A(1)
(8.23)
al/"\.ik'
(8.24) A(l) + a A(2) + a A(1)}A(I) + Tik  a I/"\. ik 2 /"\. ik 3 i /"\. jk
IJ
PI
A(I)iA(I)}A(I) } /"\. i /"\. ik
(8.25) where aI, PI etc. are all material constants. Equation (8.23) is the Newtonian model. Equations (8.24), called the secondorder model, have been used extensively in modem nonNewtonian fluid mechanics. The slowflow development is often referred to as the "retardedmotion expansion" and the resulting equl;!.tions as the "hierarchy equations" of Coleman and Noll. Equations (8.23)(8.25) a're important because they provide convenient equations for all simple fluids provided the flow is sufficiently slow. Another type of approximation may be obtained from the formal approach for the case when the "deformation is small". (Such a situation exists, for example, in the case of smallamplitude oscillatory shear flow.) When certain formal" smoothness" assumptions are made, the approximation leads to integral constitutive equations of the form (Coleman and Noll 1961, Pipkin 1964)
J:k = ~ooMI(S)Gik(S) ds,
(8.26) (8.27)
J:k=
~ooMI(S)Gik(S) ds+ ~oo~ooM2(SI' S2)G!(SI)Gjk (S2)
dS I dS 2
+ ~oo ~oo ~OO(MI(Sb S2' S3)G{(S2)Gj(S3)Gik (SI) +M4(SI, S2' S3)G!(SI)Gj(S2)G ik (S3)) dS I dS 2 ds3 ,
(8.28)
* This is an important observation for some flow situations. For example, on account of the noslip hypothesis, flow near a reentrant corner may be regarded as "slow" but in no sense can such a flow be regarded as "slowlyvarying", so that the Coleman and Non development for the flow of fluids with fading memory does not apply to such situations (see, for example, Crochet et al. 1984).
152
Theoretical rheology
[Chap. 8
where s = (  (' is the time lapse and, from the symmetry of the stress tensor, the kernel functions must satisfy (8.29)
Equations (8.26) are called the equations of finite linear viscoelasticity *, whilst (8.27) are called the equations of secondorder viscoelasticity and so on. The small~deformationdevelopment of Coleman and Noll has much in common with the integral expansions of Green, Rivlin and Spencer (1957, 1959, 1960). Crochet et al. (1984) advocate care in the use of the integral expansions since their range of applicability is not as wide as might be anticipated. Many of the flow problems which are tractable by analytic methods fall into the category of "nearly viscometric flows", which are flows that are close to viscometric flows such as Poiseuille or Couette flow; the "closeness" can be defined in a precise mathematical way. Pipkin and Owen (1967) have addressed the possibility of obtaining constitutive equations for this restricted class of flows. They conclude that, in an integral formulation, thirteen independent kernel functions are required. Socalled "motions with constant stretch history" have been studied by numerous theoretical rheologists, and the associated constitutive equations have been derived. The subject is covered in the books by Huilgol (1975), Lodge (1974) and Dealy (1982).
8.6 Simple constitutive equations of the Oldroyd/Maxwell type The developments discussed in ยง8.4 and ยง8.5 must be viewed as important contributions to the subject, but most of the associated equations are of limited utility in the solution of practical flow problems, either on account of their complexity or their limited range of applicability. Accordingly, numerous attempts have been made to develop relatively simple constitutive equations with predictive capability. The form of these equations may be guided by a knowledge of the fluid's microstructure (cf. ยง6.8) or by the requirement that they must be able to simulate real behaviour in simple (rheometrical) flow situations. For example, the popular Oldroyd models arose originally from a desire to generalize (for all conditions of motion and stress) relatively simple linear equations like the Jeffreys model (eqn. (3.15)) which were known to be useful approximations for very dilute suspensions and emulsions under conditions of small strain (see, for example, Frohlich and Sack 1946, Oldroyd 1953, Oldroyd 1958). It must be admitted that to model microstructure in any complete way would require prohibitive detail and some compromise is needed between capturing the * Employing an integration by parts, it is possible to show that (8.26) is equivalent to liquid A' (eqns. (8.12)).
8.6]
Equations of the Oldroyd / Maxwell type
153
known complexity of the physics and generating equations with predictive capability. A further factor of importance in the choice of constitutive model is the application in mind. For example, it is more important for the model to represent the extensionalviscosity characteristics (rather than, say, the normalstress differences) if the model is to be employed in a fibre spinning problem. In summary, simple constitutive models have to satisfy, If possible, the following: (z) they must satisfy the formulation principles discussed in Â§8.2. This is clearly
not an optional requirement. The Oldroyd approach is ideally suited for this purpose; (iz) they should reflect the physics of the microstructure;
(iii) they should be able to simulate the behaviour of the fluid in simple flows like
steady simple shear, oscillatory shear and extensional flow; (iv) they should have regard to the application in mind.
Given these constraints and the plethora of possibilities, it is not appropriate for us to favour one model at the expense of others, especially in view of the fact that history suggests that the popularity of a given model is often ephemeral. Rather, we list in tabular form many of the popular differential constitutive models which have appeared in the literature and can be viewed as having predictive capacity (see Tables 8.1 and 8.2). These can all be regarded as special cases of the general canonical forms *: T(I) ik
T ik 
+ T(2) ik ,
(8.30)
in which the terms on the right hand side are given by (1Âť) (1) Al (I)T(I) exp ( (AI  Tmm 1;k + a  1 ; j jk
111
Tik(2)


111
2 112 d ik,
'\ 0 (1) + I\I1;k 
2
111
d ik'
(8.31 )
(8.32)
where, unless otherwise stated, Al> 111' 112' (, and a are all material constants and the derivative D is given by * *
(8.33) where a is a scalar parameter. * For convenience, the models are expressed in a form appropriate to a rectangular Cartesian
**
coordinate system. We recommend Crochet et al. (1984, Chapter 2) and Giesekus (1984) for a funer discussion of the various time~derivatives of continuum mechanics.
Theoretical rheology
154
[Chap. 8
TABLE 8.1 Special cases of the general canonical form of constitutive equation (eqns. 8.308.33) Model
t
a
a
Al
Giesekus (1982) Phan路ThienTanner (1977) Phan路ThienTanner B (Phan路Thien 1984) JohnsonSegalman (1977) Whi te Metzner (1963) Oldroyd B Corotational Oldroyd (Oldroyd 1958) Upper convected Maxwell Secondorder model Leonov (1987)
0
a
0
Al
111
0
t
0
a
Al
111
0
0
0
a
Al
111 (12)
0
0
0
a
Al
111
0
0 0
0 0
0 0
Al(12) Al
111(12) 111
0 112
0
0
1
Al
111
112
0
0
0
0
1
2
0
(~O)
111 (
~
0)
Al 111 Not applicable in this form Al
112 ( ~ 0)
0 0
111
We may also use the alternative canonical form
(AI)
exp E Tmm "11
1;k
Al 0 + a1;j1jk + A1 1;k =
2"11 (
"11
d ik + A 2 d0 ik )
(8.34)
,
where we have now omitted the "12 contribution and essentially replaced it by a retardation time A2' TABLE 8.2 Special cases of the general canonical form of constitutive equation (eqn. 8.34) Model
t
a
a
Al ( ~ 0)
Giesekus (1982) PhanThienTanner (1977) PhanThienTanner B (PhanThien 1984) JohnsonSegalman (1977) WhiteMetzner (1963) Oldroyd B Corotational Oldroyd (Oldroyd 1958) Upper convected Maxwell Secondorder model Leonov (1987)
0
a
0
Al
0
111
t
0
a
Al
0
111
0
0
a
Al
A2
111(12)
0
0
a
Al
0
111
0 0
0 0
0 0
A1(12) Al
0 >0
111(12) 111
0
0
1
Al
>0
111
0 0 0
0 0
0 0 0
Al 0
0 <0 0
111 111 111
1
2
Al
111 ( > 0)
A2
8.6]
155
Equations of the Oldroyd/Maxwell type
TABLE 8.3 Rheometrical forms derived from some of the models in Tables 8.1 and 8.2 Model Oldroyd B
21'/1
o
1'/1 + 1'/2
+31'/2
2AI1'/tY 2 1 +2Ah 2 21'/ I Aly 2
Corotational Oldroyd JohnsonSegalman (1977)
1  2( 1 
+ White Metzner (1963)
a) Ali
1'/1 l+(la)Al i
21'/1(v'3 i) 12A 1(/3i)i
o
1'/1(Y)
1'/1
1  2A li + 1 + Ali
1'/1(/3 i) + ~='l+AI(v'3i)i
PhanlbienTanner B (Phanlbien 1984)
1'/1 ( y)
a
.
"2 Nl (Y)
21'/1 ( 13 i) 12(1a)A 1i 1'/1 (13 i) + 1 + (1 a) Ali
Giesekus (1982)
Consult the reference for detailed expressions
Equations (8.32), and by implication the term in A2 in (8.34), can be viewed as a "Newtonian dashpot" contribution, either introduced to reflect the solvent contribution in liquids like polymer solutions or to ensure that the shear stress in a steady simple shear flow is a monotonic increasing function, of shear rate. Some of the socalled Maxwell models (with 7'12 = 0 or A2 = 0) suffer from the problem of a stress maximum unless a = 0 or 2. For convenience, we list in Table 8.3 the main rheometrical functions derived from many of the models introduced in Tables 8.1 and 8.2. Not surprisingly, there have been similar developments involving integral equations instead of the implicit differential models discussed above. These range from the comparative simplicity of the Lodge (1956) rubberlike liquid (which is essentially equivalent to liquid B') and more or less stop at the complexity provided by the socalled KBKZ model (d. Bernstein et al. 1963), with constitutive equations which, in Cartesian coordinates, are essentially given by
(8.35)
Theoretical rheology
156
[Chap. 8
where 11 and 12 are now the two nonzero invariants of G ik . We remark that the DoiEdwards model discussed in ยง6.8.5 (with the added "independentalignment" assumption) leads to an equation of the KBKZ type (see, for example, Doi and Edwards 1986, Marrucci 1986).
8.7 Solution of flow problems
We now consider the application of the work of the previous sections to the solution of nonNewtonian flow problems. To facilitate this, it is helpful to attempt a flow classification (d. Crochet et al. 1984, Chapter 3). I. When the flow is "slow", the choice of constitutive model is selfevident (i.e. one of the hierarchy models (8.23)(8.25)) and there is no merit whatsoever in employing any of the more complicated implicit differential or integral models discussed in the previous section (d. Walters 1979). Flow problems in the case of slow flow invariably resolve themselves into perturbation analyses with "speed of flow" as the relevant perturbation parameter. II. When the flow is dominated by the shear viscosity, the generalized Newtonian model (8.20) can be employed. I I I. Many of the flow problems which have been solved successfully using
analytic techniques fall into the category of "nearly viscometric flows". Linear stability analyses, flow caused by rotating bodies and various pipe flows can be placed in the category of nearly viscometric flows. We have already indicated that the general description of such flows is of prohibitive complexity and approximate equations have been employed in existing analyses. These become perturbation problems using the basic viscometric flow as the primary flow and a convenient (geometrical, flow or continuum) parameter as the perturbation variable. IV. The advent of powerful digital computers has seen interest in nonNewtonian fluid mechanics moving towards the solution of complex flow problems for highly elastic liquids: situations which are of practical importance. Differential and integral equations at all levels of complexity are being employed in this expanding research field and it is probably true to say that, within reason, there are now few restrictions on the amount of detail that can be handled in the constitutive equation employed. The subject is covered in detail in the text by Crochet et al. (1984). The so called" high Weissenbergnumber problem" which restricted all early work in the field is discussed in that text. However, we remark with interest that the recent work of Crochet and his collaborators (cf. Marchal and Crochet 1987) has not been so hampered by the high Weissenbergnumber problem and the resulting numerical simulations are valid for conditions of practical importance where major changes in flow characteristics are observed. Any current discrepancies between theory and
8.7]
Solution offlow problems
157
experiment, and there are still some, can no longer be attributed (solely) to the high Weissenbergnumber problem. Attention must now be focussed on other problems, VIZ.:
(i) the possibility of threedimensional flow characteristics occurring in seem
ingly twodimensional flows; (ii) the possibility of "bifurcation" and lack of uniqueness in complex flows of
highly elastic liquids; (iii) the inadequacies of the constitutive equations complex materials;
In
current use for very
(iv) the incorrect numerical treatment of flow near reentrant comers and possibly
also the incorrect numerical treatment of the extra constitutive difficulties associated with longrange fluid memory. The field of the numerical simulation of nonNewtonian flow is developing rapidly and a constant update on current literature is recommended in this area.
159
GLOSSARY OF RHEOLOGICAL TERMS
This glossary is based mainly on the British Standard of the same title and numbered BS 5168:1975. It differs from the British Standard in that it is not intended to be comprehensive but limited to the terms which are most relevant to the present book. All quantitative terms have been given their SI units and symbols where this is feasible. The symbols are those used in this book and are therefore recommended; they include many which are recommended by the U.S. Society of Rheology and which were published in the Journal of Rheology (1984) 28, 181195. Antithixotropy
An increase of the apparent viscosity under constant shear stress/rate followed by a gradual recovery when the stress or shear rate is removed. The effect is timedependent (see negative thixotropy and rheopexy).
Apparent viscosity
The shear stress divided by rate of shear when this quotient is dependent on rate of shear. Also called viscosity and shear viscosity. 11 Pa.s.
Bingham model
A model with the behaviour of an elastic solid up to the yield stress; above the yield stress, the rate of shear is directly proportional to the shear stress minus the yield stress (see eqn. 2.8b).
Biorheology
The study of the rheological behaviour of biological materials.
Complex (shear) compliance
The mathematical representation of a (shear) compliance as the sum of a real and an imaginary part. The real part is sometimes called storage compliance and the imaginary part loss compliance. J* (for shear) Pa 1.
160
Glossary of rheological terms
Complex (shear) modulus
The mathematical representation of a (shear) modulus as the sum of a real and an imaginary part. The real part is sometimes called storage modulus and the imaginary part loss modulus. G* (for shear) Pa.
Complex viscosity
The mathematical representation of a viscosity as the sum of a real part and an imaginary part. The real part is usually called dynamic viscosity, the imaginary part is related to the real part of the complex shear modulus. TJ* Pa.s.
Compliance
The strain divided by the corresponding stress. J (for shear) Pa 1.
Consistency
A general term for the property of a material by which it resists permanent change of shape.
Constitutive equation
An equation relating stress, strain, time and sometimes other variables such as temperature. Also called rheological equation of state.
Continuum rheology
The rheology that treats a material as a continuum without explicit consideration of microstructure. Also called macrorheology and phenomenological rheology.
Couette flow (circular)
Simple shear flow in the annulus between two coaxial cylinders in relative rotation.
Couette flow (plane)
Simple shear flow between parallel plates motion in their own plane.
Creaming
The rising of particles of the dispersed phase to the surface of a suspension.
Creep
The slow deformation of a material; usually measured under constant stress.
Dashpot
A model for Newtonian viscous flow, typically represented by a piston moving in a cylinder of liquid.
10
relative
Glossary of rheological terms
161
Deborah number
The ratio of a characteristic (relaxation) time of a material to a characteristic time of the relevant deformation process.
Deformation
A change of shape or volume or both.
Die swell
A postextrusion swelling.
Dilatancy
(1) An increase in volume caused by deformation. (2) Shear thickening (deprecated usage).
Dynamic modulus
Synonym of complex modulus.
Dynamic viscosity
(1) In classical fluid mechanics a synonym of coefficient of viscosity used to distinguish this quantity from kinematic viscosity. 11 Pa.s. (2) In rheology, the quotient of the part of the stress in phase with the rate of strain divided by the rate of strain under sinusoidal conditions. 11' Pa.s.
Elastic(ity)
A reversible stress/strain behaviour.
Elastic energy
Synonym of strain energy.
Elastic liquid
A liquid showing elastic as well as viscous properties (see elastico路viscous, viscoelastic and memory fluid).
Elastic modulus
A stress divided by the corresponding elastic strain. Pa.
Elasticoviscous
A descriptive term for a liquid having both viscous and elastic properties.
Elongational viscosity
Synonym of extensional viscosity.
Equation of state
Synonym of constitutive equation.
162
Glossary of rheological terms
Extensional viscosity
The extensional (tensile) stress divided by the rate of extension. Also called elongational viscosity and Trouton viscosity. TIE Pa.s.
Extensional strain
Relative deformation in extension.
Extensional strain rate
The change in extensional strain per unit time. i s ] .
Extrastress tensor
The difference between the stress tensor and the isotropic pressure contribution; used for incompressible materials. ~k Pa.
Flow
A deformation, of which at least part is nonrecoverable (rheological usage).
Flow birefringence
The optical anisotropy caused by flow.
Flow curve
A curve relating stress to rate of shear (d. rheogram).
High elasticity
The ability of a material to undergo large elastic strains.
Hooke model
A model representing Hooke's law of elasticity, e.g. a spnng.
Intrinsic viscosity
The limiting value of the reduced viscosity as the concentration approaches zero. [TI].
Isotropic
Having the same property in all directions.
Kelvin model
A mechanical model consisting of a Hooke model and Newtonian fluid model in parallel. Also called Voigt model.
Kinematic viscosity
In classical fluid mechanics, the dynamic viscosity divided by the density of the material. JI m2 s 1.
Laminar flow
Flow without turbulence.
E:.
Glossary of rheological terms
163
Linear viscoelasticity
Viscoelasticity characterized by a linear relationship between stress and strain.
Loss angle
The phase difference between the stress and strain in an oscillatory deformation.
Loss compliance
The imaginary part of the complex compliance. J" (for shear) Pa 1.
Loss modulus
The imaginary part of the complex modulus. G" (for shear) Pa.
Macrorheology
Synonym of continuum rheology.
Maxwell model
A mechanical model consisting of a Hooke model and a Newtonian fluid model in series.
Melt fracture
The irregular distortion of a polymer extrudate after passing through a die.
Memory fluid
Synonym of elastic liquid.
Microrheology
The rheology in which account is taken of the ffilcrostructure of materials.
Model
An idealized relationship of rheological behaviour expressible in mathematical, mechanical or electrical terms.
Modulus
In rheology, the ratio of a component of stress to a component of strain. Pa.
N avierStokes equations
The equations govermng the motion of a Newtonian fluid.
Necking
The nonuniform local reduction of the crosssectional area of a test piece under extension.
Negative thixotropy
Synonym of antithixotropy.
164
Glossary of rheological terms
Newtonian fluid model
A model characterized by a constant value for the quotient of the shear stress divided by the rate of shear in a simple shear flow and with zero normal stress differences (see dashpot).
NonNewtonian fluid
Any fluid whose behaviour is not characterized by the N avierStokes equations.
Normal force
(1) A force acting at right angles to a specified area. N.
(2) In rheology, a force acting at right angles to an applied shear stress. N. Normal stress
The component of stress at right angles to the area considered. O'}} Pa.
Normal stress difference
The difference between normal stress components. N} Pa.
Normal stress coefficient
A normal stress difference divided by the square of the rate of shear. o/} Pa.s 2 .
Overshoot
The transient rise of a stress above the equilibrium value at the start up of simple shear flow.
Plastic(ity)
The capacity of a material to be moulded but also to retain its shape for a significant period under finite forces; showing flow above a yield stress.
Plastic viscosity
For a Bingham model, the excess of the shear stress over the yield stress divided by the rate of shear. 1J p Pa.s.
Poiseuille flow
Laminar flow in a pipe of circular cross section under a constant pressure gradient.
Powerlaw behaviour
Behaviour characterized by a linear relationship between the logarithm of the shear stress and the logarithm of the rate of shear in simple shear flow.
Pseudoplasticity
Synonym for shearthinning (usage deprecated).
Glossary of rheological terms
165
Rate of shear
(See shear rate).
Reduced viscosity
The specific viscosity per unit concentration of the solute or the dispersed phase. m3 kg 1.
Relative deformation
The measurement of deformation relative to a reference configuration of length, area or volume. Also called strain.
Relative viscosity
The ratio of the viscosity of a solution to that of the solvent or of a dispersion to that of its continuous phase (see viscosity ratio). Tl r â€˘
Relaxation time
The time taken for the shear stress of a fluid that obeys the Maxwell model to reduce to lie of its original equilibrium value on the cessation of steady shear flow.
Retardation time
The time taken for the strain in a material that obeys the Kelvin model to reduce to lie of its original equilibrium value after the removal of the stress.
Reynolds number
The product of a typical apparatus length and a typical fluid speed divided by the kinematic viscosity of the fluid. It expresses the ratio of the inertia forces to the viscous forces. R e .
Rheogoniometer
A rheometer designed for the measurement of normal as well as shear components of the stress tensor.
Rheogram
A graph of a rheological relationship.
Rheological equation of state
Synonym of constitutive equation.
Rheology
The science of the deformation and flow of matter.
Rheometer
An instrument for measuring rheological properties.
Rheopexy
Synonym of antithixotropy.
166
Glossary of rheological terms
Rigidity modulus
Synonym of shear modulus.
Secondary flow
The components of flow in a plane orthogonal to the main direction of flow.
Shear
(1) The movement of a layer of material relative to parallel adjacent layers. (2) An abbreviation of shear strain.
Shear compliance
The elastic shear strain divided by the corresponding shear stress. J Pa  1.
Shear modulus
The shear stress divided by the corresponding elastic shear strain. Also known as rigidity modulus. G Pa.
Shear rate
The change of shear strain per unit time. y s 1.
Shear strain
Relative deformation in shear; term often abbreviated to shear. y.
Shear stress
The component of stress parallel to (tangential to) the area considered. (J Pa.
Shearthickening
The increase of viscosity with increasing rate of shear in a steady shear flow.
Shearthinning
The reduction of viscosity with increasing rate of shear in a steady shear flow.
Shear viscosity
Synonym of apparent viscosity.
Simple shear
A shear caused by the parallel relative displacement of parallel planes (see viscometric flow).
Soft solid
A descriptive term for a material exhibiting plastic behaviour.
Glossary of rheological terms
167
Specific viscosity
The difference between the viscosity of a solution or dispersion and that of the solvent or continuous phase, divided by the viscosity of the solvent or continuous phase. Tl sp .
Spinnability
The capacity of a liquid to form stable extended threads.
Steady flow
A flow in which the velocity at every point does not vary with time.
Storage compliance
That part of the (shear) strain that is in phase with the (shear) stress divided by the stress under sinusoidal conditions. J' (for shear) Pa 1 .
Storage modulus
That part of the (shear) stress that is in phase with the (shear) strain divided by the strain under sinusoidal conditions. G' (for shear) Pa.
Stored energy
Synonym of strain energy.
Strain
The measurement of deformation relative to a reference configuration of length, area or volume. Also called relative deformation.
Strain energy
The energy stored in a material (per unit volume) by the elastic strain. Also called elastic energy. Jm ~ 3.
Stress
A force per unit area. Pa.
Stress relaxation
The decrease of (shear) stress on the cessation of steady (shear) flow, usually when the stress in the original steady (shear) flow has reached equilibrium.
Stress tensor
A matrix of the shear stress and normal stress components representing the state of stress at a point in a body. (Jik Pa.
168
Glossary of rheological terms
Taylor number
A dimensionless group associated with viscous instabilities in circular Couette flow, the value of which depends on the kinematic viscosity and on the radii and velocities of the cylinders.
Taylor vortices
The secondary flow consisting of ringlike cell vortices associated with an instability in circular Couette flow when the Taylor number exceeds a certain value.
Tension
A force normal to the surface on which it acts and directed outwards from the body. N.
Tensionthickening
An increase in extensional viscosity with increasing rate of strain in a steady extensional flow.
Tensionthinning
A decrease in extensional viscosity with increasing rate of strain in a steady extensional flow.
Thixotropy
A decrease of the apparent viscosity under constant shear stress or shear rate, followed by a gradual recovery when the stress or shear rate is removed. The effect is timedependent.
Timetemperature superposition
The scaling of the results of shear strain experiments carried out at different temperatures to fit onto a single curve.
Trouton ratio
The ratio of extensional to shear viscosities.
Trouton viscosity
Synonym of extensional viscosity.
Turbulence
A condition of flow in which the velocity components show random variation.
Velocity gradient
The derivative of the velocity of a fluid element with respect to a space coordinate. s 1 .
Glossary of rheological terms
169
Viscoelastic(ity)
Having both viscous and elastic properties. This term is sometimes restricted to solids.
Viscometer
An instrument for the measurement of viscosity.
Viscometric flow
A laminar flow which is equivalent to a steady simpleshear flow. Such a flow is determined by a maximum of three material functions: the viscosity function and two normal stress functions.
Viscosity
(1) Qualitatively, the property of a material to resist deformation increasingly with increasing rate of deformation. (2) Quantitatively, a measure of this property, defined as the shear stress divided by the rate of shear in steady simpleshear flow. Often used synonymously with apparent viscosity, Tl Pa.s.
Viscosity ratio
Synonym of relative viscosity.
Voigt model
Synonym of Kelvin model.
Weissenberg effect
An effect found in nonNewtonian fluids manifested, for example, in the climbing of the fluid up a rotating rod dipping into it. A normal stress effect.
Weissenberg number
The product of the relaxation time, or some other characteristic time of a material, and the rate of shear of the flow. U:.
Yield stress
The stress corresponding to the transition from elastic to plastic deformation. (Jy Pa.
Young's modulus
The extensional (tensile) stress divided by the corresponding extensional strain of an elastic material, measured in uniaxial extension. EPa.
171
REFERENCES
[1906] EINSTEIN, A.: Eine neue Bestimmung der Molekuldimension, Ann. Physik 19, 289306. [1911] EINSTEIN, A.: Berichtigung zu meiner Arbeit: Eine neue Bestimmung der Molekuldimension, Ann. Physik 34, 591592. [1945] ALFREY, T.Jr.: Methods of representing the properties of viscoelastic materials, Quart. Appl. Math. 143150. REINER, M.: A mathematical theory of dilatancy, Am. J. Math. 67, 350362.
J,
[1946] FROHLICH, H., SACK, R.: Theory of the rheological properties of dispersions, Proc. Roy. Soc. A185, 415430. GREEN, M.S., TOBOLSKY, A.V.: A new approach to the theory of relaxing polymeric media, J. Chem. Phys. 14, 8092. [1948] RIVLIN, R.S.: The hydrodynamics of nonNewtonian fluids, Part 1, Proc. Roy. Soc. A193, 260281. [1950] OLDROYD, J.G.: On the formulation of rheological equations of state, Proc. Roy. Soc. A200, 523541. ROSCOE, R.: Mechanical models for the representation of viscoelastic properties, Brit. J. Appl. Phys. !, 171173. [1953] GROSS, B.: " Mathematical Structure of the Theories of Viscoelasticity", Hermann et Cie., Paris. OLDROYD, J.G.: The elastic and viscous properties of emulsions and suspensions, Proc. Roy. Soc. A218, 122132. ROBERTS, J.E.: Pressure distribution in liquids in laminar shearing motion and comparison with predictions from various theories, in Proceedings of the 2nd. International Congress on Rheology, Ed. V.G.W. Harrison, Butterworths Sci. Pub., 9198. ROUSE, P.E.Jr.: A theory of linear viscoelastic properties of dilute solutions of coiling polymers, J. Chem. Phys. 21, 12721280. [1954] BUECHE, F.: Influence of rate of shear on the apparent viscosity of dilute polymer solutions and bulk polymers, J. Chem. Phys. 22, 15701576. KRIEGER, I.M., MARON, S.H.: Direct determination of the flow curves of nonNewtonian fluids, J. Appl. Phys. 25, 7275.
172
References
[1955] RIVLIN, R.S., ERICKSEN, J.L.: Stressdeformation relations for isotropic materials, J. Rat. Mech. Anal. ~, 323425. [1956] LODGE, A.S.: A network theory of flow birefringence and stress in concentrated polymer solutions, Trans. Faraday Soc. 52, 120130. STAVERMAN, AJ., SCHWARZL, F.R.: "Die Physik der Hochpolyrneren" Vol 4, Ed. H.A. Stuart, Springer Verlag, 215235. TORDELLA, J.P.: Fracture in the extrusion of amorphous polymers through capillaries, J. Appl. Phys. 27, 454458. ZIMM, RH.: Dynamics of polymer molecules in dilute solution: viscoelasticity, flow birefringence and dielectric loss, J. Chern. Phys. 24, 269278. [1957] BAGLEY, E.B.: End corrections in the capillary flow of polyethylene, J. Appl. Phys. 28,624627. GREEN, A.E., RIVLIN, R.S.: The mechanics of nonlinear materials with memory, Part I, Arch. Rat. Mech. Anal. !, 121. [1958] COX, W.P., MERZ, E.H.: Correlation of dynamic and steady flow viscosities, J. Polyrn. Sci. 28, 619622. OLDROYD, J.G.: NonNewtonian effects in steady motion of SOme idealized elasticoviscous liquids, Proc. Roy. Soc. A245, 278297. SISKO, A.W.: The flow of lubricating greases, Ind. Eng. Chern. 50, 17891792. TRUESDELL, c.: Geometrical interpretation for the reciprocal deformation tensors, Quart. Appl. Math. 15, 434435. [1959] GREEN, AE., RIVLIN, R.S., SPENCER, A.J.M.: The mechanics of nonlinear materials with memory, Part 2, Arch. Rat. Mech. Anal. 2, 8290. KRIEGER, I.M., DOUGHERTY, T.J.: A mechanism for nonNewtonian flow in suspensions of rigid spheres, Trans. Soc. Rheol. 2, 137152. [1960] BRAMHALL, A.D., HUTTON, J.F.: Wall effect in the flow of lubricating greases in plunger viscometers, Brit. J. Appl. Phys. 11, 363371. COLEMAN, B.D., NOLL, W.: An approximation theorem for functionals, with applications in continuum mechanics, Arch. Rat. Mech. Anal. 2, 355370. GREEN, AE., RIVLIN, R.S.: The mechanics of nonlinear materials with memory, Part 3, Arch. Rat. Mech. Anal. ~, 387404. SPAIN, B.: "Tensor Calculus", Oliver and Boyd. [1961] COLEMAN, B.D., NOLL, W.: Foundations of linear viscoelasticity, Rev. Mod. Phys. 33,239249. [1962] SEGRE, G., SILBERBERG, A.: Behaviour of macroscopic rigid spheres in Poiseuille flow. Part I, J. Fluid Mech. 14, 115135; Part 2, J. Fluid Mech. 14, 136157. 
References
173
[1963] BERNSTEIN, B., KEARSLEY, A.E., ZAPAS, L.: A study of stress relaxation with finite strain, Trans. Soc. Rheol. 1,391410. KOLSKY, H.: "Stress Waves in Solids ", Dover Publications. van WAZER, J.R., LYONS, J.W., KIM, K.Y., COLWELL, R.E.: "Viscosity and Flow Measurement: A Laboratory Handbook of Rheology", Interscience, London. WHITE, J.L., METZNER, A.B.: Development of constitutive equations for polymeric melts and solutions, J. Appl. Polym. Sci. 1, 18671889. [1964] CHACON, R.V.S., RIVLIN, R.S., Representation theorems in the mechanics of materials with memory, ZA.M.P. 15, 444447. LODGE, A.S~" Elastic Liquids ", Academic Press. OLDROYD, J.G.: Nonlinear stress, rate of strain relations at finite rates of shear in socalled "linear" elasticoviscous liquids, in "Secondorder effects in Elasticity, Plasticity and Fluid Dynamics", Ed. D. Abir, Pergamon, 520529. PIPKIN, AC.: Small finite deformation of viscoelastic solids, Rev. Mod. Phys. 36, 10341041. WHITE, J.L.: A continuum theory of nonlinear viscoelastic deformation with application to polymer processing, J. Appl. Polym. Sci. ~, 11291146. [1965] CROSS, M.M.: Rheology of nonNewtonian fluids: a new flow equation for pseudoplastic systems, J. Colloid Sci. 20,417437. HUTTON, J.F.~The fracture of liquids in shear: the effects of size and shape,' Proc. Roy. Soc. A287, 222239. MAXWELL, B., CHARTOFF, R.P.: A polymer melt in an orthogonal rheometer, Trans. Soc. Rheol. 2, 4152. OLDROYD, J.G.: Some steady flows of the general elasticoviscous liquid, Proc. Roy. Soc. A283, 115133. TRUESDELL, c., NOLL, W.: "The nonLinear Field Theories of Mechanics ", Springer Verlag. [1966] CAMERON, A.: "Principles of Lubrication", Longman. COLEMAN, B.D., MARKOVITZ, H., NOLL, W.: "Viscometric Flows of nonNewtonian Fluids", Springer Verlag. KAYE, A: An equation of state for nonNewtonian fluids, Brit. J. Appl. Phys. 17, 803806. LESLIE, F.M.: Some constitutive equations for anisotropic fluids, Quart. J. Mech. Appl. Math. 19, 357370. PIPKIN, A.C.: Approximate constitutive equations, in "Modern Developments in the Mechanics of Continua", Ed. S. Eskinazi, Academic Press, 89108. [1967] BARLOW, A.J., ERGINSAV, A, LAMB, J.: Viscoelastic relaxation of supercooled liquids, II, Proc. Roy. Soc. A298, 481494. CLARKE, B.: Rheology of coarse settling suspensions, Trans. Inst. Chem. Eng. 45,251256. EDWARDS, S.F.: The statistical mechanics of polymerized material, Proc. Phys:Soc. 92, 916. PIPKIN, A.c., OWEN, D.R.: Nearly viscometric flows, Phys. FlUids 10, 836843. SCHWARZL, F.R., STRUIK, L.C.E.: Analysis of relaxation measurements, Adv. Mol. Relaxation Proc. 1,201255. [1968] BERRY, G.c., FOX, T.G.: The viscosity of polymers and their concentrated solutions, Adv. Polym. Sci. ~, 261357.
174
References
BROADBENT, J.M., KAYE, A., LODGE, A.S., VALE, D.G.: Possible systematic error in the measurement of normal stress differences in polymer solutions in steady shear flow, Nature 271, 35. CHENG, D.CH.: The effect of secondary flow On the viscosity measurement using the cone~andplate viscometer, Chem. Eng. Sci. 23, 895899. COGSWELL, F.N.: Rheology ofpolymer melts under tension, Plastics & Polym. 36, 109111. DAVIS, S.S., DEER, J.J., WARBURTON, B.: A concentric cylinder air turbine viscometer, J. Sci. Instrum. (Ser. 2) 1. 933936. FARRIS, R.J.: Prediction of the viscosity of multimodal suspensions from unimodal viscosity data, Trans. Soc. Rheol. 12, 281301. MARKOVITZ, H.: The emergence of rheology, Physics Today 21, 2330. PLAZEK, D.J.: Magnetic bearing torsional creep apparatus, J. Polym. Sci. A2 ~, 621638. [1969] GLICKSMAN, M. "Gum Technology in the Food Industry", Academic Press. TANNER, R.I.: Network rupture and the flow of concentrated polymer solutions, AIChE J. 15, 177183. TANNER, R.I., PIPKIN, A.c.: Intrinsic errors in pressurehole measurements, Trans. Soc. Rhea!., 13, 471484. [1970] ASTARITA, G., NICODEMO, L.: Extensional flow behaviour of polymer solutions, Chem. Eng. J. 1, 5765. BATCHELOR, G.K.: The stress system in a suspension of forcefree particles, J. Fluid Mech. 41, 545570. DYSON, A.: Frictional traction and lubricant rheology in elastohydrodynamic lubrication, Phil. Trans. Roy. Soc. A266, 133. METZNER, A.P., METZNER, A.B.: Stress levels in rapid extensional flows of polymeric fluids, Rheol. Acta 2, 174181. SHERMAN, P.: "Industrial Rheology", Academic Press. TANNER, R.I.: Some methods of estimating the normal stress functions in viscometric flows, Trans. Soc. Rheol. 14, 483507. [1971] BATCHELOR, G.K.: The stress generated in a nondilute suspension of elongated particles in pure straining motion, J. Fluid Mech. 46, 813829. de GENNES, P.G.: Reptation of a polymer chain in the presence of fixed obstacles, J. Chem. Phys. 55, 572579. GRISKEY, R.G., GREEN, R.G.: Flow of dilatant (shearthickening) fluids, AIChE J. 17, 725731. [1972] BROADBENT, J.M., LODGE, A.S.: Determination of normalstress differences in steady shear flow, Part 3, Rheol. Acta 10,557573. CARREAU, P.J.: Rheological equations from molecular network theories, Trans. Soc. Rheol. 16,99127. COGSWELL, F.N.: Converging flow of polymer melts in extrusion dies, Polym. Eng. Sci. 12,6473. COGSWELL, F.N.: Measuring the extensional rheology of polymer melts, Trans. Soc. Rheol. 16, 383403. HOFFMAN, R.L.: Discontinuous behaviour in concentrated suspensions, Trans. Soc. Rheol. 16, 155173. HUTTON, J.F.: Effect of changes of surface tension and contact angle on normal force measurement with the Weissenberg rheogoniometer, Rheol. Acta !.!., 70 72. KRIEGER, I.M.: Rheology of monodisperse latices, Adv. Colloid Interface Sci.], 111136. LODGE, A.S., STARK, J.H.: On the description of rheological properties of viscoelastic continua, Part 2. Proof that Oldroyd's 1950 formalism includes all simple fluids, Rhea!. Acta !.!.' 119126.
References
175
MEISSNER, J.: Development of a universal extensional rheometer for the uniaxial extension of polymer melts, Trans. Soc. Rheol. 16, 405420. [1973] CHENG, D.CH.: Some measurements on a negative thixotropic fluid, Nature 245, 9395. KESTIN, J. SOKOLOV, M., WAKEHAM, W.: Theory of capillary viscometers, Appl. Sci. Res. 27, 241264. [1974] ASTARITA, G., MARRUCCI, G.: "Principles of nonNewtonian Fluid Mechanics", McGrawHill. LODGE, A.S.: "BodyTensor Fields in Continuum Mechanics", Academic Press. OLIVER, D.R., BRAGG, R.: The triple jet: A new method for measurement of extensional viscosity, Rheol. Acta 13, 830835. TADMOR, Z., BIRD, R.B.: Rheological analysis of stabilizing forces in wirecoating dies, Polym. Eng. Sci. 14, 124136. [1975] DAVIES, J.M., HUTTON, J.F., WALTERS, K.: Measurement of the elastic properties of polymercontaining oils by the jetthrust technique, in Polymeres et Lubrification, Colloques Int. du C.N.R.S., 6167. HUILGOL, R.R.: "Continuum Mechanics of Viscoelastic Liquids ", John Wiley & Sons. MUNSTEDT, H.: Viscoelasticity of polystyrene melts in tensile creep experiments, Rheo/. Acta 14, 10771088. NOLTINGK, RE.: (Ed) "The Instrument Manual", 5th edition, United Trade Press. TRELOAR, L.R.G.: "The Physics of Rubber Elasticity", 3rd edition, Clarendon Press, Oxford. WAKEMAN, R.: Packing densities of particles with lognormal size distribution, Powder Tech. 11, 297299. WALTERS, K.: "Rheometry", Chapman and Hall. [1976] ACIERNO, D., LA MANTIA, F.P., MARRUCCI, G., TITOMANLIO, G.: A nonlinear viscoelastic model with structuredependent relaxation times, J. nonNewtonian Fluid Mech., !, 125146. BINDING, D.M., WALTERS, K.: Elasticoviscous squeeze films, Part 3. The torsionalbalance rheome~ ter, J. nonNewtonian Fluid Mech. L 277286. HAN, C.D.: "Rheology in Polymer Processing", Academic Press. HARRISON, G.: "The Dynamic Properties of Supercooled Liquids ", Academic Press. HUDSON, N.E., FERGUSON, J.: Correlation and molecular interpretation of data obtained m elongational flow, Trans. Soc. Rheo/. 20, 265286. PETRIE, c.J.S., DENN, M.M.: Instabilities in polymer processing, AIChE J. 22, 209236. TOWNSEND, P., WALTERS, K., WATERHOUSE, W.M.: Secondary flows in pipes of square cross section and the measurement of the secondnormal stress difference, J. nonNewtonian Fluid Mech. !. 107123. [1977] BATCHELOR, G.K.: The effect of Brownian motion on the bulk stress in a suspension of spherical particles, J. Fluid Mech. 83, 97117. BOGER, D.V.: A highly elastic constantvisc0sity fluid, J. nonNewtonian Fluid Mech. 1, 8791. BOGER, D.V.: Demonstration of upper and lower Newtonian fluid behaviour in a pseudoplastic fluid, Nature 265, 126128. DAVIES, J.M., HUTTON, J.F., WALTERS, K.: A critical reappraisal of the jetthrust technique for normal stresses, with particular reference to axialvelocity and stress rearrangement at the exit plane, J. nonNewtonian Fluid Mech. 1, 141160.
176
References
GRAY, R.W., HARRISON, G., LAMB, J.: Dynamic viscoelastic behaviour of lowmolecularmass polystyrene melts, Proc. Roy. Soc. A356, 77102. JOHNSON, M.W.Jr., SEGALMAN, D.: A model for viscoelastic fluid behaviour which allows nonaffine deformation, J. nonNewtonian Fluid Mech. ~, 255270. MIDDLEMAN, S.: "Fundamentals of Polymer Processing", McGrawHill. NIELSEN, L.E.: "Polymer Rheology", Marcel Dekker. PHANTHIEN, N., TANNER, R.I.: A new constitutive equation derived from network theory, J. nonNewtonian Fluid Mech. ~, 353365. TURIAN, R., YUAN, TF.: Flow of slurries in pipelines, A IChE J. 23,232243. WALTERS, K., WATERHOUSE, W.M.: A note on kinematical tensors, J. nonNewtonian Fluid Mech. l,293296. [1978] JENKINS, J.T.: Poiseuille and Couette flows of nematic liquid crystals, Ann. Rev. Fluid Mech. 10, 197219. LAUN, H.M., MUNSTEDT, H.: Elongational behaviour of a low density polyethylene melt, Part 1, Rheol. Acta 17, 415425. QUEMADA, D.: Rheology of concentrated disperse systems, Rheol. Acta 17, 643653. SCHOWALTER, W.R.: "Mechanics of nonNewtonian Fluids ", Pergamon Press. WHITCOMB, P.J., MACOSKO, C.W.: Rheology of Xanthan gum, J. Rheol. 22,493505. WILLEY, S.J., MACOSKO, C.W.: Steady shear rheological behaviour of PVC plastisols, J. Rheol. 2, 525545. [1979] de GENNES, P.G.: "Scaling Concepts in Polymer Physics ", Cornell University Press. FOSTER, J., NIGHTINGALE, J.D.: "A Short Course on General Relativity", Longman. PETRIE, c.J.S.: "Elongational Flows", Pitman. GRAVSHOLT, S.: Physicochemical properties of viscoelastic detergent solutions, in "Polymer Col/oids II", ed. R. Fitch, Plenum Press, 405417. LESLIE, F.M.: Theory of flow phenomena in liquid crystals, Adv. Liq. Cryst. ~, 181. MEWIS, J.: ThixtropyA general review, J. nonNewtonian Fluid Mech. 2, 120. MUNSTEDT, H.: New universal extensional rheometer for polymer melts. Measurement on a PS sample, J. Rheol. 23,421436. WALTERS, K.: Developments in nonNewtonian fluid mechanicsA personal view, J. nonNewtonian Fluid Mech. 2, 113124. WILLIAMS, R.W.: Determination of viscometric data from the Brookfield RVT viscometer, Rheol. Acta 18, 345359. WILLIAMS, G.E., BERGEN, J.T., POEHLEIN, G.W.: Rheological behaviour of high resin level plastisols, J. Rheol. 23, 591616. WINTER, RH., MACOSKO, C.W., BENNETI', K.E.: Orthogonal stagnation flow, a framework for steady extensional flow experiments, Rheol. Acta 18, 323334. [1980] BALL, R., RICHMOND, P.: Dynamics of colloidal dispersions, J. Phys. Chern. Liquids 2, 99116. BEAZLEY, K.M.: Industrial aqueous suspensions, in "Rheometry: Industrial Applications" ed. K. Walters, John Wiley & Sons, 339413. BOGER, D.V., DENN, M.M.: Capillary and slit methods of normal stress measurements, J. nonNewtonian Fluid Mech. ~, 163185. de KEE, D., TURCOTTE, G., CODE, R.K.: Rheology characterisation of timedependent foodstuffs, in "Rheology Vol.3: Applications", Eds. G. Astarita, et aI., Plenum Press, 609614. FERGUSON, J., ELTAWASHI, M.K.R: The measurement of the elongational viscosity of polymer solutions, in "Rheology Vol.2: Fluids ", Eds. G. Astarita, et aI., Plenum Press, 257262.
References
177
FERRY, J.D.: "Viscoelastic Properties of Polymers", 3rd edition, John Wiley & Sons. HUTTON, J.F.: Lubricants, in "Rheometry: Industrial Applications", ed. K. Walters, John Wiley & Sons, 119177. IPPOLITO, M.: Rheology of disperse systemsinfluence of NaCl on the viscous properties of aqueous bentonite suspensions, in "Rheology Vol.2: Fluids", Eds. G. Astarita et aI., Plenum Press, 651658. KEENTOK, M., GEORGESCU, A.G., SHERWOOD, AA., TANNER, R.L: The measurement of the second normal stress difference for some polymer solutions, J. nonNewtonian Fluid Mech. ~, 303324. MILLS, P., RUBI, J.M., QUEMADA, D.: Suspension flow, in "Rheology Vol. 2: Fluids", Eds. G. Astarita et aI., Plenum Press, 639643. ONOGI, S., ASADA, T.: Rheology and rheooptics of polymer liquid crystals, in "Rheology Vol. I. Principles ", Eds. G. Astarita et aI., Plenum Press, 127147. VINOGRADOV, G.V., MALKIN, AYa.: "Rheology of Polymers, Mir, Moscow; English translation, Springer Verlag. WALTERS, K.: (ed) "Rheometry: Industrial Applications", John Wiley & Sons. WALTERS, K., BARNES, H.A: Anomalous extensionalflow effects in the use of commercial viscometers, in "Rheology Vol. I: Principles", Eds. G. Astarita et aI., Plenum Press, 4562. WALTERS, K., BROADBENT, J.M.: "NonNewtonian Fluids", Film/Video (U.C.W., Aberystwyth). WHITE, J.L.: Molten polymers, in "Rheometry: Industrial Applications", Ed. K. Walters, John Wiley & Sons, 209280. WHORLOW, R.W.: "Rheological Techniques", John Wiley & Sons. [1981] BARNES, H.A: "Dispersion rheology: 1980", Royal Soc. of Chern., Industrial Division, London. BRYDSON, J.A.: "Flow Properties of Polymer Melts", 2nd edition, George Godwin, London. COGSWELL, F.N.: "Polymer Melt Rheology", George Godwin, London. GALVIN, G.D., HUTTON, J.F., JONES, B.: Development of a highpressure, highshear~rate capillary viscometer, J. nonNewtonian Fluid Mech. ~, 1128. MEISSNER, J., RAIBLE, T., STEPHENSON, S.E.: Rotary clamp in uniaxial and biaxial extensional rheometry of polymer melts, J. Rheol. 25, 128. MUNSTEDT, H., LAUN, H.M.: Elongational properties (and the recoverable strain in the steady state of elongation) and molecular structure of polyethylene melts, Rheol. Acta 20, 21122. [1982] BIRD, R.B.: Polymer kinetic theories and elongational flows, Chem. Eng. Commun. 16, 175187. GIESEKUS, H.: A simple constitutive equation for polymer fluids based on the concept of deformationdependent tensorial mobility, J. nonNewtonian Fluid Mech. 11,69109. DEALY, J.M.: "Rheometers for Molten Plastics", Van Nostrand Rheinhold. JONES, W.M., REES, 1.1.: The stringiness of dilute polymer solutions, J. nonNewtonian Fluid Mech. 11, 257268. [1983] ALINCE, B., LEPOUTRE, P.: Flow behaviour of pigment blends, TAPPI J. 66, 5760. GIESEKUS, H.: Disperse systems: dependence of rheological properties on the type of flow with implications for food rheology, in "Physical Properties of Foods", Ed. R. Jowitt et aI., Applied Science Publishers, Chap. 13. JANESCHITZKRIEGL, H.: "Polymer Melt Rheology and Flow Birefringence", Springer Verlag. MEISSNER, J.: Polymer melt rheologya challenge for the polymer scientist and engineer, IUPAC Macro8] Bucharest, Romania, Plenary and invited lectures, Part 2, IUPAC Macromolecular Division, 203226. PRILUTSKI, G., GUPTA, R.K., SRIDHAR, T., RYAN, M.E.: Model viscoelastic liquids, J. nonNewtonian Fluid Mech. 12, 233241.
178
References
SAUT, J.e., JOSEPH, D.D.: Fading memory, Arch. Rat. Mech. Anal. 81, 5395. SCHOMMER, P., TEBEL, K.H.: A new elongational rheometer for polymer solutions, J. nonNewtonian Fluid Mech., 12, 331347. WALTERS, K.:The second normal stress difference project, !UPAC MacroB3 Bucharest, Romania, Plenary and invited lectures, Part 2, IUPAC Macromolecular Division, 227237. [1984] CROCHET, M.J., DAVIES, A.R., WALTERS, K.: "Numerical Simulation of nonNewtonian Flow", Elsevier. GIESEKUS, H.: On configuration dependent generalized Oldroyd derivatives, J. nonNewtonian Fluid Mech. 14,4765. GUPTA, R.K., SRIDHAR, T.: A novel elongational viscometer, in "Advances in Rheology, Vol. 4.Applications" Eds. B. Mena et aI., Univ. Nacional Autonom. de Mexico, 7176. JACKSON, K.P., WALTERS, K., WILLIAMS, R.W.: A rheometrical study of Boger fluids, J. nonNewtonian Fluid Mech. 14, 173188. OLDROYD, J.G.: An approach to nonNewtonian fluid mechanics, J. nonNewtonian Fluid Mech. 14, 946. PHANTHIEN, N.: Squeezing a viscoelastic liquid from a wedge: an exact solution, J. nonNewtonian Fluid Mech. 16, 329345. [1985] ALVAREZ, G.A., LODGE, A.S., CANTOW, H.H.: Measurement of the first and second normal stress differences: correlation of four experiments on a polyisobutylene/dekalin solution Dl, Rheol. Acta 24, 368376. BARNES, HA., WALTERS, K.: The yield stress myth? Rheol. Acta 24,323326. BIRD, R.B.: From molecular models to constitutive equations, in "Viscoelasticity and Rheology ", Eds. A.S. Lodge, M. Renardy, J.A. Nohel, Academic Press, 105123. CHAPOY, L.L.: (Ed.) "Recent Advances in Liquid Crystalline Polymers", Elsevier Appl. Sci. de KRUIF, e.G., van IEVSEL, E.M.F., VRIJ, A., RUSSEL, W.B.: Hard sphere colloidal dispersions: Viscosity as a function of shear rate and volume fraction, J. Chem. Phys. 83, 471725. GIESEKUS, H.: A comparison of molecular and networkconstitutive theories for polymer fluids, in "Viscoelasticity and Rheology" Eds. A.S. Lodge, M. Renardy, JA. Nohel, Academic Press, 157180. KELLER, A., ODELL, J.A.: The extensibility of macromolecules in solution; a new focus for macromolecular science, Colloid Polym. Sci. 263, 181201. MEISSNER, J.: Experimental aspects in polymer melt elongational rheometry, Chem. Eng. Commun. 33, 159180. ODELL, J.A., KELLER, A., MILES, M.J.: Assessment of molecular correctedness in semidilute polymer solutions by elongational flow, Polymer 26, 12191226. PEARSON, J.R.A.: "Mechanics of Polymer Processing", 2nd edition, Elsevier, Barking. SOSKEY, P.R., WINTER, H.H.: Equiaxial extension of two polYJ;ller melts: polystyrene and low density polyethylene, J. Rheol. 29,493517. TANNER, R.L: "Engineering Rheology", Clarendon Press, Oxford. WALTERS, K.: Overview of macroscopic viscoelastic fl0W, in "Viscoelasticity and Rheology", eds. A.S. Lodge, M. Renardy, J.A. Nohel, Academic Press, 47..:]79. WILLIAMS, P.R., WILLIAMS, R.W.: On the planar extensional viscosity of mobile liquids, J. nonNewtonian Fluid Mech. 19,5380. WOODCOCK, L.V.: Molecular dynamics and relaxation phenomena in glasses, Proceedings of a Workshop on Glass Forming Liquids, Ed. Z.LP. Bielefeld, Springer Lecture Series in Physics, Vol. 277, 113124. [1986] DOl, M., EDWARDS, S.F.: "The Theory of Polymer Dynamics", Clarendon Press, Oxford. HEYES, D.M.: NonNewtonian behaviour of simple liquids, J. nonNewtonian Fluid Mech. 21, 137155.
References
179
JONES, W.M., WILLIAMS, P.R., VIRDI, T.S.: The elongation of radial filaments of a Boger fluid on a rotating drum, J. nonNewtonian Fluid Mech. 21, 5164. LAUN, H.M.: Prediction of elastic strains of polymer melts in shear and elongation, J. Rheol. 30, 459501. MARRUCCI, G.: The DoiEdwards model without independent alignment, J. nonNewtonian Fluid Mech. 21, 329336. MARRUCCI, G., GRIZZUTI, N.: The DoiEdwards model in slow flows. Predictions on the Weissenberg effect, J. nonNewtonian Fluid Mech. 21, 319328. PAL, R., BHATTACHARYA, S.N., RHODES, E.: Flow behaviour of oilinwater emulsions, Can. J. Chern. Eng. 64, 310. RAMAMURTHY, A.V.: Wall slip in viscous fluids and the influence of materials of construction, J. Rheol. 30, 337357. [1987] BARNES, H.A, EDWARDS, M.F., WOODCOCK, L.V.: Applications of computer simulations to dense suspension rheology, Chern. Eng. Sci. 42, 591608. BINDING, D.M., WALTERS, K, DHEUR, 1., CROCHET, M.J.: Interfacial effects in the flow of viscous and elasticoviscous liquids, Phil. Trans. Roy. Soc. A323, 449469. BIRD, R.B., ARMSTRONG, R.C, HASSAGER, 0.: "Dynamics of Polymeric liqUids", Vol. J, Fluid Mechanics, 2nd edition, John Wiley & Sons. BIRD, R.B., CURTISS, CF., ARMSTRONG, R.C, HASSAGER, 0.: "Dynamics of Polymeric Liquids", Vol. 2, Kinetic Theory, 2nd edition, John Wiley & Sons. BOGER, D.V.: Viscoelastic flows through contractions, Ann. Rev. Fluid Mech. 19, 157182. FULLER, G.G., CATHEY, CA, HUBBARD, B., ZEBROWSKI, B.E.: Extensional viscosity measurements for lowviscosity fluids, J. Rheol. 31, 235249. GOODWIN, J.: The rheology of colloidal dispersions, in "Solid/Liquid Dispersions" Ed. Th. Tadros, Academic Press, Chap. 10. HUNTER, R.J.: "Foundations of Colloid Science", Vol. 1, Oxford University Press, Oxford. JONES, D.M., WALTERS, K, WILLIAMS, P.R.: On the extensional viscosity of mobile polymer solutions, Rheol. Acta 26, 2030. LEONOV, AI.: On a class of constitutive equations for viscoelastic liquids, J. nonNewtonian Fluid Mech. 25, 159. LODGE, AS., ALHADITHI, T.R.S., WALTERS, K: Measurement of the first normalstress difference at high shear rates for a polyisobutylene/decalin solution "D2", Rheol. Acta 26, 516521. MARCHAL, J.M., CROCHET, M.J.: A new mixed finite element for calculating viscoelastic flow, J. nonNewtonian Fluid Mech. 26, 77114. MATHYS, E.F., SABERSKY,R.H.: Rheology, friction and heat transfer study of a discontinuously shearthickening antimisting polymer solution, J. nonNewtonian Fluid Mech. 25, 177196. [1988] ALHADITHI, T.S.R., WALTERS, K, BARNES, RA: The relationship between the linear (oscillatory) and steady shear properties of a series of polymeric systems, in Proceedings of the JOth International Congress on Rheology Vol. J" Ed. P.RT. Uhlherr, Australian Society of Rheology, 137139. BINDING, D.M.: An approximate analysis for contraction and converging flows, J. nonNewtonian Fluid Mech. 27, 173189. DEALY, J.M., GIACOMIN, A.J.: Slidingplate and slidingcylinder rheometers, in "Rheological Measurement", Eds. AA Collyer, D.W. Clegg, Elsevier. LODGE, AS.: Normal stress differences from holepressure measurements, in "Rheological Measurement", Eds. AA Collyer, D.W. Clegg, Elsevier. MARRUCCI, G.: Paper presented at Int. Congress on Extensional Flow, Chamonix, France, Jan. 1988. MOAN, M., MAGUEUR, A: Transient extensional viscosity of dilute flexible polymer solutions, J. nonNewtonian Fluid Mech. 30, 343354.
180
References
WALTERS, K.: Editorial; Int. Congress on Extensional Flow, Chamonix, France, Jan. 1988, J. nonNewtonian Fluid Mech. 30, 9798. WALTERS, K., JONES, D.M.:Extension.dominated flows of polymer solutions with applications to EaR, in Proceedings of the 10th International Congress on Rheology, Vol. 1, Ed. P.RT. Uhlherr, Australian Society of Rheology, 103109. [1989] BARNES, H.A.: Review of shearthickening of suspensions, J. Rheol. 33, 329366. LAUN, RM., SCHUCH, R: Transient elongational viscosities and drawability of polymer melts, J. Rheol. 33, 119175.
181
AUTHOR INDEX (Numbers in italics refer to entries in the Reference section i.e. pp 171  180 )
Acierno, D. 108, 175 AlHadithi, T.R.S. 58, 73, 111, Alfrey, T. 1m. 44, 171 Alinee, B. 131, 177 Alvarez, G.A. 59, 60, 178 Annstrong, RC. 9, 37, 65, 76, 89, 97, 106, 107, 141, 179 Asada, T. 22, 177 Astarita, G. 88, 141, 143, 145,
179
77, 82, 142, 143, 174, 175
Bagley, E.B. 87, 172 Ball, R. 121, 176 Barlow, A.1. 54, 173 Barnes, H.A. 17, 21, 22, 26, 73, Ill, 115, 120, 123, 129, 137, 138, 177, 178, 179, 180 Batchelor, G.K. 82, 120, 174, 175 Beazley, K.M. 23, 176 Bermett, K.E. 86, 176 Bergen, I.T. 131, 176 Bernstein, B. 155, 173 Berry, G.C. 103, 173 Bhattacharya, S.N. 135, 179 Binding, D.M. 70, 88, 100, 175, 179 Bird, RB. 9, 37, 64, 65, 76, 77, 81, 82, 83, 89, 97, 106, 107, 109, 141, 142, 143, 175, 177, 178, 179 Boger, D.V. 10, 19, 59, 70, 100, 175, 176, 179 Bragg, R. 89, 175 Bramhall, A.D. 128, 172 Broadbent, I.M. 68, 70. 95, 174, 177 Brydson, I.A. 104, 177 Bueche, F. 107, 171 Cameron, A. 14, 173
Cantow, H.H. 59, 60, 178 Carreau, p.r. 18, 174 Cathey, C.A. 89, 179 Chacon, R.V.S. 150, 173 Chapoy, L.L. 105, 178 Chartoff, R.P. 54, 173 Cheng, D.CH. 31, 119. 174, 175 Clarke, B. 124, 125, 173 Code, R.K. 22, 176 Cogswell, F.N. 75, 84, 88, 104, 111, 174 177 Coleman, B.D. 151, 172, 173 Colwell, RE. 26, 173 Cox, W.P. 72, 98, 172 Crochet, M.I. 10, 100. 141, 142, 147, 151. 152, 153, 156, 178, 179 Cross, M.M. 18, 173 Curtiss, F.C. 97, 106, 107, 141, 179 Davies, A.R 10, 141, 142, 147, 151, 152, 153, 156, 178 Davies, I.M. 63, 70, 175 Davis, S.S. 18, 174 De Germes, P.G. 108, 174, 176 De Kee, D. 22, 176 De Kruif, C.G. 125, 126, 178 Dealy, I.M. 8, 9, 65, 75, 152, 177, 179 Deer, 1.1. 18, 174 Derm, M.M. 70. 113, 175, 176 Dheur, I. 100, 179 Doi, M. 9, 106, 108, 109, 141, 156, 178 Dougherty, T.I. 121, 172 Dyson, A. 38, 174 Edwards, M.P. 137, 138, 179 Edwards, S.P. 9, 106, 108, 109, 141, 156, 173, 178
182
Einstein, A. 119, 171 ElTawashi, M.K.H. 86, 176 Erginsav, A. 54, 173 Ericksen, J.L. 148, 150, 172
Jones, D.M. 114, Jones, W.M. Joseph, D.O.
Farris, RJ. 123, 174 Ferguson, J. 85, 86, 91, 175, 176 Ferry, J.D. 38, 53, 101, 103, 109, 177 Foster, J. 143, 176 Fox, T.G. 103, 173 Frohlich, H. 42, 152, 171 Fuller, G.G. 89, 179
Kaye, A. 68, 108, 173, 174 Kearsley, A.E. 155, 173 Keentok, M. 59, 100, 177 Keller, A. 89, 178 Kestin, J. 33, 175 Kim, K. Y. 26, 173 Kolsky, H. 53, 173 Krieger, LM. 28, 121, 126, 171, 172, 174
Galvin, G.D. 33, 177 Georgescu, A.G. 59, 100, 177 Giacomin, A.J. 65, 179 Giesekus, H. 107, 108, 124, 125, 153, 155, 177, 178 Glicksman, M. 105, 114, 174 Goodwin, J. 131, 134, 179 Gravsholt, S. 23, 176 Gray, R.W. 103, 176 Green, A.E. 150, 152, 172 Green, M.S. 108, 171 Green, R.G. 129, 174 Griskey, R.G. 129, 174 Grizzuti, N. 109, 179 Gross, B. 38, 50, 171 Gupta, R.K. 86, 100, 177, 178 Han, C.D. 111, 175 Harrison, G. 53, 103, 175, 176 Hassager, O. 9, 37, 65, 76, 77, 82, 89, 97, 106, 107, 109, 141, 142, 143, 179 Heyes, D.M. 138, 178 Hoffmarm, R.L. 128, 129, 174 Hubbard, B. 89, 179 Hudson, N.E. 85, 91, 175 Huilgol, R.R. 152, 175 Hunter, R.J. 116, 179 Hutton, J.F. 15, 33, 63, 68, 70, 113, 128, 172, 173, 174, 175, 177 Ippolito, M. 133, 177 Jackson, K.P. 99, 178 JaneschitzKriegl, H. 9, 177 Jenkins, J.T. 142, 176 Johnson, M.W. Jnt. 108, 154, 155, 176 Jones, B. 33, 177
85, 86, 91, 94, 96, 95, 179, 180 89, 177, 179 150, 178
La Mantia, F.P. 108, 175 Lamb, J. 54, 103, 173, 176 Laun, H.M. 75, 76, 83, 84, 86, 90, 91, 104, 111, 176, 177, 179, 180 Leonov, A.I. 108, 154, 155, 179 Lepoutre, P. 131, 177 Leslie, F.M. 142, 173, 176 Lodge, A.S. 9, 55, 58, 59, 60, 65, 68, 70, 108, 141, 142, 152, 155, 172, 173, 174, 175, 178, 179 Lyons, J.W. 26, 173
Macosko, C.W. 19, 86, 134, 176 Magueur, A. 88, 179 Malkin, A.Ya. 104, 105, 111, 177 Marchal, J.M. 156, 179 Markovitz, H. 3, 173, 174 Maron, S.H. 28, 171 Marrucci, G. 100, 108, 109, 141, 143, 145, 156, 175, 179 Mathys, E.F. 23, 179 Maxwell, B. 54, 173 Meissner, J. 75, 82, 83, 84, 89, 90, 175, 177, 178 Men, RH. 72, 98, 172 Metmer, A.B. 79, 148, 154, 155, 173, 174 Metzner, A.P. 79, 174 Mewis, J. 24, 142, 176 Middleman, S. 111, 176 Miles, M.J. 89, 178 Mills, P. 19, 177 Moan, M. 88, 179 Munstedt, H. 75, 83, 84, 175, 176, 177 Nicodemo, L. 88, 174 Nielsen, L.E. 104, 176 Nightingale, J.D. 143, 176
183
Noll, W. 141, 142, 143, 149, 150, 151, 172, 173 Noltingk, RE. 35, 175 Odell, JA. 89, 178 Oldroyd, J.G. 38, 42, 136, 143, 145, 146, 147, 150, 152, 154, 171, 172, 173, 178 Oliver, D.R. 89, 175 Onogi, S. 22, 177 Owen, D.R. 152, 173 Pal, R. 135, 179 Pearson, J.R.A. Ill, 112, 178 Petrie, CJ.S. 75, 77, 78, 113, 175, 176 PhanThien, N. 81, 108, 154, 155, 176, 178 Pipkin, A.C. 150, 151, 152, 173, 174 Plazek., D.J. 52, 174 Poehlein, G.W. 131, 176 Prilutski, G. 100, 177 Quemada, D. 19, 176, 177 Raible, T. 82, 177 Ramamurthy, A.V. 113, 179 Rees, I.J. 89, 177 Reiner, M. 149, 171 Rhodes, E. 136, 179 Richmond, P. 121, 176 Rivlin, R.S. 148, 149, 150, 152, 171, 172, 173 Roberts, J.E. 59, 171 Roscoe, R. 43, 171 Rouse, P.E. Jm. 107, 171 Rubi, J.M. 19, 177 Russel, W.B. 125, 126, 178 Ryan, M.E. 100, 177 Sabersky, R.H. 23, 179 Sack, R. 42, 152, 171 Saut, J.C. 150, 178 Schowalter, W.R. 9, 141, 142, 176 Schuch, H. 76, 83, 84. 86, 90. 91, 104. 180 Schummer, P. 89. 178 Schwanl, P.R. 38, 50, 172, 173 Segahnan, D. 108, 154. 155, 176 Segre, G. 128, 172 Shennan, P. 18, 174 Sherwood. A.A. 59, 100, 177 Silberberg, A. 128, 172
Sisko, A.W. 19, 172 Sokolov, M. 33, 175 Soskey, P.R. 76. 86, 178 Spain, R 143, 172 Spencer, A.J.M. 150, 152, 172 Sridhar, T. 86, 100, 177, 178 Stark, J.H. 142, 174 Stavennan, AJ. 38, 172 Stephenson, S.E. 82, 177 Stroik, L.C.E. 50, 173 Tadmor, Z. 64, 175 Tanner, R.L 9, 59, 70. 77, 79, 81, 100, 101, 106, 108, 109, 112, 141, 154, 155, 174, 176, 177, 178 Tebel, K.H. 89, 178 Titomanlio, G. 108, 175 Tobolsky. A.V. 108, 171 Tordella, J.P. 68, 172 Townsend., P. 64, 175 Treloar, L.R.G. 106, 175 Truesdell, C. 141, 142, 143, 146, 149, 150, 172, 173 Turcotte, G. 22, 176 Turian. R. 125, 176 Vale. D.G. 68, 174 Van Ievsel, E.M.F. 125, 126, 178 Van Wazer, J.R. 26, 173 Vinogradov, G.V. 104, 105, 111, 177 Virdi, T.S. 89, 179 Vrij, A. 125, 126, 178 Wakeham, W. 33, 175 Wakeman, R. 121, 175 Walters, K. 9, 10, 17, 21, 26, 31, 32, 34, 37, 51, 53, 54, 58, 59, 63, 64, 65, 66, 67, 70, 73, 77, 80, 83, 85, 86, 91, 94, 95, 96, 99, Ill, 114, 141, 142, 147, 148, 151, 152, 153, 156, 175, 176, 177, 178, 179, 180 Warburton, B. 18, 174 Waterhouse, W.M. 64, 148, 176 Whitcomb. P.J. 19, 176 White, J.L. 101, 104, 146, 148, 154, 155, 173, 177 Whorlow. R.W. 9, 51, 53, 67, 110, 177 Willey, S.J. 134. 176 Williams, G.E. 131, 176 Williams, P.R. 80, 85, 86, 89, 178, 179 Williams, R.W. 86, 99, 176, 178
184
Winter, H.H. 76, 86, 176, 178 Woodcock, L.V. 118, 137, 138, 178, 179 Yuan, TF. 125, 176 Zapas, L. 155, 173 Zebrowski, RE. 89, 179 Zimm, RH. 107, 172
185
SUBJECT INDEX (N urnbers in italics refer to entries m the
Glossary
Le. pp 159  169 )
AblUpt contractions, flow into, 10, 88 Absotption of suspending phase, 127 Accuracy of measurement in rheometers, 59 Activation energy, 132 Adsorbed molecules, 104, 117, 118, 133, 136, 137 Aggregates of particles, 116, 117 Air, viscosity of, 11 Amplitude ratio, 53 Anisotropy, flow induced, 56 Antimisting polymer, 23 Antithixotropy, 99, 142, 159, 163, 165 Apparent viscosity, 159, 166 Application of creams and lotions, 13 Argon, 137 Arrhenius relationship, 13 Asphalt, 1 Asymmetric particles, suspensions of, 124 Atmospheric pressure, 67 (see isotropic pressure) Atomisation, shear rate during, 13 Attraction between the particles, 116 Automotive oil grade number, 113 Bagley correction, 33, 87 Ballpoint pen ink powerlaw parameters, 22 Balloon inflation, 76 (see biaxial flow) Beadspring (necklace) model, 106, 107 Bentonite (Supergel) clay, 118, 133 Biaxial extensional flow, 76, 86 Bicycle oil viscosity, 11 Bifurcation, 157 Binary particlesize fraction, 122 Binding analysis orifice flow for, 88
Bingham equation, 20 model, 20, 21, 133, 159 plastic, 16, 17 plot, 20 Biological materials, rheology of, 159 Biorheology, 3, 159 Biotechnology, 3 Bitumen, viscosity of, 11 Block copolymers, 137 Blood viscosity, 19, 115, 135 Blood flow, shear rate during. 13 Blow moulding, 112 Body.centred cubic packing, 120 Boger fluid, description of, 59, 100 Boltzmann's principle, 38, 45 Bouncing putty, S Boundary conditions, 141
B.P. (Hyvis 07), 61 (Hyvis 30), 59 (see polyisobutylene) Bridging flocculation, 137 British Society of Rheology, 1 Brookfield viscometer, 26 Brownian (thermal) randomising force, 116, 117, 119 BlUshing, shear rate during, 13 Bueche treatment, 107 Burgers model, 43 Calcium carbonate blends, 131 Calendering importance of extensional flow, 79 Calibration of viscometers, 25 Canonical forms constitutive equation of, 154 mechanical models of, 43, 44
186
Capillary flow, 14 rheometer. 87 viscometer. 32 online version l 35 Omstatter, 18 Carbon black, polymer melts in, 104 Carbopol solution Sisko model use of, 22 Carreau model, 18 CauchyGreen tensor, 147. 148 Cement. 115 Chain branching influence of, 104 prevention of crystallisation by. 102 Chain rigidity, influence of, 104 Characteristic time, 161, 169 Characteristic time of lubricating oils. 5 Maxwell model. 48 polymer melts. 6 water, 5 Chemical cross linking, 97 Chemical process industries, 1 Chewing, shear rate during, 13 Chlorine, 137 Chocolate, molten power law parameters of, 22 Circular Couette flow, 65, 7l. 168 Classification of rheological behaviour, 5 Clay and soap suspensions, 119 Clay particles. edge/face attraction, 116 Clay slurries, (deflocculated), 23 Clays. 131 Coaxial cylinders, 160 Coal slurries, 115 Coating dip, 13 drainage during, 13 high speed, 13 Codeformational derivative, 146 Coefficient of viscosity, 161 Coiled chain, polymer structure, 25 Coleman and Noll theory, 148 Colloidal contribution to viscosity, 116, 131 forces, 117 interactions temperature sensitivity of, 25 liquids highly elastic, viscoelasticity in, 25 inelastic, thixotropy in, 24
extensional viscosity of, 95 Complex compliance, 49, 159, 163 modulus, 46, 50, 51, 160, 161 viscosity, 48, 160 Complex flow problems, solution of, 156 Compliance, 160 complex, 159 loss, 159 shear, 159 storage, 159 Computational fluid dynamics, 9 Computer modelling, 121 Computer simulation suspension rheology of, 137, 138, 139 Concentrated suspensions, 115, 119 Concentric cylinder rheometer, 52 Taylor vortices in, 29 viscometer. 14 narrowgap, 27 online, 35 widegap, 28 Coneandplate errors, 67 rheometer. 52, 65 viscometer, 14, 30 FerrantiShirley, 18 nonnal stress measurement. 65 Confectionery, 13 Consistency, definition and units of, 19, 160 Constant strain relaxation tests, 51 Constant stress creep tests, 51 extensional viscosity from, 84 rheometer, 52 Deer, 27 viscometer, 17 Constitutive equations, 9. 10. 80, 107, 109, 141, 143, 149, 150, 152, 155, 156, 160, 161, 165 canonical fonn of. 154 differential, 145 integral, 151 isotropic pressure in, 8 slow flow, 56 Constitutive model, 153, 156 theory, 149 Contact adhesives, 3 Continuity, equation of, 141
187
Continuous phase viscosity, 123, 126 role in suspensions, 25 Continuum rheology, 160 mechanics, 6, 7, 10, 56, 80, 141, 142, 145, 154 Contraction flow, 10, 77, 87, 88 extensional viscosity from, 98 Contravariant metric tensor, 146 suffices, 143 Contraves viscometer, 27 Controlled strain experiment extensional viscosity from, 82 Coordinate system convected, 144, 145, 146 fixed laboratory, 146 Corotational Oldroyd model, 154, 155 Couette circular, 160, 168 flow, 152 plane, 160 CoxMen. rule, 72, 73, 98, 99, 111 Creaming, 127, 137, 160 Creams, application of, 13 Creep tests, 18, 51, 160 Critical shear rate, 128 Cross model, 18, 19, 20 Crosslinks, 108 Crowding effect, 121 Crude oil reservoir, 113 CfAsaL, 23 (see surfactant solution) D1 polymer solution, 72 D3 polymer solution, 73 Dashpot, 40, 42, 155, 160 Deborah number, 5, 6, 161 Deflocculated suspensions, 23, 116 Deformation history, 145, 161 Depletion flocculation, 137 Detergents, v, 25 Di(2~ethylhexyl)sebacate, 15 Die swell, 62, 63, 161 negative, liquid crystals in, 105 Differential constitutive equation, 144, 145, 153, 155, 156 Digital computers, 156 Dilatancy, 16, 161 Dilute emulsions, 42 polymer solutions, 75, 99
suspensions, 120 solid elastic spheres, 42 Dip coating, 13 Disc impellers, 63 Dispersed phase concentration, 123 Dispersion stabilisers, 137 Displacement fluid, 114 Displacement functions, 144 Distribution function relaxation times of, 45 DoiEdwards model/theory, 109, 156 DoiEdwardsde Gennes tube concept, 109 Double~layer thickness, 132 Drag reduction in turbulent flow, 79 Drainage toilet bleaches, 13 coating, 13 painting, 13 Drilling fluids, viscosity, 15, 115 Droplet breakup, 135 stretching extensional viscosity from, 89 Dumbell model, 107 Dynamic viscosity, 38, 48, 53, 160, 161, 162 CoxMen. rule in, 99 Dynamic rigidity, 47, 48, 53, 71, 72, 134, 161 CoxMerz rule in, 99 Edge effects in rheometry, 65, 68 Edge/face attraction, clay particles, 116 Effective phase volume, 133 Einstein's equation, 119, 136 Elastic effects, 134 liquid mixing in, 63 energy, 161, 167 liquids, 3, 6, 161 complex flows of, 9, 10, 156 modulus, 105, 161 recovery, 106 shear strain, 166 solid, 159, 163 Elasticity modulus, 45 Elasti~vi8COUS, 6, 161 Electrostatic effects, 116118, 131, 132 Ellis model, 126 Elongational viscosity, 161, 162 (see extensional viscosity)
188
Eknulsions, 16, 75, 115, 135, 136, 152 dilute, 42 droplets in, 56 manufacture, 136 stabilisers, 137 silicone oil in water, 135 wideparticlesize, 136 End effects in viscometers, 28 Energy dissipation, rate of, 14 Engineering applications use of Bingham model, 21 Enhanced oil recovery (EOR), 78, 113 Entanglements, 98, 103, 108 (see intermolecular associations) Entrance correction extensional viscosity, 33 Entropic repulsion, 116, 137 forces, 132 polymeric systems, 56 springs, 106 Equation of continuity, 141 of state (rheological), 148, 160, 161 Etymology of rheology, 1 Eulerian, 145 steadiness, 54, 85 Everyday timescale, 4 Exit effects in pipeflow, 33 Exitpressure measurement technique, 70 Extensional flow, 9, 114, 129, 153, 161, 168 biaxial, 76, 86 planar, 77 steady, 168 strain, 162 strain rate, 75, 162 uniaxial, 16 Extensional viscosity, 75, 112, 114, 155, 161, 162, 168 biaxial, 77 planar, 77 uniaxial, 75 (see elongational viscosity) Extensional viscosity from constant stress devices, 84 contraction flow, 98 controlled strain rate experiment, 82 controlled stress experiment, 82 dropletstretching, 89 fibre spinning, 84, 85 homogeneous stretching method, 83
opensyphon method, 89 opposingjet techniques, 89 radial fIlament elongation, 89 stagnationpoint devices, 89 triplejet technique, 89 Extensional viscosity of IIDPE, 90 nJPAC A LOPE, 91 LOPE, 90 Phan Thien and Tanner model, 81 polyacrylamide, 95 1175 grade, 92 ElO grade, 93 polyethylene oxide WSR 301 grade, 95 polystyrene, 90 suspensions of slender particles, 82 xanthan gum, 93 Extra stress tensor, 143, 162 Extraction of oil, 113 Extrusion, 13, 63, 112, 113 shear rates in, 13 Fabric conditioner powerlaw parameters of, 22 Sisko model use of, 22 Facecentred cubic packing of particles, 120, 132 Fading memory, 151 Fallingball viscometer, 26 Fanis effect, 122 FENEdumbell model, 108 FerrantiShirley viscometer, 27 Fibre spinning, 153 and extensional viscosity, 77, 84, 85 fIlamentnecking imperfection in, 78 Fibres, 112 Film blowing, 112 Finger tensor, 148 First normal stress difference, 55, 57, 59, 98, 99, 107, 111, 155 First (lower) Newtonian region, 16, 99, 115 Flamethrowers, 3 Flocculation, 116, 119, 121, 137 bridging, 137 depletion, 137 Floes, 117, 121, 133, 137 Flow birefringence, 9, 65, 162 classification, 156 curve, the, 162 induced anisotropy, 56
189
induced structures, 119, 138 through contractions, 10, 112 Fluid mechanics Newtonian, 3 nonNewtonian, 141, 149, 151 Fluid memory, 142, 143 Flushmounted transducers, 65, 68, 70, 71 Foodstuffs, 3, 115 Forced oscillation testing, 53 Fordcup viscometer, 26 Fonnulation principles, 142, 144 Fourroll mill, 96 Fracturing of polymers, 101 Frame indifference, 143 Free oscillation/vibration testing, 53 Free volume, 101 Functional analysis, 7, 148 Gap setting errors in viscometers, 31 Gap width, importance of, 14 Gasoline engines, lubrication in, 13 Gc rule, use of, 98 Gear teeth, flow between, 5 Gelatine, 104 Gels, yield stress in, 17, 105 General integral representation, 46, 48 Generalised Kelvin model, 43 Maxwell model, 43 Newtonian model, 149 Giesekus model, 155 GiesekusBird theories, 107, 108 Glass plate and rod suspensions, 125 processing of, 13 viscosity of, 11 Glassfibre suspensions, 124, 125 Glass forming polymers, 101 Glass transition and free volume, 101 and latentheat, 101 in liquidstate theories, 101 polymers in, 101 temperature of high density polyethylene, 101 low density polyethylene, 101 nylon66, 101 polyethylene terephthalate, 101 polystyrene, 101 Glycerine, 2 (see also glycerol)
Glycerol, viscosity of, 11 Golden syrup, viscosity of, 11 Greases, 12, 20, 128 GreenRivlin fluids, 150 GroWld gypsum suspensions, 125 Gum arabic, 137 Haake viscometer, 18 Hagenbach and Couette formula, 33 lIDPE, extensional viscosity of, 90 (see highdensity polyethylene) Heatsensitive polymers, 112 Heattransfer pipeflow in, 34 viscometers in, 14 Hencky strain defInition of, 82 largest used, 83 Hierarchy equations, 56, 151 model, 156 High Weissenbergnumber problem, 156 High density polyethylene glass transition temperature of, 101 melt路processing temperature of, 101 melting point of, 101 Holepressure error, 33, 68, 70 Homogeneous stretching method for extensional viscosity, 83 Hooke model, 40, 162 Hooke's law, 3, 162 Hookean elastic response, 2, 3, 5, 6, 37, 39, 52 Hoop stress in rodclimbing, 60 HPBL equations, 71 Hydrodynamic forces, 116 lubrication, 113 resistance, 137 Ice cream, yield stress in, 17 Independent.alignment assumption, 109, 156 Indicial notation, 7 Industrial process modelling, 9 Industrial shop floor viscometers, 26 Inelastic nonNewtonian fluids, 24, 114, 149 defInition of, 55 Inert fillers, 137 Inertia in rheometry, 51
190
Inertia (cont) in pipe路flow, 33 Injection moulding, 112 Integral equations, 143, 151, 155 expansions, 152 formulation, 152 Interfacial effects, 42, 113 Internal friction, 2 Intramolecular forces and viscoelastic phenomena, 106 Intrinsic viscosity, 103, 104, 121, 123, 162 Isotropic pressure, 143, 162 constitutive equations in, 8 nJPAC A LDPE sample, 82 extensional viscosity of, 91 Jeffreys model, 42, 43, 152 Jetthrust technique, 63, 70 JohnsonSegalman model, 108, 154 Journal bearings, 113 Judges, Book of, 5
Kaolin in medicines, 114 KBKZ model, 109, 155 Kelvin model, 39, 40, 41, 43, 44, 162, 165 Kernel functions, 152 Kinematic viscosity, 161, 162 Kinetic theories, 106108 Krieger variable, 126 KriegerDougherty equation, 125, 132 Kronecker delta, 143 Lagrangian steadiness, 54 Laterite suspensions, 125 Latices, 125, 126, 130 LOPE, extensional viscosity of, 90 (see lowdensity polyethylene) Lennard路Jones interactions, 137 Leonov model, 154, 155 Levelling effects, 13 Light diffraction, 119 Linear stability analyses, 156 viscoelastic behaviour, 4, 37, 46, 49, 107 static and dynamic, 51 viscoelasticity, 50, 143, 163 general differential equation, 38, 47, 144
Liquid defmition of, 6 Newtonian, 5 Liquid A, 151 Liquid B, 155 Liquid abrasive cleaners, 114, 115 Liquid crystal polymers, 22, 56, 105 ~ Liquid detergents, 3 Liquidlike behaviour, 6 material, 52 solids, 4 Liquidstate theories, 101 Lodge rubberlike liquid, 108, 155 stressmeter, 70 viscometer version of, 35 Londonvan der Waals attraction, 116 Loss angle, 49, 163 compliance, 163 modulus, 47, 163 Lotions, application of, 13 Low density polyethylene glass transition temperature of, 101 meltprocessing temperature of, 101 melting point of, 101 Lower Newtonian region, 16 Lubricants, 1 highshear rate viscosity, 38 viscosity I pressure dependence of, 15 Lubricateddie rheometer, 86 Lubricating grease, 118 yield stress in, 17 Lubricating oils, 6 characteristic time of, 5 temperature dependence of, 14 Lubrication, 113 approximation, 112 high temperature, 25 shear rate during, 13 Macrorheology, 160, 163 Margarine, yield stress in, 17 Master curves, 111 Maximum packing fraction or phase volume, 120, 121, 123 Maxwell model, 39, 41, 42, 47, 144, ISS, 163, 165 characteristic natural time, 48 generalised, 43 oscillatory shear behaviour, 49
191
upperconvected, 107, 154 Maxwell orthogonal rheometer, 54 Maxwell's elastic fluid, 3 Measurement accuracy rheometry in, 68 viscometry in, 13 Mechanical models, 40, 162 canonical forms of, 43, 44 Medicines, 13, 115 Melt flow instabilities, 113 fracture, 113, 163 Meltprocessing temperature of high density polyethylene, 101 low density polyethylene, 101 nylon路66, 101 polyethylene terephthalate, 101 polystyrene, 101 Melting point of high density polyethylene, 101 low density polyethylene, 101 nylon66, 101 polyethylene terephthalate, 101 Memory fluid, 6, 161, 163 Method of reduced variables, 109 Microrheology, 163 Microstructure, 141 Milling of pigments, 13 Minimum.energy state, molecules in, 106 Mixing, shear rate during, 13, 112 Modulus, 163 complex, 160, 161 loss, 160 rigidity, 166 shear, 160 storage, 160 Molecular adsorption, 137 models and extensional flow, 81 structure, 10 theories, 106 Molecular weight distribution, 25, 63 influence of, 104 viscosity relationship polybutadiene, 102 polydimethylsiloxane, 102 polymethyhnethacrylate, 102 polystyrene, 102 Mooney system viscometers based on, 28 Motions
with constant stretch history, 152 Multigrade oils, 3, 25, 71, 113 Naphthenic mineral oil, 15 Narrowgap approximation, 29 Natural gums, 114 NavierStokes equations, 2, 3, 6, 163, 164 Nearly viscometric flows, 152 Necking, 163 Necklace model, 106, 107 Negative die swell and nonnal stress difference, 105 Negative nonnal stress effect inertial origin of, 67 Negative thixotropy, 24, 159, 163 (see also antithixotropy) NEMD calculation, 138, 139 Network models, 108 Newtonian behaviour, 2, 3, 5, 6, 8, 11, 15, 65 dashpot, 40, 155 equations, 137 fluid mechanics, 3 model, 164 generalised, 149, 156 standardised liquids, 25 Noslip hypothesis, 151 NonNewtonian, 6, 16 flow, 156 fluid mechanics, 141, 149, 151 fluids, 164, 169 Non路drip paint, 3, 4 Non.equilibrium molecular dynamics (NEMD), 137 Non路linear viscoelasticity, 37 Non路linear crosssection pipe flow, 64 Nonlinearity, importance of, 4 Nonsettling suspensions, 20 Nonnal force, 164 measurement using coneandplate flow, 65 flushmounted transducers, 65 pump, 62 Normal stress difference, 8, 9, 15, 55, 113, 138, 141, 149, 150, 153, 164, 167, 169 coefficients, 55, 108, 169 fll'St, 55, 56, 57, 59, 98, 99, 107, 108 negative, 105 second, 55, 56, 57, 59, 70, 107 thennodynamic origin, 57
192
Nonnal stress distribution, 149 tension along streamlines equivalence, 59 Nonnal stress effects in mixing, 63 Nonnalised frequency, 48 (see reduced frequency) Numerical simulation, 10, 147, 156, 157 Nylon66 glass transition temperature of, 101 meltprocessing temperature of, 101 melting point of, 101 Optical anisotropy, 162 Oil bicycle, viscosity of, 11 lubricating temperature dependence of, 12 multigrade, 25, 71 olive, viscosity of, 11 Oldroyd models, 107, 152, 154, 155 Online viscometers, 35 Onset of shearthickening, 130 melt flow instabilities, 113 Open tilted trough technique, 71 Opensyphon effect with polyethylene oxide, 94, 95 Opensyphon method extensional viscosity from, 89 Oppanol (B50), 58 (B200), 60, 61, 72 (see polyisobutylene) Opposingjet techniques extensional viscosity from, 89 Optical diffraction system, 128 Orientation vector, liquid crystals m, 105 Orifice flow, 77, 87 Binding analysis for, 88 Oscillatory shear, 47, 153 high frequency measurements, 103 Maxwell model, 49 Rheogoniometer for, 52 small amplitude, 9, 46, 71, 107 Osmotic pressure, 138, 139 Overshoot, 164 Packing fraction, maximum, 135 Painting drainage during, 13 shear rate during, 13 Paints, v, I, 13, 13, 114, 115, 133
Paper coating importance of extensional flow in, 79 shear rate during, 13 Parallel sliding plate rheometer, 65 Parallelplate viscometer, 31 Particle asymmetry, 123 density, 116 hydrodynamic redistribution, 128 layers, 119 migration, 128 overall attraction between, 133 polyhedral, 135 shape, 120 size, 136 surfaces, polymer adsorbed onto, 132 Particlefilled polymer gel, 105 Particleparticle interaction, 137 Particlesize distribution, 120, 121, 128, 131 Pastes, yield stress in, 17 Peclet number (modified), 126 Pennanent crosslinks, 108 Perturbation analyses, 156 parameter, 156 Phan Thien and Tanner model, 154, 155 extensional viscosity of, 81 Pharmaceutical industry, 3 Phase separation, 127 Phase changes detergent based liquids, 25 Phase lag, 53 Phase volume, 116 effect of, 127 effective, 133 maximum, 135 (see packing fraction) Phenomenological rheology, 160 Photodegradation antimisting polymer of, 23 Physical chemistry, 6 Pigment dispersion, 117 milling of, 13 Pipe flow entrance effects in, 33 exit effects in, 33 heattransfer in, 34 inertial losses in, 33 laminar, Newtonian, 32 nonlinear crosssection pipe, 64
193
powerlaw liquids, flow in, 32, 34 Rabinowitsch correction, 32 scaleup of, 33 shear rate during, 13 shearstress in, 32 thixotropic material in, 25 velocity profile in, 34 viscous IOlses in, 33 Plane Couette flow, 65, 160 Plastic behaviour, 166 deformation, 169 viscosity, 164 Plastic(ity), 164 Plasticrigid solid, 5 Plastics, v, 1 Plasticsprocessing industry, 3 Plastometer, 18 Poiseuille equation, 32 flow, 70, 87, 152, 164 Polarisability, 116 Polarity influence of in, 104 Polypbenzamide, 105 Polyacrylamide, 62, 114, 114, 137 1175 grade, 94 aqueous !IOlution viscosity, 19 ElO grade, 57, 94 extensional viscosity of, 92, 93, 95 maltose syrup/water base, 100 (see Boger fluid) tension thickening, 96 Polybutadiene in dekalin, 91 moL weight/viscosity relationship, 102 Polybutene in polyisobutylene, 61 Polydimethylsiloxane, 102 Polydispersity, influence of, 122 Polyethylene oxide opensyphon effect with, 94 extensional viscosity of WSR 301 grade, 95 Polyethylene terephthalate glass transition temperature of, 10 1 meltprocessing temperature of, 101 melting point of, 101 Polyhedral particles, 135 Polyisobutylene in dekalin, 58, 60, 72 kerosenelpolybutene, 59, 100 polybutene, 61
Polymer blends influence on viscosity, 104 Polymer extrudate, 163 Polymer flooding, 78, 114 (see enhanced oil recovery) Polymer gels, 104 Polymer liquid crystal Sisko model use of, 22 Polymer melts, 57, 68, 97 carbon black in, 104 characteristic time of, 6 handling of, 13 powerlaw parameters of, 22 viscosity of, 11 Polymer processing, 6, 111 importance of extensional flow in, 77 Polymer rheology, 1 effect of molecular weight on, 102 effect of temperature on, 101 from molecular theories, 106 Polymer solutions, 16, 57, 97, 155 dilute, 75 Polymer structure (coiled chains), 25 Polymeric liquid crystals, 104 Polymers adsorbed onto particle surfaces, 132 as thickeners, 136 crystallisation and freezing, 101 engine lubricants, 113 extrusion of, 13 fracturing, 101 glass forming, 10 1 liquid crystal formation, 105 solubility of, 25 Polymethylmethacrylate (PMMA), 102 Polypropylene copolymer, 57 isotactic glass transition temperature of, 101 melting point of, 101 meltprocessing temperature of, 101 Polysaccharidetype polymers, 114 Polystyrene, 90 a noncrystallising polymer, 101 benzene, 104 extensional viscosity of, 90 glass transition temperature of, 101 meltprocessing temperature of, 101 modes of motion in chains of, 103 moL weight/viscosity relationship, 102 Pores of sedimentary rock, 113 Positive dissipation principle, 145
194
Postextrusion swelling. 62. 161 (see die swell) Powders, sedimentation in liquids. 13 Powerlaw index. 129 definition of, 19 liquids in pipeflow, 324 model, 19, 20, 21, 23, 28, 58, 112,
164 shearthinning region, 115 Powerlaw parameters of ballpoint pen ink, 22 fabric conditioner, 22 polymer melts, 22 synovial fluid, 22 Pressure concept of, 7 dependence of viscosity on, 14 measurement with flushmounted transducers, 68 Prevention of crystallisation by chain branching, 102 rapid cooling, 102 Principle of fading memory, 145 material objectivity, 143 Printing inks, v, 13. 115, 133 Process control, 9 modelling, 112 time, 161 Processing of glass, 13 PS.â€˘ 90 extensional viscosity of, 90 (see polystyrene) Pseudocrystal/lattice. 117 Pseudoplasticity, 16. 164 (see shear thinning) Pumping, shear rate during. 13 Pure shear, 77 (see planar extensional flow) Putty. bouncing. 5 PVC organosol, 134 Quality control, 9 use of viscoelastic parameters in. 37 Quartz grain suspensions, 125 QWERTY keyboard, 5 Rabinowitsch conection. pipeflow in, 32 Racemic poly"(benzyl glutamate. 22 Radial distribution nmction. 125 Radial filament elongation
extensional viscosity from, 89 Random close packing, 120 disordered state, 117 Rapid cooling prevention of crystallisation by, 102 Rate of energy dissipation, 14 Rateofshear, 165 Rateofstrain tensor, 143 Recoverable shear, 58 Reduced shear rate, 111 variables method, 109 viscosity, 162, 165 Reentrant comers, 151. 157 ReinerRivlin fluid, 55. 149 Relative defonnation, 165 viscosity, 125, 165, 169 Relaxation function, 45, 50, 51 spectrum, 43, 45, 50, 51 tests at constant strain, 51 time, 41, 45, 51, 52. 109, 161. 165,
169 Reptation (models), 108. 109 Repulsion, 116, 131 entropic, 137 Rest structures in suspensions, 117 Retardation time. 40, 154. 165 Retardedmotion expansion. 151 Reynolds number, 165 Rheogoniometer, 98. 165 oscillatory methods. 52 Weissenberg, 59 Rheograms. 165 Rheological behaviour, classification of. 5 Rheological equations of state. 10, 141, 48, 160, 165 formulation of. 144 Rheology. 113. 165 continuum. 160 defmition, v etymology. 1 mathematical description of, 5 phenomenological. 160 suspensions, 115 theoretical, 141 timescale in, 5 Rheometer. 165 accuracy of measurement. 59 capillary. 87
195
concentric cylinder, 52 coneandplate, 52, 65 constant stress, 27, 52 lubricatedconvergingflow, 86 lubricateddie, 86 Maxwell orthogonal, 54 parallel sliding plate, 65 Rheometries, 27 spinline, 85, 98 torsional balance, 32 Weissenberg, 27 Rheometry, 9 edge effects in, 68 inertia in, 51 measurement accuracy in, 68 role of, 9 speed of sound in, 51 surface tension in, 68 Rheopexy, 159, 165 Ribbons, 119 Rigidity modulus, 2, 4, 38, 166 Risingbubble viscometer, 26 RivlinEricksen fluid, 150 tensors, 148, 150 Rodclimbing effect, 60, 67 Rods, suspensions of, 112, 124 Rollwave motion in turbulent flow, 79 Rotameter used as a viscometer, 35 Rotating bodies, flow caused by, 156 Rotational viscometers, 26 RouseZimm model, 106, 107 Rubber vulcanisation, 98 Rubbing, shear rate during, 13 Sample changing in viscometers, 31 Scaleup of pipeflow, 33 Second normal stress difference, 5559, 70, 155 coefficient, 108 Second (upper) Newtonian regIon, 16, 99 Second order model, 151, 154 extensional viscosity from, 81 simple fluid version, 71 viscoelasticity from, 152 Secondary flow, 31, 166, 168 mistaken for shearthickening, 31 Secondary recovery process, 113 Sedimentation of powders, 13, 127, 137 Selfdiffusion, 132 Semicrystalline solid polymers shear modulus of, 101
Semirigid polymer extensional viscosity of, 98 Separation processes, 137 Servomechanism for gapmaintenance, 67 Sharkskin, 113 Shear, 166 compliance, 159, 166 definition, 2 fracture, 68 modulus, 50, 160, 166 of metals, 101 of solid polymers, 101 of unhardened rubber, 101 oscillatory, 153 simple, 153, 155, 160 smallamplitude oscillatory, 151 strain, 166 stress, 166 in pipeflow, 32 viscosity, 159, 166 Shear rate, 166 critical, 128 definition, 2 Shear rate during atomisation, 13 blood flow, 13 brushing, 13 chewing, 13 extmsion, 13 lubrication, 13 mixing, 13 painting, 13 paper coating, 13 pipe flow, 13 pumping, 13 rubbing, 13 spraying, 13 stirring, 13 swallowing, 13 Shear thinning, 4, 16, 119, 164, 166 Shear thickening, 16, 23, 128, 129, 130, 131, 138, 161, 166 dilute polymer solutions in, 99 heattransfer in pipeflow, 34 onset of, 130 region, 129 secondary flow mistaken as, 31 surfactant solution for, 23 Shift factors, 110, 111 SI units, viscosity, 2, 12 Silica dispersions, 117
196
Silicone, 5 Simple cubic packing, 120 fluids, 148, 151 hypothesis, 150 rheometrical flows, 141, 152  shear, 160, 166 Sisko model, 19, 20, 22 carbopol solution for, 22 fabric softener for, 22 polymer liquid crystal for, 22 yogurt for, 22 Slit flow, 14, 35, 70 Slow flow, 45, 56, 71, 150, 156 Slowly varying, 151 Slumping of grease, 20 Small.amplitude oscillatory flow, 9, 46, 71, 99, 107, 134, 151 Smoothness assumptions, 151 Soap crystals, 118 Soft solids, 105, 166 Solid defmition of, 6 elastic, 159 Hookean elastic, 5 plasticrigid, 5 Solidparticle dispersions, 135 Solidlike behaviour, 6 liquids, 4 materials specimen preparation, 52 testing of, 53 Solids, 4 Hookean elastic, 3 liquidlike, 4 Solubility of polymers, 25 Solvent/polymer interactions, 104 SPeCific viscosity, 165, 167 SPeCimen p:eparation of solidlike materials, 52 SPeCtrum of relaxation frequencies, 45 Speed of sound in rheometry, 51 Spheres, 124, 125 Spin.line technique (rheometer), 85, 86, 9194, 98 Spinnability, 77, 167 Spinning, 112 Spraying, shear rate during, 13 Spring.dashpot models, 42 canonical forms of, 44 Springs in mechanical models m, 40
Squeeze film flow, lubricated, 76 (see biaxial flow) Stabilisers for dispersions, 137 emulsions, 137 Stability analyses (linear), 156 Stagnation路point devices extensional viscosity from, 89 Standardised liquids (Newtonian), 25 Starch suspensions, 129 Startup of shear flow, 108 Statistical mechanics, 6 Steadiness Eulerian definition of, 54 Lagrangian definition of, 54 Steady flow, 167 Eulerian, 85 extensional, 168 shear, 149, 150, 153, 155, 169 Steel (modulus), 5 Steric repulsion, 117 Stirring, shear rate during, 13 Stokes' drag law, 20 equation, 106 Stone路Weierstrass theorem, 150 Storage compliance, 159, 167 modulus, 47, 160, 167 Stored energy, 167 Strain definition of, 2, 167 energy, 161, 167 hardening, 89 Stress relaxation, 167 overshoot at startup of shear flow, 108 tensor, 138, 152, 162, 165, 167 extra, 143 trace of the, 139 Stretching of thin sheets, 76 (see biaxial flow) String.ofpearls structure, 117 Stringiness, 114 Strings of molecules, 139 Structural engineering, 5 Suction device, spin路line technique in, 86 Superposition principle, 38, 45 (see Boltzmann's principle) Surface tension rheometry in, 68
197
and levelling, 13 Surfactant solution shearthickening behaviour, 23 Suspensions, 75 asymmetric particles, 124 fine particles, 114 flocculated, 133 nonsettling, 20 slender particles (extensional viscosity), 82 solid elastic spheres of, 42 starch, 129 submicron, 126 truncated cones for, 31 very dilute, 152 viscometers for, 28 viscosity of, 17, 116 Swallowing, shear rate during, 13 Swelling, postextrusion, 161 (see die swell) Symmetric contravariant tensor, 146 covariant tensor, 146 Synovial fluid powerlaw parameters of, 22 Synthetic latex, Bingham plot of, 20, 21 Syntheticfibre industry, 3 Taylor number, 168 vortices, 168 in concentriccylinders 29 Taylorseries expansion, 150 Temperature dependence of viscosity, 4, 12 lubricating oils, 14 colloid interactions, 25 Temporary viscosity loss, 16 Tension, 168 along streamlines, 59 thickening, 7678, 81, 91, 94, 168 thinning, 76, 77, 78, 91, 93, 94, 168 Tensor, 38, 146 analysis, 7, 143 valued functional, 148 Tertiary mixtures, 122 Tertiary or enhanced oil recovery (EOR), 114 Theology, misprint for rheology, 5 Theoretical rheology, 141 Thermodynamic equilibrium, 117
ongm of normal stresses, 57 principles, 145 Thickening sauces and soups, 114, 136 Thixotropic material in pipe flow, 25 Thixotropy, 4, 24, 25, 142, 168 negative, 159 Timedependent frame, 143 materials, 142 Timescale everyday, 4 rheology, 5 Timetemperature superposition, 109, 110, 168 Titanium dioxide, 125 Toilet bleach, drainage, 13 Toothpastes, 4, 114, 137 Torsional balance rheometer, 32 flow, 31, 65, 68 (see parallel plate geometry) Trace of the stress tensor, 139 Transformation rules, 146 Transient junctions, 108 Tribology, 38 Trimodal suspensions, 123 Triplejet technique for extensional viscosity, 89 Trouton behaviour, 89 ratio, 80, 81, 94, 95, 99, 100, 168 viscosity, 168 Truncated cones for suspensions, 31 Turbulence, 162, 168 drag reduction in, 79 rollwave motion in, 79 viscometers in, 29 vortex stretching in, 79 Twodimen sional layering, 128, 132 structures, 125 Twophase liquids temperature effects, 25 Uniaxial extensional flow, Unvulcanized rubber, 110 Upper Newtonian plateau, (see second Newtonian Upperconvected Maxwell
16 16, 99, 115 region) model, 107,
154 Van der Waals attraction, 117 Variant suffices, 143
198
Velocity gradient, 168 profile in pipeflow, 34 Very high frequency measurements, 103 Viscoelastic(ity), 37, 46, 51, 107, 113, 136, 149, 161, 163 defmition of, 6 due to intramolecular forces, 106 linear, 4, 46, 50, 51, 55, 107, 152 secondorder, 152 Viscometers, 169 Brookfield, 26 calibration, 25 capillary, 32 Omstatter type, 18 concentric cylinder, 14 narrowgap, 27 online version of, 35 widegap, 28 coneandplate, 14, 30 FerrantiShirley, 18 constant stress, 17 Deer type, 18 Contraves, 27 convenience, 26 defmition of, 12 end effects, 28 fallingball, Glen Creston, 26 FerrantiShirley, 27 for suspensions, 28 Fordcup, 26 gap setting errors, 31 Haake, 18 heat transfer in, 14 industrial shop floor, 26 Lodge stressmeter used as, 35 Mooney system, 28 online, 35 parallelplate, 31 risingbubble, 26 robustness, 26 rotameters used as, 35 rotational, 26 sample changing in, 31 secondary flows in, 31 slit, 35 torsional parallelplate, 31 turbulence in, 29 viscous heating in, 29 Viscometric flows, 152, 169 Viscosity, 169 apparent, 159, 166
coefficient of, 161 colloidal contribution to, 131 complex, 48, 72 dynamic, 38, 48, 53, 71, 160 CoxMea rule use in, 99 elongational, 162 (see extensional viscosity) extensional, 161 biaxial, 77 planar, 77 uniaxial, 75 International standard of, 25 intrinsic, 103 kinematic, 161 measuring accuracy of, 13 pressure dependence of, 14 ratio, 165, 169 reduced, 162 relative, 169 shear, 11 SI units, 12 specific, 165 temperature dependence of, 12 Trouton, 162 Viscosity of air, 11 bitumen, 11 glass, 11 glycerol, 11 golden syrup, 11 liquid honey, 11 polymer melts, 11 suspensions, 17 water, 11 ViscosityIndex (or VI) improvers, 113 Viscous heating in viscometers, 14, 29, 38, 68 losses in pipe flow, 33 Voigt model, 39, 162, 169 (see Kelvin model) Vortex enhancement, 88 stretching in turbulent flow, 79 Vulcanisation of rubber, 98 Wall depletion effect, 127, 128 Water, 2 characteristic time of, 5 viscosity, 11 as International standard, 25 pre ssure dependence of, 14 temperature sensitivity, 25
199
Waterclarification, 137 Water/oil interface, 113 Wavepropagation methods, 53 Weather maps, 7 Weber's silk threads, 3 Weighing errors, 127 Weissenberg hypothesis, 59 nwnber, 169 definition of, 63 rheogoniometer, 27 origin of, 59 rodclimbing effect, 60, 67, 169 White路Metzner model, 154, 155 tensors, 148 WilliamsLandelFerry ~~ equation, 111 Wire coating, 64 Wobbliness, 114 Xanthan gwn, 94, 95, 114 aqueous dispersion flow curve, 19 extensional viscosity of, 93 Yield stress, 5, 16, 17, 20, 21, 115, 133, 159, 164, 169 Yield stress of gels, 17 ice cream, 17 lubricating greases, 17 margarine, 17 pastes, 17 Yogurt, Sisko model use of, 22 Young's modulus, 169 Zeroshear viscosity, 16 effect of molecular weight on, 103
an_introduction_to_rheology__barnes